physical Properties of Carbon Nanotubes
Rysical Properties of Carbon Nanotubes GDRESSELElAUS & M S DRBSELMUS MZT
Imperial College Press
Published by
Imperial College Press 203 Electrical Engineering Building Imprial College London SW7 2BT Distributed by
World Scientific Publishing Co. Pte.Ltd. P 0 Box 128, Farrer Road, Singapore912805 USA oflce: Suite lB, 1060 Main Street, River Edge, NJ 07661 WK oflce: 57 Shelton Street, Covent Garden, London WC2H 9HE!
British Library C a ~ o g ~ ~ ~Data  ~ b ~ ~ ~ o n A catalogue record for this book is available from the British Library.
PHYSICAL PROPERTIES OF CARBON NANOTWES Copyright 0 1998 by Imperial College Press All rig& reserved. This book or parts thereof. m y not be reproduced in anyform or by any means, elecironic or mechanical, including photocopying, recording or any information storage and retrieval system ROW known or fo be invented, withmf writfen~ e ~ i s s i o n ~the om Publishm
For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher.
ISBN 1860940935
This book is printed on acidfree paper.
Printed in Singapore by UtePrint
Preface
A carbon nanotube is a honeycomb lattice rolled into a cylinder. The diameter of a carbon nanotube is of nanometer size and the length of the nanotube can be more than l p m . The nanotube diameter is much smaller in size than the most advanced semiconductor devices obtained so far. Thus the availability of carbon nanotubes may have a large impact on semiconductor physics because of its very small size and the special electronic properties that are unique to carbon nanotubes. Because of the large variety of possible helical geometries known as chirality, carbon nanotubes provide a family of structures with different diameters and chiralities. One of the most significant physical properties of carbon nanotubes is their electronic structure which depends only on their geometry, and is unique to solid state physics. Specifically, the electronic structure of a singlewall carbon nanotube is either metallic or semiconducting, depending on its diameter and chirality, and does not requiring any doping. Thus we can imagine that the smallest possible semiconductor devices are likely to be based on carbon nanotubes. Further, the energy gap of semiconducting carbon nanotubes can be varied continuously from 1 eV to 0 eV, by varying the nanotube diameter. Thus, in principle, it may be possible to specify the desired semiconducting properties using only carbon atoms with a specified geometric structure. The purpose of this book is t o define the structure of carbon nanotubes as clearly as possible, starting from basic physics and chemistry. Since the uniqueness in the electronic structure comes directly from the uniqueness of the electronic structure of graphite, this volume provides background information about the structure and properties of graphite and related carbon materials. From our definition of the structure of carbon nanotubes, we can explain the electronic structure and phonon dispersion relations based on simple physical models, which the reader can follow with a pen and paper. Thus the contents of the book are rather theoretically oriented, and experimental results are used primarily t o provide evidence for the validity of the theory. This is actually the V
vi
PREFACE
way that the field of carbon nanotubes developed. At an early stage, the theory stimulated experiments in carbon nanotube physics, since obtaining sufficient quantities of pure carbon nanotubes has been difficult in practice. The early experiments were made through electron microscope observation. The direct evidence provided by electron microscopy for the existence of carbon nanotubes was sensational to many physicists and chemists, and because of this fascination, the field of carbon nanotubes has grown explosively, with many active research groups worldwide working independently or in collaborative research projects. In this book, using basic ideas of the lattice, electronic and phonon structures, the physical properties are discussed in the terminology of carbon nanotubes, which are characterized by the chiral index (n,rn). The chiral index (n, m) consists of a set of integers which specify each carbon nanotube uniquely. Since quantum effects are prominent in nanotube physics, the magnetic and transport quantum effects are very significant. Although progress in the field is still at an early stage, the book focuses on the basic principles behind the physical properties. Another unique property of a carbon nanotube is its st,iffness, corresponding to the upper limit of the best carbon fibers, which are commonly used as a strong lightweight material. The special properties of carbon nanotubes are explained in the various chapters in this book. Thus the physical properties of carbon nanotubes provide a new dimension for solid state physics, based on the great variety of possible geometries that are available for carbon nanotubes. In order to expand this field into the future, many researchers in different fields of science should contribute to this field. The authors hope that readers from any field of science can read this book without any special background requirements. This book is not intended to be a collection of all activities on carbon nanotubes worldwide because this field is already so extensive, and is moving forward so rapidly at the present time. When this book was started three years ago, the present status of the field could not have been anticipated. Thus future progress is beyond our imagination. We hope that through this book, we will find many new friends in this field. So please enjoy the book and please communicate to the authors any comments you might have about this book. The authors would like to acknowledge many carbon nanotube researchers who have contributed t o the contents of the book. The authors also thank the New Energy Development Organization (NEDO) of the Japanese Ministry for
PREFA CE
vii
International Trade and Industry (MITI), Japan Society for the Promotion of Science (JSPS), and their generous support for international collaboration which made the writing of this book possible. The authors especially thank Ms. Junko Yamamoto and Ms. Laura Doughty for their help in preparing the indexes and figures of the book. Finally the authors wish to say to readers: “Welcome to Carbon Nanotube Physics.” R. Saito, Tokyo M .S. Dresselhaus, Cambridge, Massachusetts G. Dresselhaus, Cambridge, Massachusetts
Contents
1 Carbon Materials 1 1.1 History . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.2 Hybridization in A Carbon Atom . . . . . . . . . . . . . . . . . . 4 1.2.1 sp Hybridization: Acetylene, HCECH . . . . . . . . . . . 5 1.2.2 sp2 Hybridization: Polyacetylene, (HC=CH), ...... 7 1.2.3 sp3 Hybridization: Methane, (CH4) . . . . . . . . . . . . 8 1.2.4 Carbon Is Core Orbitals . . . . . . . . . . . . . . . . . . . 9 1.2.5 Isomers of Carbon . . . . . . . . . . . . . . . . . . . . . . 11 1.2.6 Carbynes . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 1.2.7 Vapor Grown Fibers . . . . . . . . . . . . . . . . . . . . . 14 2 Tight Binding Calculation of Molecules and Solids 2.1 Tight Binding Method for a Crystalline Solid . . . . . . . . . 2.1.1 Secular Equation . . . . . . . . . . . . . . . . . . . . . . .
. .
17 17 17 21 22 25 26 29
3 Structure of a SingleWall Carbon Nanotube 3.1 Classification of carbon nanotubes . . . . . . . . . . . . . . . . . 3.2 Chiral Vector: C h . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Translational Vector: T . . . . . . . . . . . . . . . . . . . . . . . 3.4 Symmetry Vector: R . . . . . . . . . . . . . . . . . . . . . . . . . 3.5 Unit Cells and Brillouin Zones . . . . . . . . . . . . . . . . . . . . 3.6 Group Theory of Carbon Nanotubes . . . . . . . . . . . . . . . . 3.7 Experimental evidence for nanotube structure . . . . . . . . . . .
35 35 37 39 41 45 48 53
2.2 2.3
..
2.1.2 Procedure for obtaining the energy dispersion . . . . . . Electronic Structure of Polyacetylene . . . . . . . . . . . . . . . TwoDimensional Graphite . . . . . . . . . . . . . . . . . . . . . 2.3.1 x Bands of TwoDimensional Graphite . . . . . . . . . . 2.3.2 B Bands of TwoDimensional Graphite . . . . . . . . . .
ix
. .
X
CONTENTS
4 Electronic Structure of SingleWall Nanotubes 4.1 Oneelectron dispersion relations . . . . . . . . . . . . . . . . . . 4.1.1 ZoneFolding of Energy Dispersion Relations . . . . . . . 4.1.2 Energy Dispersion of Armchair and Zigzag Nanotubes . . 4.1.3 Dispersion of chiral nanotubes . . . . . . . . . . . . . . . 4.2 Density of States, Energy gap . . . . . . . . . . . . . . . . . . . . 4.3 Effects of Peierls distortion and nanotube curvature . . . . . . .
59 59 59 61 65
5 synthesis of Carbon Nanotubes 5.1 SingleWall Nanotube Synthesis . . . . . . . . . . . . . . . . . . . 5.2 Laser Vaporization Synthesis Method . . . . . . . . . . . . . . . . 5.3 Arc Method of Synthesizing Carbon Nanotubes . . . . . . . . . . 5.4 Vapor Growth and Other Synthesis Methods . . . . . . . . . . . 5.4.1 Vapor Growth Method . . . . . . . . . . . . . . . . . . . . 5.4.2 Other Synthesis Methods . . . . . . . . . . . . . . . . . . 5.5 Purification . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.6 Nanotube Opening, Wetting, Filling and Alignment . . . . . . . 5.6.1 Nanotube Opening . . . . . . . . . . . . . . . . . . . . . . 5.6.2 Nanotube Wetting . . . . . . . . . . . . . . . . . . . . . . 5.6.3 Nanotube Filling . . . . . . . . . . . . . . . . . . . . . . . 5.6.4 Alignment of Nanotubes . . . . . . . . . . . . . . . . . . . 5.7 Nanotube Doping, Intercalation, and BN/C Composites . . . . . 5.8 Temperature Regimes for Carbonization and Graphitization . . . 5.9 Growth Mechanisms . . . . . . . . . . . . . . . . . . . . . . . . .
73 73 74 77 79 80 82
6 Landau Energy Bands of Carbon Nanotubes 6.1 Free Electron in a Magnetic Field . . . . . . . . . . . . . . . . . . 6.2 Tight Binding in a Magnetic Field . . . . . . . . . . . . . . . . . 6.3 Cosine Band in a Magnetic Field . . . . . . . . . . . . . . . . . . 6.4 Landau Energy Bands . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Landau Energy Bands: AharonovBohm . . . . . . . . . . . . . . 6.6 Landau Energy Bands: QuantumOscillation . . . . . . . . . . .
95 95 98 100 104
108 111
7 Connecting Carbon Nanotubes 7.1 Net Diagrams of a Junction . . . . . . . . 7.2 The Rule for Connecting Two Nanotubes
115 115 119
............. .............
66 70
83
84 84 85 85 86 86 87 89
CONTENTS 7.3 Shape of a Junction . . . . . . . . . . . . . . 7.4 Tunneling Conductance of a Junction . . . 7.5 Coiled Carbon Nanotubes . . . . . . . . . . .
xi
...........
............ ...........
120 123 130
8 Transport Properties of Carbon Nanotubes 137 8.1 Quantum transport in a onedimensional wire . . . . . . . . . . . 137 8.1.1 A ballistic conductor ( L
bpb>
where Ci are coefficients. Using the orthonormality conditions (spa(spa) = 0, (sp,Isp,) = 1, and (SpbISpb) = 1, we obtain the relationship between the coefficients Ci : c1c3+c2c4 =
c3”+ c4”
0,
= 1,
c;+c;= c,z+c:=
1, 1.
(1.2)
The last equation is given by the fact that the sum of 12s) components in Ispa) and Ispb), is unity. The solution of (1.2) is C1 = C2 = C, = 1/./2 and C4 =  1 / d so that
In Fig. 1.3 we show a schematic view of the directed valence of the Ispa) (upper panel) and Jspb) (lower panel) orbitals. The shading denotes a positive amplitude of the wavefunction. The wavefunction of 12s) 12p,) is elongated in the positive direction of 2 , while that of (2s) (2p,) is elongated in the negative direction of x. Thus when nearestneighbor atoms are in the direction of x axis, the overlap of Ispa) with the wavefunction at x > 0 becomes large compared with the original (2p,) function, which gives rise to a higher binding energy. If we select 12py) for 12p,), the wavefunction shows a directed valence in the direction of y axis. It is only when an asymmetric shape of the wavefunction (see Fig. 1.3) is desired for forming a chemical bond that a mixing of 2p orbitals with 2s orbitals occurs. The mixing of only 2p orbitals with each other gives rise to the rotation of 2p orbitals, since the 2p,, 2p, and 2pz orbitals behave like a vector, ( 2 ,y, z ) . A wavefunction C,12p,)+Cy)2py)+C,)2pt), where C i C i + C,” = 1, is the 2p
+
+
1.2. HYBRIDIZATION IN A CARBON ATOM
yL
H
'i' I \ C /"\ C /"\ C/ I I I H
H
H
x
7
Fig. 1.4: transpolyacetylene, (HC=C€I)nl the carbon atoms form a zigzag chain with an angle of 120' , through sp2 hybridization. All u bonds shown in the figure are in the plane, and in addition, one T orbital per carbon atom exists p e r p e n d ~ c u to l ~ the plane.
wavefunction whose direction of positive amplitude is the direction (Csl C,, C z ) . The 2p wavefunctions of Eq. ( 1 . 3 ) correspond to (C,,C,,C,) = ( l , O , O ) and (C,) Cy,C,)= (1,O,O), respectively. A simple carbonbased material showing s p hybridization is acetylene, HC=CH, where 5 is used by chemists to denote a triple bond between two carbon atoms. The acetylene molecule HCzCH is a linear molecule with each atom having its equilibrium position along a single axis and with each carbon atom exhibiting s p hybridization. The hybridized Ispa) orbital of one of the carbon atoms in HCrCH forms a covalent bond with the ISPb) orbital of the other carbon atom, called a u bond. The 2p, and 2% wavefunctions of each carbon atom are perpendicular to the u bond, and the 2p, and 2p, wavefunctions form relatively weak bonds called T bonds with those of the other carbon atom. Thus, one u bond and two T bonds yields the triple bond of HCzCH. 1.2.2 sp2 Hybr2~z~ation: F o ~ y a c e ~ y ~(HC=CH)n e~e,
In sp2 hybridization, the 2s orbital and two 2p orbitals, for example 2p, and 2 q , are hybridized. An example of sp2 hybridization is polyacetylene, (HC=CH)as is shown in Fig.l.4, where carbon atoms form a zigzag chain with an angle of 120O. All u bonds shown in the figure are in a (xy) plane, and, in addition, a T orbital for each carbon atom exists perpendicular to the plane. Since the directions of the three u bonds of the central carbon atom in Fig.l.4 are ( 0 , l , O ) , ( f i / 2 , 1 / 2 , 0 ) , and (  f i / 2 , 1 / 2 , 0 ) , the corresponding sp2 hybridized
CHAPTER 1 . CARBON MATERIALS
8
orbitals Isp:) (i = a , b , c ) are made from 2s, 2p,, and 2py orbitals as follows: ISP3
= C112S)  G
T 12py)
We now determine the coefficients C1,C2, and Cs. F'rom the orthonormal requirements of the Ispi) and 12s), 12p,,,) orbitals, we obtain three equations for determining the coefficients, Ci (i = 1, . , 3 ) :

+
c;+c;+c;= c,c2 2 ClC3+
JCZj
1
=o = 0,
;J1.1.J1.;.
(1.5)
yielding the solution of Eq. (1.5) given by C1 = C2 = l / f i and C, =  l / f i . The sp2 orbitals thus obtained have a large amplitude in the direction of the three nearestneighbor atoms, and these threedirected orbitals are denoted by trigonal bonding. There are two kinds of carbon atoms in polyacetylene, as shown in Fig. 1.4, denoting different directions for the nearestneighbor hydrogen atoms. For the upper carbon atoms in Fig. 1.4, the coefficients of the )2py)terms in Eq. (1.4) are positive, but are changed to  1 2 ~ ~for ) the lower carbon atoms in the figure. 1.2.3 sp3 Hybridization: Methane, (CH4)
The carbon atom in methane, (CH4), provides a simple example of sp3 hybridization through its tetragonal bonding to four nearest neighbor hydrogen atoms which have the maximum spatial separation from each other. The four directions of tetrahedral bonds from the carbon atom can be selected as (l ,l ,l ), (1, 1, l ) , (  1 , 1 , l), (1, 1,l). In order to make elongated wavefunctions to these direction, the 2s orbital and three 2 p orbitals are mixed with each other, forming an sp3 hybridization. Using equations similar to Eq. (1.4) but with the four unknown coefficients, Ci, (i = 1, . . . ,4), and orthonormal atomic
1.2. f f Y ~ R X ~ X Z AINT A ~0 CARBON ~ ATOM
9
wavefunctions, we obtain the sp3 hybridized orbitals in these four directions:
+
In general for spn hybridization, n 1 electrons belong to the carbon atom occupied in the hybridized u orbital and 4  ( n 1) electrons are in ?r orbital. In the case of sp3 hybridization, the four valence electrons occupy 2s' and 2p3 states as u bonding states. The excitation of 2s' and 2p3 in the solid phase from the 2sa2p2 atomic ground state requires an energy approximately equal to the energy difference between the 2s and 2 p (4 eV) Levels. However the covaient bonding energy for u orbitals is larger (3 4 eV per bond) than the 2s2p energy separation. It is important to note that the directions of the three wavefunctions in the sp3 hybridization are freely determined, while the remaining fourth direction is determined by orthonormal conditions imposed on the 2p orbitals. This fact gives rise to possible sp2 hybridization of a planar pentagonal (or heptagonal) carbon ring and sp2+q (0 < q < I) hybridization* which is found in fullerenes. A general sp2+q hybridization is expected to have a higher excitation energy than that of the symmetric sp2 hybridization discussed here because of the electronelectron repulsion which occurs in the hybridized orbital.
+

1.2.4
Carbon Is Core Orbitals
Carbon Is core orbitals do not generally affect the solid state properties of carbon materials, since the energy position of the 1s core levels is far from the Fermi energy compared with the valence levels. Because of the small overlap between the Is orbitals on adjacent atomic sites in the solid, the energy spectrum of the 1s core levels in carbon materials is sharp and the core level energies lie close to that of an isolated carbon atom. Using Xray photoelectron spectroscopy (XPS), the energy of the Is core level is measured relative to the position of the *This notation denotes an admixture of sp2 and sp3 hybridization.
CHAPTER 1. CARBON MATERIALS
10
c,,
c Is
I
1.9 eV
hv= 1486.6 eV
5
10
l
I
1
I
60
l
L
45
I
I
0
1
30
1
I
I
1
15
Relalive Binding Energy (eV)
I
I
0
J
Fig. 1.5: Xray photoelectron spectra (XPS) for the carbon 1sderived satellite structures for c60 films [25]. The sharp feature 1 is the fundamental XPS line, while the downshifted features 210 refer t o c60 excitations (see text). The XPS data are shown on two energy sales to emphasize features near EF (upper spectrum) and features farther away in energy (lower spectrum) "&].
vacuum level, and this energy difference is especially sensitive to the transfer of electric charge between carbon atoms. Specifically, the 1s core level shifts in energy relative to the vacuum level by an amount depending on the interaction with nearestneighbor atoms, and this effect is known as the chemical shift of XPS. Furthermore, XPS refers to the photoelectron spectroscopy (PES) process when the excitation photon is in the xray range and the electron excitation is from a core level. XPS spectra have been obtained for the unoccupied orbitals for a variety of fullerenes. For example, Fig. 1.5 shows the XPS spectrum for c 6 0 [25]. In this spectrum, we can see welldefined peaks which show an intense, narrow main line (peak #1 in Fig. 1.5) identified with the emission of a photoexcited electron from the carbon 1s state, which has a binding energy of 285.0 eV and a very small linewidth of 0.65 eV at halfmaximum intensity [25].
1.2. HYBRIDIZATION IN A CARBON ATOM
Dimension isomer hybridization density [g/cm31 Bond Length
tJ4l
electronic properties
Table 1.1: Isomers made of 1D CEO nanotube fullerene carbyne sp2 SP2 (SP) 1.72 1.22.0 2.683.13 1.40(C=C) 1.44(C=C) 1.46(CC) semiconductor metal or E, = 1.9eV semiconductor 0D
11
carbon 2 D graphite fiber
3D diamond amorphous
SP2
SP3
2.26 N2 1.42(C=C) 1.44(C=C) semimetal
3.515 23 1.54(CC)
insulating E, = 5.47eV
The sharpest sideband feature in the downshifted XPS spectrum (labeled 2) is identified with an onsite molecular excitation across the HOMOLUMO gap at 1.9 eV [ZS]. Features 3, 4 and 5 are the photoemission counterparts of electric dipole excitations seen in optical absorption, while features 6 and 10 represent i n t r a m o l e c u l ~plasmon collective oscillations of the T and cr charge distributions. Plasma excitations are also prominently featured in core level electron energy loss spectra (EELS). 1.2.5 Isomers of Carbon
The sp" hybridization discussed in the previous section is essential for determining the dimensionality of not only carbonbased molecules, but also carbonbased solids. Carbon is the only element in the periodic table that has isomers from 0 dimensions (OD) to 3 dimensions (3D), as is shown in Table 1.1. Here we introducepossible structures of carbon materials in the solid phase, which are closely related t o the sp" hybridization. In sp" hybridization, (n 1) u bonds per carbon atom are formed, these cr bonds making a skeleton for the local structure of the ndimensional structure. In s p hybridization, two c bonds make only a onedimensional chain structure, which is known as a 'carbyne'. A threedimensional solid is formed by gathering these carbyne chains. In sp3 hybridization, four D bonds defining a regular tetrahedron are sufficient to form a threedimensional structure known as the diamond structure. It is interesting that sp2 hybridization which forms a planar structure in twodimensiona1 graphite also forms a planar local structure in
+
CHAPTER 1 . CARBON MATERIALS
12
1400
OlPUOND
400
\,,
;
LllUlD
’
OUMONO
Fig. 1.6: One version of the phase diagram of carbon suggested by Bundy [26]. The diamond (Di) and graphite (Gr) phases are emphasized in this figure. Other phases shown in the diagram include hexagonal diamond and a high temperaturehigh pressure phase, denoted in the diagram by du Pont, meteorites and shockquench, which has not been studied in much detail and may, in part, be related to carbynes. Liquid carbon, which has been studied at low pressures and high temperatures, and an unexplored high pressure phase, which may be metallic, are also indicated on the figure.
the closed polyhedra (0dimensional) of the fullerene family and in the cylinders (1dimensional) called carbon nanotubes. Closely related to carbon nanotubes are carbon fibers which are macroscopic onedimensional materials, because of their characteristic high length to diameter ratio. A carbon fiber, however, consists of many graphitic planes and microscopically exhibits electronic properties that are predominantly twodimensional, Amorphous carbon is a disordered, threedimensional material in which sp2 and sp3 hybridization are both present, randomly. Amorphous graphite, which consists mainly of sp2 hybridization, is a graphite with random stacking of graphitic layer segments. Because of the weak interplanar interaction between two graphitic planes, these planes can move easily relative to each other, thereby forming a solid lubricant. In this sense, amorphous graphite can behave like a twodimensional material. Under ambient conditions and in bulk form, the graphite phase with strong inplane trigonal bonding is the stable phase, as indicated by the phase diagram of Fig. 1.6 [26281. Under the application of high pressure and high temperature (both of which are somewhat reduced when catalyst particles like iron or nickel
I .2. ~ Y ~ ~ I ~ ~ Z A INTA ICOA N ~ B O NA T O ~
13
are used), transformation to the diamond structure takes place. Once the pressure is released, diamond remains essentially stable under ambient conditions although, in principle, it will very slowly transform back to the thermodynamically stable form of solid carbon, which is graphite. When exposed to various perturbations, such as irradiation and heat, diamond will quickly transform back t o the equilibrium graphite phase. Hereafter we introduce the ‘onedimensional’ isomers, carbynes and carbon fibers, which are related to nanotubes, as the subject of the following chapters.
1.2.6 Carbynes Linear chains of carbon which have s p bonding have been the subject of research for many years [29]. A polymeric form of carbon consisting of chains [. * C=C . * Itp for la > 10 has been reported in rapidly quenched carbons and is referred to as “carbynes.” This carbon structure is stable at high temperature and pressure as indicated in the phase diagram of Fig. 1.6 as shockq~enchedphases. Carbynes are silverwhite in color and are found in meteoritic carbon deposits, where the carbynes are mixed with graphite particles. Synthetic carbynes have also been prepared by sublimation of pyrolytic graphite [30,31]. It has been reported that carbynes are formed during very rapid solidification of liquid carbon, near the surface of the solidified droplets formed upon solidification [32], Some researchers [31351 have reported evidence that these linearly bonded carbon phases are stable at temperatures in the range 2700 < T < 4500 K. Carbynes were first identified in sampfes found in the Ries crater in Bavaria [36] and were later synthesized by the dehydrogenation of acetylene I31,37]. The carbynes have been characterized by xray diffraction, scanning electron microscopy (TEM) , ion micromass analysis, and spectroscopic measurements which show some characteristic features that identify carbynes in general and specific carbyne polymorphs in particular. The crystal structure of carbynes has been studied by xray diffraction through identification of the Bragg peaks with those of synthetic carbynes produced from the sublimation of pyrolytic graphite [33,37]. In fact, two poIymorphs of carbynes (labeled Q and /3) have been identified, both being hexagonal and with lattice constants a, = 8.94 A, ca = 15.36 A;
[email protected]= 8.24 A, cp = 7.68 A [31]. Application of pressure converts the

CHAPTER 1. CARBON MATERIALS
14
a phase into the ,f3 phase. The numbers of atoms per unit cell and the densities are, respectively, 144 and 2.68 g/cm3 for the a phase and 72 and 3.13 g/cm3 for
the p phase [38]. These densities determined from xray data [31] are in rough agreement with prior estimates [39,40]. It is expected that other less prevalent carbyne polymorphs should also exist. In the solid form, these carbynes have a hardness intermediate between diamond and graphite. Because of the difficulty in isolating carbynes in general, and specific carbyne polymorphs in particular , little is known about their detailed physical properties. 1.2.7
Vapor Grown Fibers
Vaporgrown carbon fibers can be prepared over a wide range of diameters (from less than 1000 A to more than 100 prn) and these fibers have hollow cores [9]. In fact vaporgrown fibers with diameters less than lOOA were reported many years ago [41431. The preparation of these fibers is based on the growth of a thin hollow tube of about 1000 A diameter from a transition metal catalytic particle (100 di diameter) which has been supersaturated with carbon from a hydrocarbon gas present during fiber growth at 1050OC. The thickening of the vaporgrown carbon fiber occurs through an epitaxial growth process whereby the hydrocarbon gas is dehydrogenated and sticks to the surface of the growing fiber. Subsequent heat treatment to w25OO0C results in carbon fibers with a tree ring concentric cylinder morphology [44]. Vaporgrown carbon fibers with micrometer diameters and lengths of 30 cm provide a close analogy t o carbon nanotubes with diameters of nanometer dimensions and similar length to diameter ratios (see Chapter 5). Carbon fibers represent an important class of graphiterelated materials from both a scientific and commercial viewpoint. Despite the many precursors that can be used to synthesize carbon fibers, each having different crosssectional morphologies [9,44], the preferred orientation of the graphene planes is parallel t o the fiber axis for all types of carbon fibers, thereby accounting for the high mechanical strength and high modulus of carbon fibers [9]. Asprepared vaporgrown fibers have an “onion skin” or “tree ring” morphology [Fig. 1.7(a)], and after heat treatment to about 30OO0C, they form facets [Fig. 1,7(b)]. Of all carbon fibers [9], these faceted fibers are closest to crystalline graphite in both crystal structure and properties. The commercial pitch and PAN fibers with other
1.2. HYBRIDIZATION IN A CARBON ATOM
a
15
b
Fig. 1.7: Sketch illustrating the morphology of vaporgrown carbon fibers (VGCF): (a) asdeposited at llOO°C [9], (b) after heat treatment to 30OO0C [9]. morphologies (not shown), are exploited for their extremely high bulk modulus and high thermal conductivity, while the commercial PAN (polyacrylonitrile) fibers with circumferential texture are widely used for their high strength [9]. The high modulus of the mesophase pitch fibers is related to the high degree of caxis orientation of adjacent graphene layers, while the high strength of the PAN fibers is related to defects in the structure, which inhibit the slippage of adjacent planes relative to each other. Typical diameters for these individual commercial carbon fibers are 10 pm, and since the fibers are produced in a continuous process, they can be considered to be infinite in length. These fibers are woven into bundles called tows and are then wound up as a continuous yarn on a spool. The remarkable high strength and modulus of carbon fibers are responsible for most of the commercial interest in these fibers [9,44].

CHAPTER 2.
Tight Binding Calculation of Molecules and Solids
In carbon materials except for diamond, the 7r electrons are valence electrons which are relevant for the transport and other solid state properties. A tight binding calculation for the 7r electrons is simple but provides important insights for understanding the electronic structure of the 7~ energy levels or bands for graphite and graphiterelated materials. 2.1
Tight Binding Method for a Crystalline Solid
In this section we explain the tight binding method for a crystalline solid. In the following sections, we show some examples of energy bands for carbon materials discussed in the Chapter 1. 2.1.1
Secdur ~ q ~ u ~ ~ o n
Because of the translational symmetry of the unit cells in the direction of the , any wave function of the lattice, $, should lattice vectors, a'i, (i = 1, + 3), satisfy Bloch's theorem
a
where Tai is a translational operation along the lattice vector 4, and is the wave vector[45,46]. There are many possible functional forms of 9 which satisfy Eq. (2.1). The most commonly used form for Q is a linear combination of plane waves. The reason why plane waves are commonly used is that: (1) the integration of the plane wave wavefunction is easy and can be done analytically, (2) the numerical accuracy only depends on the number of the plane waves used. However, the plane wave method also has limitations: (1) the scale of the
17
18
CHAPTER 2. TIGHT BINDING CALCULATION
computation is large, and (2) it is difficult to relate the plane wave wavefunction to the atomic orbitals in the solid. Another functional form which satisfies Eq. (2.1) is based on the j th atomic orbital in the unit cell (or atom). A tight binding, Bloch function @j(z,q is given by,
Here R' is the position of the atom and pj denotes the atomic wavefunction in state j. The number of atomic wavefunctions in the unit cell is denoted by n , and we have n Bloch functions in the solid for a given To form @j(c,qin Eq. (2.2), the 'pj's in the N ( loz4) unit cells are weighted by the phase factor exp(iz 2)and are then summed over the lattice vectors of the whole crystal. The merits of using atomic orbitals in Bloch functions are as follows: (1) the number of basis functions, n , can be small compared with the number of plane waves, and ( 2 ) we can easily derive the formulae for many physical properties using this method.* Hereafter we consider the tight binding functions of Eq. (2.2) to represent the Block functions. It is clear that Eq. (2.2) satisfies Eq. (2.1) since
z.
where we use t,he periodic boundary condition for the M in each S;i direction,
N1/3 unit vectors
consistent with the boundary condition imposed on the translation vector T M ~=, 1. From this boundary condition, the phase factor appearing in Eq. (2.2) satisfies exp{ikMui} = 1, from which the wave number lC is related by the integer *The limitations of the tight binding method are that: (1) there is no simple rule to improve the numerical accuracy and (2) atomic orbitals do not describe the interatomic region.
2.1. TIGHT BINDING METHOD FOR A CRYSTALLINE SOLID
19
In three dimensions, the wavevector is defined for the z, y and z directions, as k,, Icy and lcz. Thus M 3 = N wave vectors exist in the first Brillouin zone, where the ki can be considered as continuum variables. The eigenfunctions in the solid @ j ( z ,3( j = 1, *  . , n),where n is the number of Bloch wavefunctions, are expressed by a h e a r combination of Bloch functions @ji[Z,3 as follows:
c n
q z , q=
Cjjl(rC'>@j,(lc',3 ,
(2.6)
j'=l
where C j j ~ ( $are ) coefficients t o be determined. Since the functions Sj(Z,q should also satisfy Bloch's theorem, the summation in Eq. (2.6) is taken only for the Bfoch orbitals @j/(g, with the same value of 2. + The jth eigenvalue Ej(k) (j= 1, * , n ) as a function of 5 is given by
 
where H is the Hamiltonian of the solid. Substituting Eq. (2.6) into Eq. (2.7) and making a change of subscripts, we obtain the following equation, n
C
n
CGCijt(@
[email protected],)
j,j}=l
C Sjj,(i)CGCij, j,ji=l
where the integrals over the Block orbitals, R j j ~ ( 2and ) S j j t ( i ) are called transfer integral matrices and overlap integral matrices, respectively, which are defined by .*
Bjj/(lc)= { @ j p i I @ j / ) , Sjj,$)
= ((ajlay) ( j , j ' = l,'.*,?Z),
(2.9)
When we fix the values of the n x n matrices ' ? i j j t ( i ) and Sjji($) in Eq. (2.9) for a given value, the coefficient C$ is optimized 80 as to minimize &(Z).
CHAPTER 2. TIGHT BINDING CALCULATION
20
It is noted that the coefficient CTj is also a function of i, and therefore Czj is determined for each $. When we take a partial derivative for Ci;. while fixing the other Ciji, CGl,and Cij coefficients,+we obtain zero for the local minimum condition as follows, N
N
(2.10) N
When we multiply both sides of Eq. (2.10) by
S j j i ( ~ ) C ~ Cand i j ~substitute j,jl=l
the expression for E i ( i ) of Eq. (2.8) into the second term of Eq. (2.10), we obtain N
N
C Rjji(k)Ciji = Ei(Z)C Sjji(Z)Ciji. +
j'=l
(2.11)
ji=l
Defining a column vector,
ci =
(c:)l
(2.12)
G N
Eq. (2.11) is expressed by
xci = E j ( i ) S C i .
(2.13)
Transposing the right hand side of Eq. (2.13) to the left, we obtain ['H E i ( i ) S ] C i = 0. If the inverse of the matrix ['Id  E i ( z ) S ] exists, we multiply both sides by [X Ei(i)S]' to obtain Ci = 0 (where 0 denotes the null vector), which means that no wavefunction is obtained. Thus the eigenfunction is given only when the inverse matrix does not exist, consistent with the condition given by det[X  ES] = 0, (2.14) where Eq. (2.14) is called the secular equation, and is an equation of degree + n , whose solution gives all n eigenvalues of Ei( i) (i = 1, . . n ) for a given k. 'Since C,, is generally a complex variable with t w o degrees of freedom, a real and a complex part, both C,, and C:, can be varied independently.
Using the expression for Ei(2) in Eqs. (2.7) and (2.11), the coefficients Ci as a function of $ are determined. In order to obtain the energy dispersion relations we solve the secular equation Eq. (2.14), for a number (or energy bands) E{($)), of high symmetry ipoints. 2.1.2 Procedure for obtaining the energy dispersion
In the tight binding method, the oneelectron energy eigenvalues E ; ( l ) are obtained by solving the secular equation Eq. (2.14). The eigenvalues Ei(g) are a periodic function in the reciprocal lattice, which can be described within the first Brillouin zone. In a two or three dimensional solid, it is difficult t o show the energy dispersion relations over the whole range of k values, and thus we plot Ei($) along the high symmetry directions in the Brillouin zone. The actual procedure of the tight binding calculation is as follows: #
1. Specify the unit cell and the unit vectors, 4. Specify the coordinates of the atoms in the unit cell and select n atomic orbitals which are considered in the calculation. 2. Specify the Bril~ouinzone and the reciprocal lattice vectors, &. Select the high symmetry directions in the Brillouin zone, and points along the high symmetry axes.
3. For the selected $ points, calculate the transfer and the overlap matrix element, 3cij and Sij.*
4. For the selected $ points, solve the secular equation, Eq. (2.14) and obtain the eigenvalues Ei(2) (i = 1,. . ' , n ) and the coefficients Cij($). Tightbinding calculations are not selfconsistent calculations in which the occupation of an electron in an energy band would be determined selfconsistently. That is, for given electron occupation, the potential of the Hamiltonian is calculated, from which the updated electron occupation is determined using, for example, Mulliken's gross population analysis [47]. When the input and the output of occupation of the electron are equal to each other within the desired accuracy, the eigenvalues are said to have been obtained selfconsistently. *Whenonly the transfer matrix is calculatedand the overlap matrix is taken as the unit matrix, then the SlaterKoster extrapolationscheme results.
CHAPTER 2. TIGHT BINDING CALCULATION
22
............... iH
i I \
dp/\ ci c i I ;
1 :
H i
H i
..........*.....
/
Fig. 2.1: The unit cell of iranspolyacetylene bounded by a box defined by the dotted lines, and showing two inequivalent carbon atoms, A and B, in the unit cell.
C
I
H
In applying these calculational approaches t o real systems, the symmetry of the problem is considered in detail on the basis of a tightbinding approach and the transfer and the overlap matrix elements are often treated as parameters selected to reproduce the band structure of the solid obtained either experimentally or from first principles calculations. Both extrapolation methods such as 5 perturbation theory or interpolation methods using the SlaterKoster approach are commonly employed for carbonrelated systems such as a 2D graphene sheet or 3D graphite [9]. 2.2
Electronic Structure of Polyacetylene
A simple example of nenergy bands for a onedimensional carbon chain is polyacetylene (see Sect. 1.2.2). In Fig. 2.1 we show, within the box defined by the dotted lines, the unit cell for transpolyacetylene (CH),which contains two inequivalent carbon atoms, A and B, in the unit cell. As discussed in Sect. 1.2.2, there is one 7relectron per carbon atom, thus giving rise to two nenergy bands called bonding and antibonding nbands in the first Brillouin zone. The lattice unit vector and the reciprocal lattice vector of this onedimensional molecule are given by a'l = (a, 0,O) and b l = ( a / 2 ~ , 0 , 0 )respectively. , The Brillouin zone is the line segment a/n < b < a / a . The Bloch orbitals consisting of A and B atoms are given by 4
(2.15) where the summation is taken over the atom site coordinate R, for the A or B
2.2. ELECTRONIC STRUCTURE OF POLYACETYLENE
23
carbon atoms in the solid. The ( 2 x 2) matrix Hamiltonian, X , p , ( o , P = A , B ) is obtained by substituting Eq. (2.15) into Eq. (2.9). When o = ,d = A,
+(terms equal to or more distant than R = R' & 2a) = €a,,
+ (terms equal to or more distant than R = R' f a).
In Eq. (2.16) the maximum contribution to the matrix element RAAcomes from R = R', and this gives the orbital energy of the 2p level, ~ 2 ~ .The * next order contribution t o X A A comes from terms in R = R ' f a , which will be neglected for also gives cZp for the same order of approximation. simplicity. Similarly, Next let us consider the matrix element X A B ( T ) .The largest contribution to X A B ( P ) arises when atoms A and B are nearest neighbors. Thus, in the summation over R', we only consider the cases R' = R f a/2 and neglect more distant terms to obtain
= 2t cos(lca/2) where the transfer integral 1 is the integral appearing in Eq. (2.17) and denoted byt. t = ('PA(TR)lXIPB(rRf a/2))* (2.18) It is stressed that t has a negative value. The matrix element X E A ( T )is obtained from X A B ( Y )through the Hermitian conjugation relation 3  l = ~ X;,, ~ but since X A B is real, we obtain X B A = FLAB. 'Note that czP is not simply the atomic energy value for the free atom, because the Hamiltonian contains a crystal potential. tHere we have assumed that all the T bonding orbitals are equal (1.5A bonds). In the real (CH), compound, bond alternation occurs, in which the bond energy alternates between 1.7A and 1.3A bonds, and the two atomic integrations in Eq. (2.17) me not equal. Although the distortion of the lattice lowers the energy, the electronic energy always decreases more than the lattice energy in a onedimensional material, and thus the lattice becomes deformed by a process called the Peierls instability. See details in Sect. 11.3.1
CHAPTER 2. TIGHT BINDING CALCULATION
24
J
L
2.0
1.0
I
.
0.5
,
.
0.0 ka/n
,
0.5
.
1.0
Fig. 2.2: Th: energy dispersion relation E*(L) for polyacetylene [(CH),], given by Eq. (2.21) with values for the parameters t =  1 and s = 0.2. Curves E+(L)and E(k)are called bonding a and antibonding a* energy bands, respectively, and the plot is given in units of Itl.
The overlap matrix Sij can be calculated by a similar method as used for Xij, except that the intraatomic integral yields the energy for the crystal Hamiltonian Xij, but the overlap matrix rather yields unity for the case of Saj, if we assume that the atomic wavefunction is normalized, SAA = SBB = 1 and SAB = S B A = 2scos(ba/2), where s is the overlap integral between the nearest A and B atoms, (2.19) S = ( ‘ P A ( r  R)l(oB(r  R k a/2)). The secular equation for the 2pz orbital of [(CH),] is given by 2(t  s E ) CoS(ka/2) E 2(t  sE)COS(LQ/~) ~2~  E 62p
(2.20)
=
(cap
 E)’ 4(t  s E ) cos2(ka/2) ~
= 0, yielding the eigenvalues of the energy dispersion relations of Eq. (2.20) given by
E*(i) =
+
f 2t cos(Ica/2) a a ( < L < ) 1 f 2s cos(ka/2) ’ Q Q
EZp
(2.21)
in which the sign defines one branch and the  sign defines the other branch, as shown in Fig. 2.2, where we use values for the parameters, ~2~ = 0, t = 1, and s = 0.2. The levels E+ and E are degenerate at La = &T. E + ( k ) and E  ( k ) are called bonding a and antibonding a* energy bands, respectively. Since there are two a electrons per unit cell, each with a different
25
2.3. TWODIMENSIONAL GRAPHITE
(b) ,
"L ~
&$.,K
[email protected] [email protected][email protected] ........... .......,.... .. . M .. ... ,,
0.7 nm), the range that has been observed experimentally. The simple tight binding result for singlewall nanotubes which considers only x orbitals, that one third of the nanotubes are metallic and two thirds are semiconducting, has a symmetry basis which is discussed in *When we see unfolded energy bands of carbon nanotubes in the t w ~ ~ m e n s i oBrillouin n~ zone of graphite, the degenerate point at the K point moves away from the A' point by taking account of the hybridi~tioneffect. However, the degeneracy of the conduction and valence bands is not affected by the hybridization. This degeneracy comes from the symmetry that A and 3 atoms are equivalent to each other in the unit cell of graphite. Thus, since the hybridieation effect does not change the equivalence between the A and B atoms, this symmetry holds. In armchair nanotubes, since the shift of the k vector at the Fermi energy by the curvature effect is along the onedimensional Brillouin zone, we get a metallic condition for armchair nanotubes even when curvature effects are taken into account.
72
CHAPTER 4 . ELECTRONIC STRUCTURE OF NANOTUBES
Sect. 4.1.1. There are several physical processes that tend to modify these simple considerations. A first principles LDA calculation [go] has determined that for very smalldiameter nanotubes the curvature of the graphene sheet results in band shifts which move their band edges into the semiconducting energy gap, hence suggesting that all very smalldiameter nanotubes should be metallic. A contrary conclusion could be reached if a Peierls distortion of the 1D conductor produced an energy gap at the Fermi level. LDAbased calculations have also been carried out for BN nanotubes, and the results suggest that BN nanotubes should be stable and should have a band gap of 5.5 eV, independent of diameter [90,91], and the band gap of crystalline BN is of about the same magnitude throughout the Brillouin zone. Thus no quantum effects as are observed in carbon nanotubes are expected for B N nanotubes. However, a relatively large energy gap is expected, compared with carbon nanotubes, so that BN nanotubes on either the inside or outside of carbon nanotubes can be used to provide insulation to carbon nanotubes. These calculations for the electronic structure of BN nanotubes stimulated experimental work, leading to the successful synthesis of pure BN multiwall nanotubes [92], with inner diameters of 13 nm and lengths up to 200 nm. The B N nanotubes are produced in a carbonfree plasma discharge between a BNpacked tungsten rod and a cooled copper electrode. Electron energy loss spectroscopy studies on individual nanotubes confirmed the BN stoichiometry [92,93].
CHAPTER 5.
Synthesis of Carbon Nanotubes
This chapter describes synthesis methods for carbon nanotubes, with primary emphasis on singlewall nanotubes. Two relatively efficient methods to synthesize singlewall carbon nanotubes have been identified: laser vaporization and carbon arc synthesis, and both methods depend on the use of catalysts. Other techniques such as vapor growth are also reviewed. Also discussed in this chapter are the synthesis of multiwall carbon nanotubes, the purification of carbon nanotubes, the insertion of metals into the hollow core of carbon nanotubes, and the doping of carbon nanotubes with alkali metals. 5.1
SingleWall Nanotube Synthesis
The first experimental identification in 1991 of carbon nanotubes was on multiwall nanotubes[l9]. This report stimulated a large number of theoretical works on the structure and properties of the simpler and more fundamental singlewall carbon nanotubes, one atomic layer in thickness in the radial direction (see Fig. 3.1). The experimental discovery of singlewall carbon nanotubes in 1993[58, 941 further stimulated work in the field, though, at first, only small quantities of singlewall nanotubes were available experimentally for systematic studies. These singlewall nanotubes were generally found along with very much larger concentrations of amorphous carbon, carbon nanoparticles and other carbonbased materials, and the singlewall constituents contained a distribution of diameters and chiral angles, as explained below. For these reasons most of the experimental studies continued to be done on multiwall nanotubes. The recent discovery in 1996 of a much more efficient synthesis route, involving laser vaporization of graphite [55] t o prepare arrays or “ropes” of ordered singlewall nanotubes, offered major new opportunities for quantitative experi73
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES mental studies of carbon nanotubes. By making the singlewall nanotubes available to many research groups worldwide, progress was made for the first time in quantitative measurements of the physical properties of singlewall carbon nanotubes. The detailed mechanisms responsible for the growth of these nanotubes are not yet well understood. Therefore we can expect extensive research to be carried out on the growth mechanism and on the development of new growth techniques that provide more controlled growth of nanotubes. Whereas multiwall nanotubes require no catalyst for their growth, catalyst species are necessary for the growth of the singlewall nanotubes, and more than one catalytic species seem t o be necessary t o grow ropes of singlewall nanotubes. Soon after the publication of the laser vaporization method for the ;synthesis of singlewall carbon nanotube ropes, another synthesis route was found for the synthesis of gram quantities of singlewall carbon nanotubes, using the carbon arc method [52]. Because of the potential interest of carbon nanotubes for practical applications, there is also interest in developing continuous synthesis methods more appropriate for scaleup and low cost, and this may perhaps be accomplished by vapor growth methods discussed in Sect. 5.4. The remaining sections of the chapter briefly deal with the purification of nanotube samples (Sect. 5.51, nanotube opening, wetting, filling and alignment (Sect. 5.6), nanotube doping (Sect. 5.7), temperature regimes for carbonization and graphitization (Sect. 5.8), and growth mechanics (Sect. 5.9). 5.2
Laser Vaporization Synthesis Method
An efficient route for the synthesis of bundles of singlewall carbon nanotubes with a narrow diameter distribution employs the laser vaporization of a graphite target. In the early reports of the laser synthesis technique [55], high yields with >70%90% conversion of graphite to singlewall nanotubes were reported in the condensing vapor of the heated flow tube (operating at 12OOOC). A CoNi/graphite composite laser vaporization target was used, consisting of 1.2 atom 3' % CoNi alloy with equal amounts of Co and Ni added to the graphite (98.8 atom %) [55].Two sequenced laser pulses were used to evaporate a target containing carbon mixed with a small amount of transition metal from the target (see
5.2. LASER VAPORIZATION SYNTHESIS METHOD
75
furnace at 1,200’ Celsius
\
LL
watercooled copper collector
argon
1
graphite target
neodymiumyttfiumalumlnumgarnet laser
Fig. 5.1: Singlewalled nanotubes produced in a quartz tube heated to 1200°C by the laser vaporization method, using a graphite target and a cooled collector for nanotubes [95]. Fig. 5.1). Flowing argon gas sweeps the entrained nanotubes from the high temperature zone to the watercooled Cu collector downstream, just outside the furnace [55 961. The material thus produced appears in a scanning electron microscope (SEM) image as a mat of “ropes” 1020 nm in diameter and up to 100 pm or more in length [see Fig. 5.2(a)]. Under transmission electron microscope (TEM) examination [see Fig. 5.2(b)], each rope is found to consist primarily of a bundle of singlewall carbon nanotubes aligned along a common axis. Xray diffraction (which views many ropes at once) and transmission electron microscopy experiments (which view a single rope) show I551 that the diameters of the singlewall nanotubes have a strongly peaked distribution at 1.38ir0.02 nm, very close to
76
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES
Fig. 5.2: (a) Ropes of singlewall carbon nanotubes observed by scanning electron microscopy (SEM). The ropes are 1020 nm thick and 100 p m long. (b) At higher magnification, the TEM image shows that each rope contains a bundle of singlewall nanotubes with diameters of 1.4 nm, arranged in a triangular lattice (with lattice constant 1.7 nm). Such an image is seen when the rope bends through the image plane of the microscope [55I* the diameter of an ideal (10,lO) nanotube which is defined in Eq. 3.2. A detailed transmission electron microscopy study of carbon nanotubes prepared by the laser vaporization method [55] has shown that the carbon nanotube chiral indices (n,rn) are mainly (10,lO) (44%), (9,9) (20%), and some (12,8) [97], while others, presumably using different growth conditions, have reported chiral angles in the range A0 = 7.3O [56,98]. Thus for nanotube diameters ranging from that for the (8,8) to ( 1 1 , l l ) armchair nanotubes, there are only 17 possible nanotubes [97]. The singlewall nanotubes are held together by weak van der Waals internanotube bonds to form a twodimensional triangular lattice with a lattice constant of 1.7 nm, and an intertube separation of 0.315 nm at closest approach within a rope [55]. By varying the growth temperature, the catalyst
5.3. ARC METHOD OF SYNTHESIZING CARBON NANOTUBES
77
composition and other growth parameters, the average nanotube diameter and diameter distribution can be varied [99]. It is found that the spread in nanotube diameters within a single rope is smaller than between ropes grown at the same time and under the same nominal growth conditions.
5.3
Arc Method of Synthesizing Carbon Nanotubes
The carbon arc provides a simple and traditional tool for generating the high temperatures needed for the vaporization of carbon atoms into a plasma (>3O0O0C) [loo1021. This technique has been used for the synthesis of singlewall and multiwall carbon nanotubes, and ropes of singlewall nanotubes [52]. Typical conditions for operating a carbon arc for the synthesis of carbon nanotubes include the use of carbon rod electrodes of 520 mm diameter separated by 1 mm with a voltage of 2025 V across the electrodes and a dc electric current of 50120 A flowing between the electrodes. The arc is typically operated in 500 torr He with a flow rate of 515ml/s for cooling purposes. As the carbon nanotubes form, the length of the positive electrode (anode) decreases (see Fig. 5.3). Once the arc is in operation, a carbon deposit forms on the negative electrode. For the multiwall carbon nanotube synthesis, no catalyst need be used and the nanotubes are found in bundles in the inner region of the cathode deposit where the temperature is a maximum (25003000°C). The nanotube bundles are roughly aligned in the direction of the electric current flow (see Fig. 5.3) [ l o l l1041. Surrounding the nanotubes is a hard grey shell consisting of nanoparticles, fullerenes and amorphous carbon [1051071.' Adequate cooling of the growth chamber is necessary to maximize the nanotube yield in the arc growth process. The growth of carbon nanotubes appears to be unfavorable under the conditions that are optimized t o synthesize fullerene molecules. Catalysts used t o prepare isolated singlewall carbon nanotubes include transition metals such as Co, Ni, Fe and rare earths such as Y and Gd, while mixed catalysts such as Fe/Ni, Co/Ni and Co/Pt have been used to synthesize ropes of singlewall nanotubes. Although the details of the diameter (and chirality) distribution of the singlewall carbon nanotubes depend on the synthesis conditions, 'During arc synthesis fullerenes are predominantly found in the soot produced by the arc and removed by the helium gas flow, while the nanotubes are contained in a deposit on the cathode.
78
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES
to Pump
Gas Inlet
Window
Fig. 5.3: Crosssectional view of a carbon arc generator that can be used t o synthesize carbon nanotubes [103].
temperature of the arc and the catalyst that is used, the average nanotube diameter is usually small (51.5 nm) and the diameter distribution is usually narrow, as illustrated in Fig. 5.4. It is interesting t o note that the minimum nanotube diameter that has been observed for singlewall carbon nanotubes is 0.7 nm, corresponding to the diameter of c60, the smallest fullerene to obey the isolated pentagon rule [108]. An efficient method for the synthesis of gram quantities of bundles of singlewall carbon nanotubes using the carbon arc technique has been achieved [52]. The greatest mass of singlewall carbon nanotubes is found in a collarette around the cathode, with ~ 2 0 % of the consumed carbon being converted into singlewall carbon nanotubes in the collarette. Since the length of a carbon nanotube is typically on the order of 1 pm, and the growth rate of a 1 pm carbon nanotube is estimated to be less than 0.1 second, the time for the growth of a single circumferential carbon ring is second. This time scale is much shorter than the time needed for the direct obser
VAPOR GROWTH AND O T H E R SYNTHESIS METHODS
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Nanolube diameters (nm)
1.4
1.5
1.6
79
Fig. 5.4: Diameter distribution of isolated singlewall carbon nanotubes prepared by the arc method using a Fe catalyst [581.
vation of the carbon arc electrodes by transmission electron microscopy (TEM) but is much longer than the phonon frequency 1015 Hz. Thus the growth of carbon nanotubes occurs under stable conditions but over a limited range of He (or Ar) pressure, electric current and arc voltage. The iron or cobalt catalyst in the arc process forms both singlewall carbon nanotubes and nanometersize carbide particles surrounded by graphene layers, as well as metal clusters encapsulated within graphene layers [58,94]. Thus purification is necessary to separate out a pure singlewall nanotube sample. When certain transition metals (Fe, Co, Ni, Pb, Mo, W, Cu, Au, ...), rareearth metals (LaNd, GdTm, Lu), or their oxides are packed into a hole in the central region of the positive electrode, carbon nanocapsules are often obtained in the deposit on the negative electrode [109].t Carbon nanocapsules consist of multiwall polyhedra of graphene sheets with interlayer separations of 0.34 nm inside which are contained metals (Fe, Co, Nil Cu and Au) or metal carbides M,C (M = transition metal such as LazC (La = rare earth metal). 5.4
Vapor Growth and Other Synthesis Methods
Fe, Co, and Ni particles are known to be catalysts for vapor grown carbon fiber synthesis [9,17,44], in which hydrocarbons (e.g., CH4, C6H6) and Hz gases are reacted in the presence of Fe, Co, or Ni particles in a reaction tube at llOO°C. tIn the case of Fe, Go, and Ni, catalysts, singlewall nanotubes are observed at the surface of the deposit and nanocapsules are observed in other regions.
80
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES
Fig. 5.5: Carbon nanotubes appear after breakage of the vaporgrown carbon fiber. (a) An SEM image of a broken vapor grown carbon fiber, cut in liquid nitrogen and showing (white arrow) a carbon nanotube emerging from the center of the fiber. (b) HRTEM image showing the broken part of a very thin vapor grown carbon fiber. The nanotube is clearly observed, indicating that thin vapor grown carbon fibers grow from a nanotube core by thickening [59]. The innermost tubes of vapor grown carbon fibers are considered to be carbon nanotubes, as shown in Fig. 5.5. Growth of carbon nanotubes from the vapor phase has also been demonstrated [59]. 5.4.1
Vapor Growth Method
The synthesis of carbon nanotubes from the vapor phase utilizes equipment similar to that used for the preparation of vaporgrown carbon fibers [17,44], with the furnace temperature held at llOO°C and using Fe catalyst particles, but using a low benzene gas pressure [59,110]. A variety of other hydrocarbons, catalysts and catalyst supports have been used successfully by various groups worldwide to synthesize carbon nanotubes. One big advantage of the vapor growth approach is that carbon nanotubes can be made continuously and thus if the optimum conditions for growing pure carbon nanotubes could be found, this could be a very good way to synthesize large quantihes of carbon nanotubes under relatively controlled conditions. Thus the vapor growth method
5.4. V A P O R G R O W T H A N D O T H E R SYNTHESIS METHODS
81
Fig. 5.6: Two kinds of vaporgrown carbon fibers (VGCF) observed in an asgrown sample: (a) a thick hollow fiber formed by a catalytic metal particle, (b) an exposed nanotube and a nanotube that had been pyrolytically coated, thereby increasing the nanotube diameter. has some advantage for scaleup and commercial production. Many presently identified applications of carbon nanotubes can be met with vapor grown carbon nanotubes. Carbon nanotubes can grow at the same time as conventional vaporgrown carbon fibers, as is seen in Fig. 5.6. Most of these nanotubes are multiwall, but some singlewall nanotubes can also be present. Vaporgrown carbon nanotubes have been studied by highresolution TEM in both their asgrown form and after heat treatment. The asgrown nanotubes generally show poor crystallinity. The crystallinity, however, is much improved after heat treatment to 25003000°C in argon, as seen in highresolution TEM studies [110]. Fracture of a thin vapor grown carbon fiber shows the presence of a nanotube at the fiber core, as shown in Fig. 5.5. Referring to the bamboo structure seen on the inside of vapor grown carbon nanotubes (see Fig. 5.7), Endo [110] argues that the capping of an inner layer terminates its growth, so that the exposed cap layer provides growth along the length and the epitaxial layers follow this growth while at the same time adding to the nanotube diameter. The frequentlyobserved bending of the growth axis of the nanotubes is related to the introduction of a heptagonal defect at the bend location.
82
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES
Fig. 5.7: (a) Transmission electron micrograph of a cone containing only single conical shells. The nearly periodic structures of the conical shells appear inside the cone tips [see (a)], which are attributed to overshooting growth on the basis of the open tube growth model [107]. (b) Commonly observed nanotube structure for the cap region of vaporgrown carbon nanotubes heat treated at 28OOOC in Ar. Here a number of bamboolike structures are observed in the core region near the cap [110].
5.4.2
Other Synthesis Methods
Another method of nanotube synthesis relates to the use of carbon ion bombardment to make carbon whiskers [lll,1121. Carbon whiskers are known as a graphite material with high crystallinity [4]whose diameter is 0.11 pm and several mm in length. In the ion bombardment growth method, carbon is vaporized in vacuum through ion or electron irradiation [113], and the resulting deposit containing carbon nanotubes, along with other structures is collected on a cold surface. Little is known about the optimization of the ion bombardment technique in relation to the preparation of nanotubes. The use of solar energy for the synthesis of singlewall carbon nanotubes has
5.5. PURIFICATION
83
Fig. 5.8: (a) Transmission electron micrograph of a web of singleshell nanotubes formed in the catalytic carbon arc method. (b) TEM picture of gas phase purified nanotubes [116].
been reported [114,115], using an experimental chamber where solar energy is focussed on the crucible t o achieve a temperature of 3000 K on a clear day. A mixture of Ni and Y catalysts is used in an argon atmosphere (pressure of 450 mbar). Further research is needed to optimize and control the synthesis process, increase the yield of ropes of singlewall nanotubes, minimize the concentration of carbon nanoparticles and amorphous carbon produced, and t o characterize the carbon nanotubes that are produced. 5.5
Purification
In many of the synthesis methods that have been reported, carbon nanotubes are found along with other materials, such as amorphous carbon and carbon nanoparticles (see Fig. 5.8). Purification generally refers to the isolation of carbon nanotubes from other entities. The separation of nanotubes according to diameter (and chirality) is not considered under the topic of purification, and is not thought to be practical at this time. Three basic methods have been used with limited success for the purification of the nanotubes: gas phase, liquid phase, and intercalation methods [116]. The classical chemical techniques for purification (such as filtering, chromatography, and centrifugation) have been tried, but not found to be effective in removing the
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES carbon nanoparticles, amorphous carbon and other unwanted species shown in Fig. 5.8 [116]. Heating preferentially decreases the amount of disordered carbon relative to carbon nanotubes. Heating could thus be useful for purification, except that it results in an increase in nanotube diameter due to the accretion of epitaxial carbon layers from the carbon in the vapor phase resulting from heating. The gas phase method removes nanoparticles and amorphous carbon in the presence of nanotubes by an oxidation or oxygenburning process [104,117,118]. Much slower layerbylayer removal of the cylindrical layers of multiwall nanotubes occurs because of the greater stability of a perfect graphene layer to oxygen than disordered or amorphous carbon or material with pentagonal defects [117,118]. This method was in fact first used to synthesize a singlewall carbon nanotube. The oxidation reaction for carbon nanotubes is thermally activated with an energy barrier of 225 kJ/mol in air [118]. The gas phase purification process also tends to burn off many of the nanotubes. The carbon nanotubes obtained by gas phase purification are generally multiwall nanotubes with diameters in the range 202OOw and 10 nmlpm in length [104], since the smaller diameter tubes tend to be oxidized with the nanoparticles. Liquid phase removal of nanoparticles and other unwanted carbons has been carried out with some success using a potassium permanganate KMn04 treatment method which tends to give higher yields than the gas phase method, but results in nanotubes of shorter length [116,119]. Finally, the intercalation of unpurified nanotube samples with CuC12KCl results in intercalation of the nanoparticles and other carbon species, but not the nanotubes which have closed cage structures. Thus subsequent chemical removal of the intercalated species can be carried out [120]. A method for the purification of samples containing singlewall nanotube ropes in the presence of carbon nanoparticles, fullerenes and other contaminants has also been reported [83,1211231. 5.6
5.6.1
Nanotube Opening, Wetting, Filling and Alignment Nanotube Opening
Experimental studies show that the cap of a nanotube is more reactive than the cylindrical part because of the presence of pentagons and hence the greater
5.6. N A N O T U B E OPENING, W E T T I N G , FILLING A N D ALIGNMENT 85
curvature and reactivity of the caps. Thus in a vapor phase oxidation process, the cap region is burned off first, thereby providing one method for tube opening. The presence of the pentagons in the cap region also promote tube opening by various chemical reactions, such as with HNOs [116,124]. Tube opening can occur at quite low temperatures (4OO0C), using, for example, a lead metal catalyst in air [125]. The material that is sucked up the nanotube, however, is an oxide of lead [104]. 5.6.2 Nanotube Wetting
A number of liquids have been found to wet the hollow core of carbon nanotubes and others do not show wetting behavior [126]. On the basis of classical theories for wetting, the hollow core of the nanotube will be wet by a fluid if
where 0 is the contact angle of a liquid on a surface, y s v ,ysl and Tiv are, respectively, the solidvapor, solidliquid, and and liquidvapor interfacial surface tensions. Wetting occurs when 0 > ~ / or 2 ysv > ysr. Examples of liquids which wet carbon nanotubes are HNO3, S, Cs, Rb, Se, water, various organic solvents and various oxides such as P b and BiaO:! [124,126]. 5.6.3 Nanotube Filling
Three methods have been used to fill the hollow core of carbon nanotubes: capillarity, pressure, and solvent carrier methods [126]. The capillarity method exploits removal of the cap (or the opening of the tube) followed by wetting, where the contact angle 0 exceeds n/2, as discussed in Sect. 5.6.2. In many cases only partial filling of a nanotube compartment has been achieved, though in some cases whole compartments have been filled [124], with some reports of long continuous nanowires [127,128]. In this work sulfur was shown t o catalyze nanotube filling with many metal species. If a liquid does not wet the nanotube, then pressures exceeding 2y/r are needed for tube filling, where r is the inner radius of the nanotube. Another method that has been successful for introducing high surface tension materials such as Co, Ni, Fe is the use of a solution using H N 0 3 that performs both wetting and tube opening, and at the same time
86
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES
contains a solute which is to be deposited within the nanotube. Subsequent chemistry is used to remove the carrier solvent [129]. 5.6.4
Alignment of Nanotubes
For a variety of experiments and applications it is desirable t o align the carbon nanotubes parallel to each other. If a sample contains an assembly of randomly oriented nanotubes, alignment can be achieved by rubbing in one direction or by cutting a material such as paraffin which contains embedded nanotubes. Nevertheless, the most common source for the alignment of nanotubes is by a selfalignment growth process. Selfaligned bundles of multiwall and singlewall carbon nanotubes are found on the copper collector in the laser vaporization method, on the cathode deposit, and in the collarette for the case of growth by the arc method. 5.7
Nanotube Doping, Intercalation, and BN/C Composites
The substitutional doping of carbon nanotubes with B and N dopants to make the nanotubes ptype and ntype has been discussed [130]. Although some experimental work has been done on the substitutional doping of carbon nanotubes with B and N, most of the experimental activity on the doping of nanotubes has been with the alkali metals [131,132], which do not act as substitutional dopants, but are predicted to lead to enhanced metallic conductivity [133]. Alkali metals readily intercalate into graphite as sheets of alkali metal which are located between graphene sheets in the crystal lattice. These alkali metal layers donate electrons to the graphite layers, thus greatly increasing the electrical conductivity, while at the same time greatly expanding the sample size along the direction normal to the lattice planes. Because of the closed cylindrical structure of carbon nanotubes, the relatively large alkali metal ions cannot find easy entry into perfect nanotubes, nor is there enough space for these ions between adjacent shells of a multiwall nanotube. Therefore the alkali metal ions enter into the carbon nanotubes near structural defects. Once the ions penetrate the outer surface of the nanotube, their large size rips open the nanotube wall. This effect can be seen by microscopic probe studies on carbon nanotubes that have been attacked by alkali metals [131,132].
5.8. TEMPERATURE REGIMES FOR CARBONIZATION AND
. ..
87
For the intercalation of alkali metals and halogens into ropes of single wall carbon nanotubes, a twozone furnace was utilized similar to that previously used for similar intercalations into crystalline graphite 11341, Typical temperatures that were used in the twezone furnace for the alkali metals were 120OC for the nanotubes were 160OC. The large uptake of the alkali metals Rb and K is consistent with a decoration of the carbon atoms on the nanotube surface by a (2 x 2) superlattice of alkali metal species, as well as uptake of alkali metal in the interstitial spaces between the nanotubes in the triangular lattice [135,136]. The A , vibrational mode at 1593 cm' in the undoped nanotubes are down shifted by Rb and K intercalation, consistent with electrons donated by the alkali metals t o the nanotubes, while the Brz intercalation leads to an upshifted mode frequency, consistent with the transfer to electrons from the nanotubes to the halogen [135]. Transport measurements confirm that the intercalant uptake by the nanotube results in a dramatic increase in the electrical conductivity both for the case of Br:! and K [136]. A composite multiwall nanotube 12 nm in diameter, with 3 carbon shells at the interior followed by 6 BN shells in the central region, and 5 carbon shells on the outside, has been synthesized by the arc discharge method using an HfBz electrode and a carbon electrode in a Nz atmosphere [137]. The structure and composition was obtained by a scanning EELS probe across the diameter of the nanotube. BN nanotubes have also been prepared by packing a tungsten rod with BN [87]. 5.8
Temperature Regimes for Carbonization and Graphitization
Because of the importance of temperature as a growth parameter for carbon nanotubes, we summarize in the following some of the important temperature regimes for carbon materials. In addition to the melting (4450 K ) and vaporization (4700 K) temperatures for carbon, two other temperatures are of importance: the carbonization temperature (650750OC) and the graphitization temperature (2300 K). The carbonization temperature is the temperature at which the volatile species are driven off from precursors for carbon materials, leaving behind the basic structural units on the order 1 nm in thickness, as shown in Fig. 5.9. The graphitization temperature (23OO0C) is the temperature at which interplanar site correlation is established and the ABAB stacking
88
CHAPTER 5. SYNTHESIS OF CARBON NANOTUBES
Fig. 5.9: Various steps of the graphitization process as a function of heat treatment temperature THT[138]. arrangement of the 3D graphite structure is formed. The melting and vaporization temperatures for carbon are both extremal values for the condensed phases of matter, with only a small stability region for the liquid phase of carbon. Below the carbonization temperature, carbon cannot change its sp2 covalent bonding configuration. Thus if the solid state is formed by a rapid quenching process t o amorphous carbon, the state of amorphous carbon is metastable below the carbonization temperature. If the solid state is single crystal graphite, this phase is always the most stable state. Between the carbonization and graphitization temperatures, carbon can transform from an amorphous carbon to a stable graphite planar structure at ambient pressure by cutting and reconnecting sp2 covalent bonds. The carbonization temperature is closely related to the desorption temperature of oxygen or hydrogen that is chemically bonded at the edge of graphitic nanocrystals. Oxygen or hydrogen atoms are removed above about 7OOOC in the form of HzO, CO, CO:!, and CH, molecules by cutting carboncarbon bonds. Chemical reactions also occur in the presence of 0 2 , H 2 0 , CO2 at temperatures in the 80O0C12OO0C range where the oxidation process occurs. Dangling carbon bonds, which are related to CH, C0, and CN, etc. bonds, are broken in the
5.9. GROWTH MECHANISMS
89
carbonization process, and CC bonds are reformed at somewhat higher temperatures. The purification temperature for carbon nanotubes corresponds to the temperature for CO and COz formation. The various steps leading to graphitization have been studied by heating amorphous carbons to various temperature THT(see Fig. 5.9) and then observing the TEM micrographs [139,140]. For THT5 800°C, the basic structural units, consisting of a short length (% 10k)of about three parallel layers, start to pile up and form distorted columnar structures, as impurity atoms are released, mostly in gaseous form. For 800 5 THT 5 1500°C, the columnar structures increase in length with a lesser degree of misorientation of the basic structural units as shown in Fig. 5.9. In this step, individual misoriented basic structural units become aligned and the crystallite size along the caxis L , increases gradually. For 1500 THT 1900°C, the columnar structure disappears as wavy ribbons or wrinkled layers are formed by hooking the adjacent columns together, and in this range of THT,both the inplane and caxis crystallite sizes La and L , increase rapidly. By THT 17OO0C,the wavy planar structure begins to disappear and a turbostratic planar stacking arrangement starts to appear, with L a values higher than 200 A at THT 20OO0C. By 21OO0C, most of the inplane structural defects have been eliminated so that a rapid increase in La can occur due t o the disappearance of tilt and twist boundaries. As the graphitic structure develops further with increasing THT,the interlayer distance decreases. At higher T'T, interlayer site correlation between layers starts to develop. Although the graphitization temperature is usually given as 23OO0C, much higher THTvalues (28003000°C) are generally used to obtain 3D graphite crystals by the heat treatment approach,
k 0~ in an unoccupied state for 113 < E < p1 contributes to the microscopic current I.= e / t l , in which t l is the carrier transit time t, = L / u (See Table. 8.1). Then the total current I is given by
where the sum on k is converted to the integral with a spin degeneracy of 2 and the inverse of the level spacing L/21r. 2e/h in Eq, (8.4) is the quantized current per subband per unit energy [A/J]. f ( E  p i ) (i = 1,2) is the Fermi distribution function with the Ferrni energy denoted by pi. When we assume that the total number of conduction channels M ( E ) is constant M over p2 < E < P I , we t note that M ( E ) is not a obtain the last line of Eq. (8.4). It is i m ~ o r t a n to density of states. In fact the dimension of M ( E ) and M is not [states/J], but is rather [states]. If t,he width of a wire W is very small (less than 1 nm), M = 1 even for p1 p2 = 1 eV. On the other hand, if the width of a wire is on the order of 1 pm, and the Fermi energy is about 1 eV, M becomes very large ( lo6) for p1  p2 = 1 eV, It should be noted that we have many k states even when M = 1, All the k states are integrated in Eq. (8.4). Thus we should not count the number of k states in the direction parallel to the current to M . Since V = ( p i  pz)/e is the voltage between the electrodes, the resistance of the ballistic conductor is given by (8.5)
where R, is called the contact resistance and h/2e2 is the quantized resistance
RO ,
Ro=: 12.9Ot54kQ2,
2e2 The inverse of Eq. (8.5) gives the contact conductance G, which is related to the quantized conductance Go by
G, = GoM,
Go =:
2e2 = 77,4809 x lO'U. h
144
CHAPTER 8. TRANSPORT PROPERTIES
Thus in a wire with no scattering the conductance is proportional t o M . The quantized resistance and conductance can be observed in clean semiconductors at very low temperature on samples which have a small M [178]. When we consider the range of values of M for a metal nanotube of finite length L , we expect to find two energy bands ( M = 2) for k > 0 (see Figs. 4.4, 4.5 and 4.6). Thus in the ballistic limit, the conductance of metallic nanotubes is 2Go.f179] When the length of a nanotube L is finite, we expect to find discrete k values spaced by 27rlL. Even if the h states are discrete but still numerous, the relation v = bEj(k)/dK in Eq. (8.4) is applicable as a first approximation. When we consider static scattering, that is, scattering by a potential in one dimension, the wavefunction is solved by a onedimensional Schrodinger equation. Since the phase and amplitude of the wavefunction a t electrode 2 can be obtained from those at electrode 1, a similar discussion for the contact conduc~ancecan be applied. The conductance G and the resistance R are thus given by
where 7 is the transmission probability for a channel to go from electrode 1 to electrode 2, which is given by the sum of transmission probability from ith to j t h channel, ltaj 1” Here we assume again that 7 is constant near the Fermi energy. Equation (8.8) is known as the Landauer formula. The Landauer formula applies only if the wavefunction can spread over the whole sample. The resistance of a mesoscopic wire R,,,for a single channel is given in terms of the transmission probability 7 as
since the reflected wavefunction, which is proportional to voltage drop in the wire. 8.1.2
R = 1  7, causes a
Cdnssic ~ ~ a ~ L,s  (G>2, (8.19)
d m
where ( X ) denotes the ensemble average of X for the sample. An ensemble average means an average for many samples with different impurity distributions. Here we show that the fluctuations do not depend on M unless L , L."

*If M paths were independent,the fluctuation m / ( G ) for M paths would be proportional to r y 1/m. The fact that the fluctuation does not depend on M is an interference effect which
8.1. Q U A N T U M T R A N S P O R T IN A ONEDIMENSIONAL W I R E
.
M=4
Fig. 8.2: A scattering process of the reflected wavefunction for the path entering 1 and exiting 4 in electrode 1 (A,(1 4)). Here we consider 4 channels (M=4). Within the phase coherence length L,, the amplitude of the scattering wavefunction is given by Eq. (8.23).
111
$
..........,...... 112
AP (P4)
1
149
2
We start from the Landauer formula Eq. (8.8) for the conductance normalized by 2 e 2 / h ,

9MT=MM7Z, 2e2/h
(8.20)
where 7, R denote the average on M possible paths of 7 ( r n + n ) and R(rn + n ) , (1 5 n 5 M ) for given rn, where rn and n denote specific channels. In Fig. 8.2 we show a scattering process of R ( l + 4). There are many scattering processes in R ( l + 4) as shown below. When we have M channels, the conductance is generally proportional to M as shown in Eq. (8.20). Since ( 9 ) = M ( T ) = M  M ( R ) and (g2) = M2(?') = M 2  2 M 2 ( z ) ( E ) 2 the , conductance or of (S?), fluctuations can be derived from either the fluctuation of
+
(Sg2)
= M 2 ( 6 T 2 )= M 2 ( 6 X 2 ) .
(s")
(8.21)
Here we consider the fluctuations of the reflectivity, which are known to be relevant for the following discussion. The reflected wave function \k(n + m), for the path entering n and exiting to rn in electrode 1 (see Fig. 8.2), is given by the summation of the wavefunction A p ( m+ n ) for the pth multiple scattering processes, Q ( n + rn) = C A , ( r n + n ) , (8.22) P
where a scattering process of the reflected wave, A P ( m+ n ) can be expressed, for example, by Ap(m

n ) = t ( m + m l ) e x ~ { i k n ~ L r n l } d r n ~W )e x ~ { i h n ~ L r n ~(8.23) } . '.t(m., n)exp{it,L,}. +
+
can be seen universally. Note that the fluctuations become small for samples large compared
with L,.
CHAPTER 8. TRANSPORT PROPERTIES
150
When we assume that the overall phase of A p ( m4 n) is random in @(n4 m), the ensemble average of the reflection probability R(m + T I ) is given by
(R(mt n)) = lQ(n
+
+
m>I2=
lAPl2 (
p
ApA:t) PfP’
=(
1Ap12), P
(8.24) where we use the fact that the ensemble average of the sum of ApAil for p jt+ p’ gives zero because of the assumption of a random phase. In order to discuss the fluctuations we define the following quantity (R(pn3
n)’} =
=
C C
{ApAp/Ap//Ap/ii}
P,P’!PI’,P“‘
+
(IA,I~~A [ ~ ,p ,, p~~ ~It ~ j p t , p l l ~~ p , p l ~ + , p l l ]
(8.25)
P,P’,P” IP”’
= 2{R(~~TI)}Z Thus the fluctuations of the reflectivity are given by
(6R(m
TI)’)
Since (R(m+ n ) )

(R(m+ n)’)  (R(m+
= (R(m+ T I ) ) ’ .
(8.28)
l/Mt we get from Eq. (8.21), (Sg2)
N
(8.27)
1.
Thus the fluctuations in g are on the order of the quantum of conductance 2e2/h which does not depend on M {or on a particular choice of material). We cannot avoid this fluctuation from sample to sample with the same impurity concentration. This fluctuation can be seen by changing the length of the sample provided that the sample size is smaller than the phase relaxation length ( L c L,). The effective distribution of impurities can be changed by applying a magnetic field since the phase of each process [see Eq. (8.23)] is changed by the vector potential eA. When the phase delocalization length L, becomes smaller than L , the fluctuations can be smoothed out. When we consider N = L / L , quantum fluctuatin~ conductors in series, the fluctuation of the conductance become l/N3i2 L3/2 smaller than for a single conductor. This power dependence can be seen by changing L. N
tThe probability of choosing channel n from M channels i s on the order of 1/M. Here we assume that R and 7 are in order of 1, Note that the conductance G is N MGo.
8.1. QUANTUM T R A N S P O R T IN A ONEDIMENSIONAL W I R E
151
When we fix the sample length L , the energy h / t , can be considered as an energy width for phasecoherent motion. This means that within a lifetime t , , an electron can vary its energy by h / t , from the uncertainty relation. At high temperatures such that EBT is larger than h/t, and L , is larger than L , then N = kBT/(h/tlp) independent channels are open incoherently. When we define the thermal diffusion length LT for a given diffusion constant D , the Einstein relation savs that (8.28)
(8.29)
Thus the universal conductance fluctuations show a temperature dependence given by
{
tL
Th
constant
m=Go
(2)lJ2T1/2
(8.30)
t l p h
8.1.5 Negative Magnetoresistance
An another interesting phenomena observed in the weak localization regime is negative magnetoresistance, which refers to a decrease in the resistance with increasing magnetic field. Here we show the basic idea behind the negative magnetoresistance. Consider the special case for A, [see Eq. (8.23)] in which the starting and ending sites are identical, that is R(m + m). Consider a process A, : m + ml + ml + . . . + mp + m , and the timereversed processes A: : m + m q . . + m2 f ml + m ,so that the overall phases are identical. Thus when we consider the reflection probability of Eq. (8.24) for R(m m),we expect a coherence between A, and A:, +
+
R(m
f
m )= ((A1
+ A2 + . .) + (AT + AT + .)I2 *
*
+
/ A Aa12 = 41AI2.
(8.31) If there is no phase correlation between A and Aa, R ( m m) would give 21AI2. Actually there is no time reversal symmetry in R(m + n ) for n # m, since R ( m t n) and R ( n m) are different paths from each other, so that the $
+
152
CHAPTER 8. T ~ A ~ S P O RP T~ O P ~ ~ T ~ E
reflection probability becomes 21A1’. The coherence associated with Eq. (8.31) i s known as enhanced backward scattering, and can be applied to radar systems for searching a cloud which can be treated as a random material. When a magnetic field is applied, the phases of A and A” become different from one another. The phase difference is proportional to the magnetic flux penetrating through a loop made from a set of Ap and A?. However, since the lengths of the loops are different for different Ap’s, thus we can no longer expect any enhanced backward scattering, thus decreasing the reflection probability, This is an explanation of the origin of negative magnetoresistance under weak localization conditions. 8.2
Transport experiments on carbon nanotubes
In this section we discuss quantum transport in carbon nanotubes. Whereas Sect. 8.1, considers quantum transport in general, we start this section with a few comments about quantum transport in carbon nanotubes generally and then proceed to discuss specific experiments. Since the Fermi surface of a 1D nanotube consists of the two points f k p , scattering processes involve taking an electron from +CF to IF or visa versa. For an armchair nanotube this wouId involve a phonon of 47r/3T where T is the Iength of the 1D translation vector, whereas for zigzag nanotubes, phonon with wave vectors 2n/T are effective. Transverse acoustic (outofplane) phonons are most effective in this scattering process through the electronphonon interaction [78]. Transport, measurements of nanotubes show different aspects depending on the sample type, such as a singlewall nanotube (SWNT), a single rope (SWNT bundle), a single multiwall nanotube (MWNT) and a single MWNT bundle. The most difficult experimental problem for the transport experiments on carbon nanotubes is the attachment of electrodes to the extremely thin nanotubes, and this is discussed in Sect. 8.2.1. In the initial transport experiments on an individual carbon nanotube [184], rather large diameter (20 nm) multiwall nanotubes were used. Subsequently, single wall nanotubes became more available and the focus of research on the transport properties of carbon nanotubes shifted emphasis to the singlewall nanotubes, since singlewall nanotubes represent a model system for studies of q ~ a n t u mtransport, 51s discussed in Sect. 8.2.2, where transport properties for an isolated singlewall nanotube are presented.
8.2. TRANSPORT EXPERIMENTS ON CARBON NANOTUBES
153
This is followed by a report in Sect. 8.2.3 on transport in a single rope of singlewall carbon nanotubes where intertube interactions play a role. Phenomena associated with weak localization and universal conductance phenomena are observed in multiwall nanotubes and are discussed in Sect. 8.2.4. 8.21
Attaching Conlacis
We summarize here some of the techniques that have been used for attaching contacts t o carbon nanotubes for carrying out transport experiments [185], One method for attaching contacts t,o an n a n o t u b ~is to place a liquid drop, containing suspended nanotubes, on a substrate on which electrodes were previously deposited. For those nanotubes which connect two electrodes, transport me* surements can be carried out [150,151]. In another version of this method, a single contact is made with this technique and a scanning tunneling probe is used to make the second contact as this probe moves along the wire, continuously measuring the resista.nce as a function of nanotube length [186]. A third method involves the use of sophisticated semiconductor Si technology to attach 4 tungsten leads by a focused ion beam deposition technique, as seen in Fig. 8.3 for four contacts attached to a multiwall nanotube in the 510 nm diameter range on an oxidized silicon surface [185]. The 80 nm wide tungsten wire contacts are deposited by focusedionbeam induced deposition using a W(CO)6 carrier gas, The nanotube is visualized by the focusedionbeam with a low beam current (4 PA) for imaging the nanotube. The deposition of the contacts is performed under computer control without any visualization. The distance between the probing leads on the sample is in the 0.31.0 pm range. The four Leads are connected to a gold pad and the currents a.nd voltages are observed by a fourpoint contact measurement. The advantages of this method is that 4 contacts can be placed reliable on the single nanotube. The effect of strain introduced by lead attachment process is not understood. Another approach for making electrical contact, that utilizes so of the techniques mentioned above, is seen in Fig. 8.4 where the carbon nanotube is placed on top of a Si/SiOz substrate on which two P t electrodes had previously been deposited. This method has the advantage of perturbing the nanotube only weakly, but has the disadvantage of a high contact resistance and of not providing four contacts
154
CHAPTER 8. TRANSPORT PROPERTIES
Fig. 8.3: An individual multiwall carbon nanotube connected to four 80 nm wide tungsten wires by focused,ionbeaminduced deposition [185].
Fig. 8.4: AFM tappingmode image of a carbon nanotube on top of a Si/SiOz substrate with two 15 nmthick and 140 nm wide Pt electrodes. A schematic circuit diagram is presented at the top of this figure and is relevant to the transport experiments shown in Fig. 8.5 [51]. 8.2.2 APLI ~ ~ z Siszgle~ %Wall ~ ~~ a ~~
~
t
~
~
e
We now discuss experimental results from the first transport experiment on an individual isolated singlewall carbon nanotube [51]. In this experiment a single wail nanotube (the very thin wire in Fig. 8.4) is placed on top of a Si/SiOz substrate with two 15 nmthick and 140 nm wide P t electrodes as shown in Fig. 8.4 [51] and the bias voltage vbiw is measured between the two electrodes. A gate voltage Vgate, applied to the third electrode in the upperleft hand corner of Fig. 8.4 is used to change the electrostatic potential seen by the nanotube. The bias voltage v b i a changes the chemical potentials of the two electrodes, p1 and pz (see Fig. 8.1), while the gate voltage Vgatechanges the position of the energy levels of nanotube relative to the chemical potentials, p1 and pz, Because
8.2. TRANSPORT EXPERIMENTS ON CARBON NANOTUBES
155
Fig. 8.5: a. Currentvoltage curves of a carbon nanotube at a gate voltage of 88.2 mV (curve A), 104.1 mV (curve B) and 120.0 mV (curve C). In the inset, more I  vbim curves are shown with, ,V ranging from 50mV (bottom curve) to 136 mV (top curve). b. Current versus gate voltage at vbim = 3 0 p V . The two traces were performed under the same conditions and represent a bistability (see text) [51]. of the finite length of the nanotube ( L =3 pm), the onedimensional energy band is split into energy levels whose spacing AE = h v ~ / 2 Lis estimated t o be AE 0.6 meV, where we use an estimate for the Fermi velocity of VF = 8.1 x 105 m/s. The t w ~ p o i nresistance t at roomtemperature of such a single wall nanotube is 1 Ma. The estimated contact resistance, obtained from a similar nanotube on which a fourpoint contact geometry was used, is 300kSZ at room temperature and 1MS2 at 4 K. In Fig. 8.5a, we show the I vbia curves at a gate voltage of 88.2 mV (curve A), 104.1 mV (curve B) and 120.0 mV (curve C ) at 5 mK. The plateaus of nonzero current clearly show ballistic transport when a conducting channef is in the range of vbim = ( p l p Z ) / e . The position of the steps in the I vbim curves is changed by increasing the gate voltage, However, we must consider not only the level shift effect but also the Coulomb charging effect of the nanotube, whereby, the nanotube is considered as a capacitor with a capacitance C. At very low temperature, such that the thermal energy k g T is smaller than the charging energy E, of an electron k g T < E, = e 2/2C, the current Aow can be blocked by this energy shift when the charge from the current flow itself shifts the levels out of the bias window between p 1 and p 2 . Thus, current Row in Fig. 8.5b appears only when him> E,. Since the energy of the levels in a nanotube can be modified by Vgate, the step positions shown in the inset of Fig. 8.5a are N
N



CHAPTER 8. TRANSPORT PROPERTIES
156
0.08
5 "k
0.04
8
0.02
P 4P
0.00
3
2
1
0
1
2
3
AVgeie (mV)
Fig. 8.6: Conductance G = I/vbi, vs AVgate at the bias voltage vbim for three different temperatures with the bias window vbias = 1OpV. The solid lines represent fits to the function G 0: ~ o s h  ~ ( e A V , , ~ , / a 2 k ~ T )Left . inset shows a model for explaining the temperature dependence of G. Right inset shows the current vs gate voltage for vbim = 0.4,0.8,1.2 and 1.6 m v , showing the contribution from the lowerlying levels within the bias window [51].
smoothly changed by changing Vgate. When the bias window denoted by vbjm is very narrow ( 3 0 p V ) , the current flow appears like a delta function of Vgate,only when the energy levels are in the bias window between p1 and p2, as shown in Fig. 8.5b. Some double &functions are also observed in the two traces in Fig. 8.5b, which are taken under the same experimental conditions. This bistability may be explained as the result of switching offset charges that shift the energy levels of the 1D carbon nanotube. Figure 8.6 shows the temperature dependence of the spectra of a sharp peak that is observed in Fig. 8.5b, as a function of the gate voltage shift AV,,,, from the peak conductance point, with the minimum bias window vbim = 1OpV. A decrease in intensity and a broadening of the conductance peak with increasing temperature shows the relaxation of the phase and amplitude of the resonance tunneling by phonon scattering events. Solid lines in Fig. 8.6 are fitted to the function G 0: ~ o s h  ~ ( e A v ~ , ~ , / 2 a k B Twhere ), the factor a = 16 obtained from Fig. 8.6 is the ratio of AVgate to the shift of the energy levels. This ratio corre
8.2. TRANSPORT ~ X P ~ R I ~ E N ON T CARBON S ~ A ~ ~ T U ~ 157 E S
sponds t o the ratio of the capacitance of the gate to that of the nanotube. The temperatures in Fig. 8.6 (110, 390, and 830 mK) are the fitted temperatures for the plotted curves, while the measured temperatures are 5 , 240, and 600 mK, respectively. The discrepancy between the fitted and the observed temperatures is due t o the finite bias voltage (10pV = 116 K) and the residual noise in the measurement system. Although the absolute value of conductance is ff0.03(2e2/~), the quantum conductance 2e2fh could be obtained at a smaller bias voltage. If the conductance is observed with a smaller bias voltage and a larger ct. value, the conductance of Fig. 8.6 wiil show saturation at 2 e 2 / h , thus providing clear evidence for quantum c o n d u c t ~ c e . When the gate voltage increases (see the right inset of Fig. 8.6}, step structures are observed. For curves at high gate voltages (about 140mV) plateaus can be seen for different values of Vim. The plateaus correspond to the entry of a state at the Fermi level (denoted by the solid line in the left inset of Fig. 8.6) into the bias window. When we further decrease Vgater the next plateau appears and is attributed t o conduction processes associated with the lower level below A E 0.4 meV (see the left inset of Fig. 8.61, which is consistent with the estimated level spacing of AE 0.6 meV for a L =3pm nanotube. A value of a = 1 2 is estimated for the data in Fig. 8.6 from the ratio of AV,,, to AE. This value of a = 1 2 is in satisfactory agreement with the previous value of ~ ~ in 1 the first approximation. The further decrease of Vgatebrings the system back to a no current situation, since the state at the Fermi level is now located outside of the bias window, These results are consistent with the fact that the curves in Fig. 8.6 with a larger bias window vbim show a signal within a larger range of


Vgate *
The experiments, described in Figs. 8.4, 8.5 and 8.6, dearly show ballistic transport effects associated with the discrete levels imposed by the finite length of the onedimensional nanotube conductor. The observed phenomena can be understood by steps in the quantum conductance, and charging effects amociated with the micro capacitances of the nanotube and the gate. The resistance measurements for various nanotube samples show that there are metallic and semiconducting nanotubes, which was first predicted theoretically, as discussed in Sect. 4.1. The resistivity is about 104103 Qcm for the metallic nanotubes, while the room temperature resistivity is about 10' Qcm in semiconducting nanotubes. The semiconducting nanotubes exhibit a slope
6
CHAPTER 8. TRANSPORT PROPERTIES
158
40
20
a E.0 h
20
4 0  6  5 4  3  2  1
0
1
2
3
4
5
6
v (mY Fig. 8.7: I  V characteristics of a single 12nmdiameter rope made up about 60 1.4nmdiameter nanotubes at different temperatures for the rope segment between contacts between 2 and 3 (Left inset). In the right inset shows schematic energy levels near Fermi energy which are quantized because of the finite length of tube. [l87] in a plot of logR versus 1/T, thereby indicating an energy gap in the range 0.10.3 eV, which is consistent with the theoretical values of the energy gap for the corresponding nanotube diameters. On the other hand, for the metallic nanotubes, large variations from sample to sample are observed in the absolute values of the resistance and in its temperature dependence from 4 K to 300 K. This variation has been attributed to the presence of many defects in ~ u l t i  w a l ~ carbon nanotubes. Since the nanotube sample shows a slight positive magnetoresistance, the sample may contain a large number of defects, which seriously affect the measured conductance.
8.2.3 An I n d ~ v ~ d uRope a l of Single Wall ~ ~ n o ~ ~ b e ~ Next we show transport results from a single 12nmdiameter rope containing about 60 SWNTs of 1.4 nmdiameter [187]. In Fig. 8.7, the currentvoltage characteristics are shown for the rope segment between contacts between 2 and 3 (Left inset). At room temperature, the I V characteristics gives Ohmic behavior, while the conductance is suppressed near V = 0 for T < 10K. A similar

8.2. TRANSPORT EXPERIMENTS ON CARBON NANOTUBES
€59
Fig. 8.8: Resistance R(T) of a bundle of muitiwall nanotubes as a function of temperature at the indicated magnetic field values. The temperaturedependent resistance R(T) shows three kinds of temperature regimes (see text [150]. gap is obtained by other single ropes with different diameters and lengths [187]. From Fig. 8.7, we see that the resistivity decreases with increasing temperature, and this is not typical metallic behavior. In another experiment on a single rope, about a €O% increase of the resistivity was reported from 50 K to 280 K [l88], while a decrease in the resistivity with increasing T was found bejow 50 K. A negative with a dependence of pfT) was even found in the higher temperature region when a single rope has a disordered nanotube alignment. The reasons for these temperaturedependent trends are not explained. It is believed that the transport between singlewall nanotubes in a rope makes an essential contribution to the current at low temperatures.

8.2.4
~~~~~
Magneto Transport in Mu&&Wall Nanotubes
One of the early transport experiments on multiwall nanotube bundles with 50 nm diameter showed a negative magnetoresistance. In Fig. 8.8 we show the resistance of a bundle of multiwall nanotubes as a function of temperature at several values of the magnetic field (4 T, 7 T, I1 T, and 14 T) 21501. LFrorn
160
CHAPTER 8. TRANSPORT PROPERTIES
the figure we can see three kinds of temperature regimes denoted I, 11, and 111. In the higher temperature regime I, the resistance continuously increases with decreasing temperature. These phenomena were accounted for using a simple twoband semimetal model [189] for the electron and hole concentrations n and p as a function of temperature T,and a value of 3.7 meV for the band overlap, which is much smaller than A == 40 meV in 3D graphite [190]. Since the interlayer interaction in the multiwall nanotube is incommensurate, as discussed in Section 11.4, the band overlap can be expected to be much smaller, which is consistent with the smaller value of A in the small diameter nanotubes. In the temperature regime 11, the resistance is almost independent of temperature and has a value of loe2 to $2cm, thereby suggesting a conducting nature of carbon nanotube bundles. In the temperature regime 111, a peak in the resistance is observed whose origin may relate to possible ordered states induced by lowering the symmetry. By lowering the temperature, the resistance quickly decreases. In the low temperature regime below 77 K, a relatively small negative magnetoresistance A R / R = [R(H)R(O)]/R(O) < 0.1 is observed with I? normal to the tube axis. There are at least two possible reasons for the observed negative magnetoresistance. One explanation is the effect of weak localization, as discussed in the previous section. However, weak locatization effects are expected to occur at much lower temperatures. The other possible reason is associated with Landau level formation at the Fermi level. As shown in Chapter 6, the n = 0th Landau level in two dimension~lgraphite always appears at the Fermi energy, and the density of states increases with increasing magnetic fieid, reflecting the degeneracy of the Landau orbits. This enhancement of the density of states at the Fermi Level contributee to an increase in the current path and thus is expected to give rise to a negative magnetoresistance. Thus the negative magnetoresi~tanceabove 4 K may be associated with a Landaulevel effect (called the Bright model 11911). In the very low temperature region below 1 K , the negative magnetoresistance shows relatively large values of A R / R as shown in Fig. 8.9 [150]. In the figure, the magnetoresistance shows the same magnetic field dependence at 2.3 K and 1.13 K. However below 1 K , the magnetoresistance becomes quite large (up to A R / R = 0.3), which is a typical value for the magnetoresistance in the weaklylocalized regime [192],The phase delocalization length L , increases
8.2. TRANSPORT EXPERIMENTS ON CARBON NANOTUBES
161
0 Q.OJ 0. I
Fig. 8.9: Magnetoresistance A R / R as a function of magnetic field at low temperatures below 1 K. The data are taken on the same multiwall carbon nanotube as in Fig. 8.8 [150].
Q.15 0.2 .O.U
4.3
I
I
0
r.ao6] L
2
4
6

I
.
0
8
10
12
Magnetic Field PI
14
18
Fig. 8.10: Magnetic field dependence of the magnetoresistance of a 20 n m multiwall carbon nanotube at the indicated temperatures. The fluctuations in resistance that are observed at the same values of magnetic field at different temperatures are known as universal conductance fluctuations [184].
with decreasing temperature so that the loop of phase difference discussed in the previous section becomes large even for small magnetic fields. Thus a negative magnetoresistance effect is observed in carbon nanotubes at lower magnetic fields than is usually found in graphite. At the lowest temperature of 0.3 K in Fig. 8.9 a saturation of A R / R is observed at large magnetic fields. These data show a complete quenching of the enhanced backscattering. It is interesting that the negative magnetoresistance phenomena occur below that temperature. In Fig. 8.10 the magnetoresistance for a 20 nm multiwall nanotube at very low temperature is presented as a function of the magnetic field. Clearly the magnetoresistance is seen to fluctuate randomly by varying the magnetic field. However the peaks in the magnetoresistance for different temperatures appear at the same value of the magnetic field. Thus the fluctuations in the magnetoresistance are not associated with noise but rather are due to a quantum interference effect known as universal conductance fluctuations, which is discussed in Sect. 8.1.4. By applying an external magnetic field, the carrier scattering
CHAPTER 8. TRANSPORT PROPERTIES
162
processes are changed, thus having the same effect on the magnetoresistance as is observed in Fig 8.10. The effect of variation of the magnetic field is the same as the fluctuations in the conductance that would be observed from sample t o sample. The amplitudes of the two indicated fluctuations in Fig 8.10 are constant in magnitude below 0.4 K , AG = O.lGo, where Go = 2 e 2 / h is the quantum conductance [see Eq. (8.7)], showing that the multiwaI~carbon nanotube consists of N 5 serial quantum wires of length L,. The amplitude of the fluctuation is constant below 0.4 K and decreases as T1I2 above 0.4 K, consistent with Eq. (8.301, from which we can estimate t , = 2 x sec.

CHAPTER 9.
Phonon Modes of Carbon Nanotubes
The phonon dispersion relations of carbon nanotubes can be understood by zone fold~ngthe phonon dispersion curves for a single 2D graphene sheet. In Sec. 9.1 and See, 9.2, we first explain how to calculate phonon dispersion relations in twodimensional graphite. Then we discuss phonon dispersion relations for carbon nanotubes in See. 9.3. The r onefolding technique is the same as that used in treating the electronic structure of carbon nanotubes, which is discussed in Sec. 4.1.1. We also consider the threedimensional dynamical matrix, taking the curvature of the nanotubes into account, and obtain results for the phonon dispersion relations. 9.1
Dynamical matrix for phonon dispersion relations
We start with an approach for calculating the phonon dispersion relations within a force constant model, in which interatomic forces are represented by spring constants. Although the model is simple, we can reproduce the experimental results as closely as possible by increasing the number of the force constants. In general, the equation of motion for the displacement of the ith coordinate, ui = ( 2 1 , yi,zi) for N atoms in the unit cell is given by
Miiii =
IW(uj
Ui),
(i = 1 , .. . ,N ) ,
(9.1)
j
where Mi is the mass of the ith atom and Id”) represents the 3 x 3 force constant tensor* between the ith and the jthatoms. The sum over j in Eq. (9.l),
..
*A second rank tensor is defined by a 3 x 3 matrix whose elements ( K z s , KzY, ., K z z ) can be transformed as Ulh’U, where U is a unitary matrix which transforms the x , y, t coordinates into another orthogonal r’,y’, z’ coordinate system.
163
is normally taken over only a few neighbor distances relative to the ith site, which for a 2D graphene sheet has been carried out up to 4th nearestneighbor interactions [193]. In a periodic system we can perform a Fourier transform of the displacement of the ith atom with the wave number, Ic’, to obtain the normal mode displacements
ui’
where the sum is taken over all ( N n ) the wave vectors k’ in the first Brillouin zone+ and Ri denotes the original position of the ith atom. When we assume the same eigenfrequencies w for all ui,that is ui =  w 2 u j , then Eq. (9.1) becomes
C
I

+
+
172
CHAPTER 9. PHONON MODES OF CARBON NANOTUBES
dispersion relations for the x , g, and z v~brationsfor each atom are foIded into the onedimensional Brillouin zone of a carbon nanotube along the K2 direction (Eq. (3.20) ). The phonon dispersion relations of a carbon nanotube also depend on the chirality (n,M ) and diameter of the carbon nanotube, d t , since the phonon wave vector in the circumferential direction becomes discrete for every K1 vector [see Eqs. (3.20) and (4.1)], in accordance with the periodic boundary conditions of the chiral vector. The corresponding onedimensional phonon energy dispersion relation wyg (k) for the nanotubes is given by,
where wrD (lc) denotes the twodimensiona~ energy dispersion relations for a graphene sheet, k is a onedimensional wave vector, and T is the m a ~ n i t u d e of the onedimensional translation vector T given in Eq. (3.8). The idea of zone folding is applicable for almost all the phonon modes of a carbon nanotube. However, it has been pointed out [193] that zonefolding alone does not always give the correct dispersion relation for a carbon nanotube, especially in the low frequency region, and some additional physical concepts must be introduced. For example, the outofplane tangential acoustic (TA) modes of a graphene sheet shown in Fig. 9.5(a) on the left do not give zero energy at the r point when rolled into a nanotube as shown on the right. Here, at k = 0, all the carbon atoms of the nanotube move radially in an outofplane radial acoustic vibration, which corresponds to a breathing mode with nonzero frequency f1931 as shown in Fig. 9.5(a) on the right. In the breathing mode, only the inplane force constants, 4, and dti* in the ~ i ~ c u ~ f e r e n tdjrection ial of the tube are related t o the vibration, and this results in a finite frequency at the I? point. On the other hand, when we consider the vibrations of a carbon nanotube in the context of threedimensional space, we generally expect three acoustic modes which correspond to vibrational motions in the 2 ,y, L directions. However, the two directions which are perpendicular to the nanotube axis do not correspond ‘Since there is no vibration in the direction of the nanotube axis in the breathing mode, the bond angle of the hexagon network is modified. Thus the force constant &i is necessary to describe the breathing mode.
9.3. PHONON DISPERSION RELATIONS FOR ~ A ~ O T U ~ E S
173
Fig. 9.5: (a) The outofplane tangential acoustic modes at Ic = 0 (left) in a single layer of graphite give rise to a radial breathing mode in the carbon nanotube with nonzero frequency (right). (b) An acoustic mode of a carbon nanotube whose vibration is perpendicular to the nanotube axis (right) corresponds to a linear comb~nationof both inplane and outofplane graphitederived modes (left). These modes do not couple in the case of a single graphite layer, but do couple for the nanotube because of the curvature that is introduced by rolling up the sheet.
to any tw5dimens~onalg r ~ p h i t ephonon modes. In a graphene sheet, the inplane and outofplane modes are decoupled from each other. However, when the graphene strip is rolled up into a nanotube, the graphitederived inplane and outofplane modes do couple to each other, as shown on the lefthand side of Fig. 9.5(b), to form the acoustic mode of the nanotube shown on the right. 9.3.2 Force constant tensor of a carbon nanotube
In order to avoid these difficulties, we solve the threedimensional carbon nanotube dynamical matrix problem directly using the force constant parameters
174
CHAPTER 9. PHONON MODES OF CARBON NANOTUBES
listed in Table 9.1. Since we have 2N carbon atoms, the dynamic matrix to be solved becomes a 6 N x 6 N matrix. Here we denote the 2 N atoms as Ai and B j ( i , j = 1, + ,.N ) , where the N Ai (or N B j ) atoms are geometrically equivalent to each other, as discussed in 3.4. In fact, the position of each Ap (or Bp) atom can be obtained by operation of the symmetry vector R defined in Eq.(3.10) p  1 times on A1 (or B l ) : +
A1

RP1
Ap,
and
B1

RP 1
Bp,
( p = l , . . . , N .)
(9.14)
When we divide the big 6N x 6N dynamical matrix into the 3 x 3 small matrices V ( A i B j for ) a pair of Ai and B j atoms, we then consider (2N)' = 4 N 2 small matrices, ; D ( A i A j ) , ; D ( A i B j ) , ;D(BiAj), and V ( B i B j )( ,i , j = 1 , . . . , N ) . WheIl a pair (ApBq), (or (ApAq), (BpAq), (BpBq))are within the 4th neighbor distance, we will consider V(ApBq).The corresponding force constant tensor I d A p B q ) is calculated using
where U is a unitary matrix for rotation by an angle I = 2 r / N around the nanotube axis. Then UP' is defined in Eq. (3.16) as
UP'
=
cos(p  1 ) I sin(p  1 ) I 0 sin(p 1 ) I cos(p 1 ) I o ( 0 0 1
1
,
+
(9.16)
where the z axis is taken for the nanotube axis. When ( q  p 1) is negative or zero in Eq. (9.15), we use ( N q  p 1) for ( q  p 1). Thus we can generate all force constant tensors from the nonzero tensor related to A1 or B1. When we consider I d A l B p ) or IdBIBJ'), the effect of the curvature has been taken into account. For example, let us consider the case of (see Fig. 9.6). When we put atom A1 on the z axis, is obtained by: (a) rotating the tensor of Eq. (9.9) by (7r/6)  0 around the z axis, then (b) rotating the tensor by an angle (p/2 around the z axis, and finally (c) rotating by I around the z axis. Here the angles 0, 'p and I are, respectively, the chiral angle 0 defined in Eq. (3.4), the angle (o between A1 and B1 around the z axis, and the angle 9 between A1 and A p around the z axis defined by 2 ( p  l ) n / N in Eq. (3.4), as shown in Fig. 9.6 (a), (b) and (c), respectively.
+
+
+
Y l i )
5 fl
Fig. 9.6: The geometry of the A1 atom and its nearest neighbor atoms, B1, Bi,B j . The force constant tensor is obtained by (a) rotating the tensor of Eq. (9.9) by ( n / 6 )  8 around the z axis and by (b) rotating the force constant tensor by an angle rgf2 around the z axis. Here B is the chiral angle defined in Eq. (3.4), and the angle yo is defined in this figure by the angle between A1 and €31 in the xy plane around the z axis. The upper open circle in (a) represents the projection of B1 on the yz plane and the lower open circle represents its location after rotation by n/6  B on a 2D graphene plane. For II(APBq), we further rotate in (c) the force constant tensor by 9 around the z axis (see Eq. (9.16)).
Using the force constant tensor thus obtained and multiplying by exp ikAzij, where Azij is the component of Al&j along the z or nanotube axis, the dynamical matrix for a Ic vector is obtained. The phonon energy dispersion relation is determined by solving the dynamical matrix for many k points in the onedimensional Brillouin zone. The results thus obtained for w(lc) for a (l0,lO) armchair carbon nanotube e the unit vector along are given in Fig. 9.7(a), where T denotes the ~ a g n i t u d of the tube axis (see Eq. (3.5)). For the 2N = 40 carbon atoms per circumferential strip for the (10,lO) nanotube, we have 120 vibrational degrees of freedom, but because of mode degeneracies there are only 66 distinct phonon branches, of which 12 modes are nondegenerate and 54 are doubly degenerate. The number of distinct phonon branches can be obtained by point group theory for atoms
176
CHAPTER 9. PHONON MODES OF CARBON NANOTUBES
1600 1200
aoo 400
n
0.0 0.2 0.4 0.6 0.8 1.0 0.0 kT/
'IC
1. 1x10*
states/l Catom/cm'
Fig. 9.7: (a) The calculated phonon dispersion relations of an armchair carbon nanotube with c h = (10,lO). The number of degrees of freedom is 120 and the number of distinct phonon branches is 66. (b) Phonon density of states of (10,lO) nanotubes.
in the unit cell. In the case of the (10,lO) armchair nanotube, D l o h is the point symmetry group, and the direct product of the reducible representation for the atomic sites* with the representations for 2 , y , z is decomposed into the irreducible representations for the phonon modes. In Fig. 9.7(b) we show the phonon density of states for the (10,lO) nanotube in units of states per C atom per cml. When we integrate the phonon density of states with respect to the energy, we get 3 states/Catom as the total number of states. Since we use the same units for the phonon density of states for 2D graphite [see Fig. 9.4(b)], we can directly compare the phonon density of states for the (10,lO) nanotube and for 2D graphite. The phonon density of states for the (10,lO) nanotube is close to that for 2D graphite [see Fig. 9.4(b)] since the phonon dispersion relations are, in principle, given by the zonefolding of *The character of the atomic sites for an operation 0 of the point group is defined by the number of atoms which do not change their position when the operation 0 is carried out.
9.3. P ~ O N O N~
~
S
P RELATIONS ~ ~ ~ OFOR N NANOTUBES
200

'6
100
Ll
3
0
0.0
0.2
kT/a
0.4
177
Fig. 9.8: Phonon dispersion relations of the (10,lO) armchair carbon nanotube near the I' point. The three lines near w = 0 which intersect at k = 0 correspond to the acoustic modes of a carbon nanotube. There are four acoustic modes in this cylindrical solid, including the lower energy 2,y transverse acoustic modes (TA, doubly degenerate), the z longitudinal acoustic mode (LA), and the twisting mode (TW). The TW mode is related to the rotation of a nanotube along its axis.
those for 2D graphite. The difference in the phonon densities of states appear in the small peaks due to the onedimensional van Hove singularities. It is noted that we integrated the phonon states within an accuracy of 10 cml. Another difference between the (10,lO) nanotube and graphite relates to the phonon density of states at w = 0 cm'. Since there is k 2 dependence in the outofplane TA mode for 2D graphite, we get a finite density of states at w = 0 cml, which is known as the twodimensional van Hove singu~arityat the band edge. However, since all acoustic modes of the (10,lO) nanotube have a k dependence as shown below, we have no phonon density states at w = 0 as shown in Fig. 9.7(b). Let us focus our attention on the acoustic modes of the (10,lO) carbon nanotube. In Fig. 9.8, the phonon dispersion curves around the J? point are shown on an expanded scale for the (10,lO) carbon nanotube. The lowest energy modes are the transverse acoustic (TA) modes, which are doubly degenerate, and have 2 and y vibrations perpendicular to the nanotube ( z ) axis (see Fig. 9.5(b) right). The highest energy mode is the longitudinal acoustic (LA) mode in the direction of the nanotube axis. Since the djsplacements of all the acoustic modes are three dimensional, the frequencies of the phonon dispersion relations are proportional to k for all three phonon branches, as is commonly observed in the solid state. The corresponding phonon density of states is proportional to
178
CHAPTER 9. PHONON MODES OF CARBON NANOTUBES
the energy while the phonon density of states of 2D graphite is constant because of the k2 dispersion relation for the outofplane TA graphite mode. The sound velocities of the TA and LA phonons for a (l0,lO) armchair carbon nanotube are estimated as 9.43 km/s and 20.35 km/s, respectively.? These results cannot be obtained by the zonefolding method discussed in the previous subsection, since the sound velocity for the zonefolded outofplane TA mode is zero because of the k2 dependence as discussed above. In addition, there is a fourth acoustic mode for the carbon nanotube, which is related t o a rotation around the nanotube axis at k = 0. When we consider a single carbon nanotube as an infinite onedimensional material, a rotation around the nanotube axis is possible [83,196]. Since the driving force for this wave motion is a twisting motion of the nanotube, we call this mode a twisting mode (TW). The sound velocity of the T W mode is 15.00 km/s, which is the same as the calculated value of the inplane TA mode for 2D graphite. The reason why the T W modes have the same velocity as the TA graphite mode is that the displacements associated with the T W mode are in the cylindrical plane and are perpendicular to the tubular axis. It is noted that the sound velocities that we have calculated for 2D graphite are similar t o those observed in 3D graphite [9], for which = 12.3 km/s and vgjD = 21.0 km/s. The difference of the sound velocity is due to the existence or absence of the interlayer interaction between graphene layers for 3D graphite and a 2D graphene sheet, respectively.
vgiD
9.9.9
Force constant corrections due to curvature of 1D nanotubes
The threedimensional phonon dispersion relations of a carbon nanotube can be obtained by the methods discussed in the previous subsection. However it should be mentioned that the force constant parameters of Table 9.1 are not well defined on the curved surface of the nanotube by merely considering the planar graphene force constants.
fi,
'u = in which p is the density of carbon atoms. When we assume the triangular lattice of the nanotubes ( s o called rope) with the lattice constants of a =16.95A and c =1.44x&A, the density p becomes 1.28 x lo3 kg/m3 from which the Young modulus gives Y = 532 GPa. This value is smaller than other calculated Y values. This small Y value arises from the small mass density of the rope. Details will be discussed in Chapter 11 on elastic constants.
tThe Young modulus, Y can be estimated by the LA velocity,
9.3. PHONON DISPERSION RELATIONS FOR NANOTUBES
179
For example, in Fig. 9.9, we show the effect of the rotational motion of the twisting mode with k = 0 on the cross section of the carbon nanotube in which all vectors of the motion should be parallel to the cylindricaI surface and perpendicular to the nanotube axis. It is a physical requirement that we have a rotational mode with w = 0 at k = 0 in this system. However, the calculated result for the (10,lO) carbon nanotube gives a finite value of w = 4 cm' at k = 0 for the twisting mode when we use the method of the previous subsection with the force constant parameters of Table 9.1. The other three acoustic modes correctly give w = 0 cmI at k = 0. When we denote a nearestneighbor bond as the dotted line in Fig. 9.9, the two vectors u and G u are not in the plane which is defined by the dotted line and tube axis. Thus, for this kind of rotational motion, the force associated with the tangential outofplane force constant, 4to artificially introduces a force on the motion, which gives a nonzero value of w at k = 0. Actually when we examine the eigenvectors of the motion, we can find a small radial component of the motion which is perpendicular to the cylindrical surface and is due to the effect of curvature on the force constant parameters. The ratio of the components of the motion in the radial direction to the cylindrical direction is on the order of The curvature effect will also apply to all of the other modes by an amount up to ~ 1 cm' 0 even for the (5,5) armchair nanotube. Thus as a first approximation, this effect can be neglected compared with general nanotube phonon frequencies which are on the order of lo3 cml. In order to treat the curvature effect correctly with the given force constant parameters of twodimensional graphite, we could consider the dynamical matrix on a curved coordinate reflecting the cylindrical surface, which would mix the force constant parameters with each other depending on the curvature and the bond length. This p h en o ~ en o ncan be treated by elasticity theory for a thin film, However this treatment requires a different method from that used for a lattice of springs. When we consider a curved chemical bond, we find that the force constant parameters in Table 9.1 cannot be applicable to the curved coordinates. Actually the calculated results using the force constant parameters in Table 9.1 give less accurate values than the approach of the previous subsection. Sometimes the calculated results even give imaginary (i.e., negative w 2 ) frequencies for the acoustic phonon modes. Thus we do not use the elasticity theory approach to the curved coordinates of carbon nanotubes.
180
CHAPTER 9. PHONON MODES OF CARBON NANOTUBES
Fig. 9.9: The dependence of the twisting mode at k = 0 of a carbon nanotube on its cross section is shown. When we consider the interaction between the two atoms along the dotted line, the rotational motion appears to have a tangential outofplane motion in the plane defined by the dotted line and the nanotube axis.
x
Y
Fig. 9.10: (a) Correction of the force constant #do, which is given by Eq. (9.17) and (b) correction of the force constants of 4,. and &, which are given by Eqs. (9.18) and (9.19). Figure (a) illustrates the section of a plane perpendicular to the nanotube axis, and (b) illustrates a plane corresponding to an unrolled graphite sheet.
To avoid the difficulty of the curved coordinates, we have proposed the following approximation in which the force constants are scaled depending on their bond lengths. When we consider the tangential outofplane mode for the ith site on the cylindrical surface as shown in Fig. 9.10 (a)zthe motion is in the direction perpendicular to the cylindrical surface. On the other hand, when we denote the bond ij by the thick line, whose subtended angle around the tube
9.3. PHONON DISPERSION RELATIONS FOR NANOTUBES
181
axis is p as shown in Fig. 9.10(a), the tangential outofplane direction for that bond is defined to be perpendicular to that bond. The difference between the two directions is the angle 912 which depends on the bond length. When the bond length is large, the correction for the force constant becomes large, but not so large as the origina~force co n st~ n t.Here we scale the force constant #to by
do= 4 t o + d t o (1  cos (;)
(9.17)
as an empirical correction for the force constant. A justification for the correction of Eq. (9.17) is as follows. When we calculate the motion using the tangential outofplane dto force constant for a given bond, the Component of the force constant in the direction perpendicular t o the cylindrical surface becomes 4 ~ o c o s ( ~ / Z )In . order to obtain the same amplitude of the motion in this direction as is obtained in the case of twodimensional graphite, we add #bo(l  cos(cp/2)) to #to.* The correction of Eq. (9.17) becomes relatively large with increasing bond length or increasing p, which reIates to the corresponding bond length becoming shorter than that in a twodimensional graphite plane. Thus this bond ~e ngthdependent correction is used to describe the v~brations perpendicular to the cylindrical surface. Similarly, the force constants of 4Sp., #ti are corrected by the following formulae, respectively,
4; = #r
+ 4, cos (5 Q)
(1  cos
(~)),
(9.18)
and (9.19) where n/64 is the angle of the bond from the horizontal zy plane [see Figs. 9.10 (b) and 9.6 (a)]. Since we consider only the horizontal component of the force by a rotation of 9/2 around the z axis, we conclude that 4, cos(n/6 0) and sin(a/6  4) are the components to be corrected. Using the scaled force constants, we calculate an improved version of the phonon dispersion relations for a (10,10) armchair carbon nanotube. In this case, the frequency of the twisting mode becomes very small (Iwl < cml)

*We could also consider other corrections of the force constant, such as r#~t,/cos(cp/2). For small cp, this correction gives the same effect.as that of Eq. (9.17). However, this correction diverges at 'p = R, and thus we do not adopt it.
182
CHAPTER 9. PHONON MODES OF CARBON NANOTUBES
at k = 0. As for the other modes, the corrections are generally small (less than 5 cml). The only mode where the correction is significant is the E2, mode which gives a large softening after this correction from 22 cm' to 17 cml. It is interesting to note that the lowest phonon mode with nonzero energy at k = 0 is an Ezg mode in which the cross section of the carbon nanotube is vibrating with the symmetries corresponding to xy and x 2  y2. The calculated frequency of the E2, mode for the (10,lO) carbon nanotube is 17 cml. Since this mode is a Ramanactive mode and its frequency is sensitive to the radius of the carbon nanotube, the above arguments show the importance of investigating this mode experimentally. The observation of the Ramanactive modes, are discussed in the following chapter. Another important mode for experimental study is the Ramanactive low frequency breathing mode (Al, symmetry) shown in Fig. 9.5(a). The frequency of the breathing mode appears at 165 cm' for the (10,lO) armchair nanotube. This mode frequency quickly decreases to 0 cm' with increasing radius.
CHAPTER 10.
Raman Spectra of Carbon Nanotubes
The Ramanactive and infrareda.ctive phonon modes of carbon nanotubes are described on the basis of group theoretical arguments in Sect. 10.1, A review is given in Sect. 10.2 of Raman scattering experiments on purified s i n g ~ ~ w ananotubes li and arrays of carbon nanotubes, called ropes. To analyze the unique Raman spectra that are observed, results €rom bond polarization theory are presented in Sect. 10.3. The dependence of the Raman mode frequencies on the nanotube diameter is discussed in Sect. 10.4 and the dependence of the Raman mode ~ntensitieson nanotube orientatioii is discussed in Sect. 10.5. 10.2
Raman or infrared active modes of carbon nanotubes
Among the 6 N calculated phonon dispersion relations for carbon nanotubes whose unit cell contains 2N carbon atoms, only a few modes are Raman or infrared (IR) active, as specified by the symmetry of the phonon modes. Since only k vectors very close to k = 0 are coupled to the incident light because of the energymomentum conservation requirements for the photons and phonons, we need only consider the symmetry of the nanotube zonecenter vibrations at the I? point (k = 0). Point group theory of the unit cell, as discussed in Sect. 3.6, predicts the number of Ramanactive modes and IRactive modes. As discussed in Chapter 9, there are four acoustic modes including the rotation around the nanotube axis ( R z )at the I' point. Thus 6N4 optical phonons are considered in this section. The Raman and infrared(IR,)active modes correspond to modes whose irreducible representations transform as a quadratic form (z2 y2, z 2 , x2  y 2 , zy, yz and ).z for the Ramanactive modes, or as a vector form (8,y, and z ) for the infraredactive modes. The relationship between an
+
183
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
184
Table 10.1: Basis Functions for Point Groups Dnd and Numbers of Raman and IR Active modes. Basis functions D, CNfn Achiral Chid 9
".(
21
+Y 2 7 W zIR,
( x z ,Y2lR
 Y2r .YP
R,
("7y)IR
(RX,R,)
}
(2j,2j) 4 (0)
others
A A
(1)
4 (4)
El
EI
4(7)
6(5)
5(5)
E2
E2
2j
2j+1
A1
AI Az
Az
El
3
(n,m)
6 6 Total 6N4 16(6) 1 5 0 Numbers without and with parentheses denote the numbers of Raman and IR active modes, respectively. The superscripts and I R , respectively, denote Ramanactive and infraredactive modes. (x2
E2
8 16(7)
irreducible representation and its basis function is given in the character tables. In Table 10.1 are listed the basis functions for the irreducible representations of the carbon nanotubes and the number of Ramanactive modes for each irreducible representation. Each type of nanotube is classified by its symmetry. When we consider the nanotube axis to be in the t direction, the Raman modes whose vibrational amplitudes transform as t 2or z 2 y2 are invariant under any operation of the group, and therefore have A1 or A symmetry in the Dn or C , groups, respectively (see Section 3.6). The other Ramanactive modes belong to the El and E2 symmetry types, as shown in Table 10.1. In the case of the IRactive modes, the basis functions 2 and y are partners of a twofold degenerate mode with El ( E ) symmetry, and t transforms according to A2 ( A ) symmetry. If we know the irreducible representation of the calculated eigenfunctions of the phonon modes, we can directly assign the symmetries of the Ramanactive modes and IRactive modes among the 6 N  4 phonon modes. An eigenfiinction can be identified with an irreducible representation by applying a projection operator for the irreducible representation of the group to the phonon normal modes [197]. If the projected eigenfunction is not zero, the eigenfunction belongs to the corresponding irreducible representation. The numbers of the Ramanactive and IRactive modes for the solid can be predicted by group theory once the lattice structure and its symmetry are specified. The number of opticallyactive modes is calculated by the decomposition of the reducible representation of the vibration, Pib, which is given by the direct
+
10.1 RAMAN OR INFRARED ACTIVE MODES OF NANOTUBES
185
product of the two representations of the group as foilows (10.1)
where I'a.s. and rz,y,t are, respectively, the representations of the atomic sites for the equivalence transformation, and the irreducible representations which belong t o the vector components 2, y, z. The characters for I'a.s.are given by the number of atoms in the unit cell that remain invariant under an operation of the group. The representations which correspond to x$ y, z , are listed in Table 10.1 for the groups of nanotubes which are discussed in Section 3.6. When we into the irreducible representations of the group, using the ordecompose rvib t ~ o g o ~ i relations ~ ~ t y between the characters of the irreducible re ~ r e s ~ n ta tjo n s , the number of times an irreducible representation is contained in rvibis the number of phonon modes which belong to that irreducible representation. Since we know which irreducible representations correspond to the Ramanactive and IRactive modes, we can easily find the number of Raman and IR modes. If the z,y, A2,: z) and r ~ t a . t i o ~ (Az,: a 1 R,) motion be~ongto the t r a n ~ l a t i o ~(Elu: al and IR (Az,, El,) modes, we symmetry types of the Raman (Alg, E l g , subtract the number of those modes from the optically active modes in compiling Table l O . l . * The point group symmetries of armchair C h = ( n , n ) and zigzag Ch = (n,O) nanotubes are either Dnd or D n h , respectively, depending on whether n =odd or n =even, and the symmet~yof chiral nanotubes is the nonsymmorphic kbelian group CN,which is discussed in Sect. 3.6. From the as follows character Tables 3.4, 3.5 and 3.8, we get the decomposition of rvib 11981: for armchair nanotubes (even n = 2 j with Dnh symmetry)t
a,)
r$y = 4Aig + 2A1, + 4
4
+~242a~ + 2B1g
+ 2B2, + 4BzU + 4E1, + 8E1, + 8E2$ +4Ezu + * * * + 4 E ( j , l ) g +8E(jl)u $431,
(10.2)
*The symmetries are for achiral nanotubes. For chiral nanotubes, the symbols are as follows: transiational fE A ) , rotational ( A ) , Raman (A, E l , E2) and IR ( A , E l ) modes. tIn Eq. (10.2) we assume that j is even. If j is odd [such as for ( n , m )= (6,6)], the 4 and 8 are interchanged in the last two terms in Eq. (10.2).
+
186
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
(10.3)
For armchair and zigzag nanotubes (odd n = 2 j rvib zj+l
= 3Alg I 3A1,
+ 1 with D,d
3Azg
3A2,
+ 6E1, + 6E2g + 6Ezu + + 6Ejg + 6Eju
+6E1g
symmetry):
(10.4)
* ' '
For chiral nanotubes:
We list in Table 10.1 the numbers of Raman and IR active modes for achiral and chiral nanotubes in which the numbers without and with parentheses, respectively, refer t o the numbers of Raman and IRactive modes. Among achiral nanotubes, only armchair nanotubes with even number indexes (2j, 2j) have a different numbers of Raman and IR modes from others such as armchair nanotubes with odd number indexes ( 2 j 1 , 2 j 1) and zigzag nanotubes (n,O). From Table 10.1 we see that the numbers of Raman and infraredactive modes for a carbon nanotube do not depend much on the nanotube diameter and chirality, though the total number of phonon modes 6 N  4 is very different for different chiralities. Group theory selection rules indicate that there are 15 or 16 Ramanactive modes and 6 to 9 IRactive modes for a singlewall carbon nanotube. The difference between Dzj and Dzj+l for armchair nanotubes comes from the different numbers of El and Ez modes in the decomposition of rvibin Eqs. (10.2) and (10.4). Since the basis functions of achiralnanotubes consist of even ( 9 ) and odd ( u ) t functions, because of the existence of an inversion center, Raman and I R active
+
+
t The g and u come from the traditional notation of the German words 'gerade' and 'ungerade', respectively.
modes can be found for several different irreducible representat~ons. However for chiral nanotubes, modes with A and El symmetry are both Raman and IRactive, because of the lack of an inversion center. A phonon mode can be Raman and IR active simultaneously in the lower symmetry chiral nanotubes. However, in these cases the intense Raman modes are generally weak IR modes and vice versa. Even though group theory may indicate that a particular mode is Ramanactive, this mode may nevertheless have a small Raman cross section. In fact, we have only six or seven intense Ramanactive modes for any nanotube chirality, as shown in Sect. 10.3. Since similar eigenfunctions give similar Raman intensities for any kind of nanotube, the Raman spectra also have similar shapes, as shown by the calculations in Sect. 10.4.
10.2
Raman experiments on singlewall nanotubes
This section mainly describes Raman experiments on singlewall carbon nanotubes [52,83,99,199]. Most of the Raman studies on singlewall carbon nanotubes were made on nanotubes synthesized by the laser vaporization method [55] with transition metal catalysts, though similar results were obtained on singlewall nanotubes synthesized by the carbon arc method 1521. In both of these synthesis methods, the singlewall carbon nanotubes grow in a triangular lattice t o form a bundle or ‘rope’ containing 1050 nanotubes (see Sect. 5.2) [55,200]. Under some synthesis conditions, the (10,lO) armchair nanotube is the dominant species in the rope. However, in general, the Raman samples have a narrow distribution of diameters and chiralities, which depend sensitively on the catalysts that are used in the synthesis and the growth conditions, especially the growth temperature. For example, when 1.2 weight % of Ni/Co catalyst is used in the sample synthesis at a temperature of 1150OC in 500 torr Ar, the diameter range is 1.01.4 nm, while thinner nanotubes with diameters of 0.81.0 nm are obtained in the case of a 2.4% Rh/Pd catalyst with growth at llOO°C [99]. Even when the same catalysts are used, a higher growth temperature gives a larger diameter. This situation may be explained by the probability for generating a pentagon. When the temperature is lowered, the probability of closing a carbon pentagonal ring increases, and thus the caps that are generated tend to be smaller. At a higher temperature, however, atomic vibrations prevent the for
188
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
Fig. 10.1: Raman spectra (top) of the rope of single wall carbon nanotubes taken with 514.5 nm excitation at 2W/cm2. The features in the spectrum denoted by the symbol "*" are assigned to secondorder Raman scattering. The four bottom panels are the calculated Raman spectra for armchair ( n , n ) nanotubes, n = 8 t o 11. The arrows in the panels indicate the positions of the remaining weak, Ramanactive modes [83]. N
mation of relatively unstable pentagonal rings, compared with hexagonal rings, so the lower growth temperatures favor the growth of smaller diameter tubes. Among the 15 or 16 Ramanallowed zonecenter modes, the experiments show a few intense lines and several weaker lines, as illustrated in Fig. 10.1 [83]. The top panel of Fig. 10.1 shows Raman spectra for the singlewall nanotube rope using a laser excitation wavelength of 514.5 nm, and the lower panels show the calculated intensities for armchair nanotubes (n, n ) , n = 8 to 11, respectively. Between 1550 and 1600 cm', two strong features are observed at 1567 cm' and 1593 cm', which correspond to the graphite E2$ optic mode a t 1582 cm' which has been extensively studied in HOPG (highly oriented pyrolytic graphite) [9,201]. The strong lines between 1550 and 1600 cm' may be assigned t o the
Fig. 10.2: Plot of the observed Raman frequencies for several different singlewall carbon nanotube samples, prepared with different catalysts under different growth conditions yielding different mean nanotube radii P : (a) Fe/Ni (. = 0.55 nm), (b) Co ( P = 0.65 nm), and (c) La (r = 1.0 nm). The dashed lines are theoretical LO and TO energy dispersion curves for graphite along I'M as a function of q and q / 2 for n = 1 and n = 2 (first harmonic vibrat~on),respectively. Solid dots and the symbol 'T' correspond to the observed frequencies of the peaks and shoulders in the Raman spectra, respectively [202].
E l g , Ezg and Al, modes in carbon nanotubes with different diameters. Rao et al. [83] assigned the two strong modes of 1567 cm' and 1593 cml to the E2, (8,8), and Elg or A l , (9,9) tubes, respectively. The Raman frequencies in this high frequency region do not vary much with carbon nanotube diameter, as shown in the lower panels of Fig. 10.1. The Raman frequencies in the range 15501600 cml can be understood by zonefolding of the graphite phonon dispersion relations [202]. In Fig. 10.2, the observed Raman spectral frequencies are shown for three singlewall nanotube samples prepared with different catalysts and under different growth conditions yielding nanotubes with different mean diameters (radii) and different distribu
190
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
tions of diameters (radii). Specifically the catalysts and resulting average radii are: (a) Fe/Ni ( T = 0.55 nm), (b) Co ( T = 0.65 nm), and (c) La ( T = 1.0 nm). The dashed lines are theoretical LO and TO energy dispersion curves in graphite along I?M as a function of wavevector q and q/2 in units of lo9 cm' for n = 1 and n = 2 (first harmonic vibration), respectively. In armchair nanotuhes, the r  M direction corresponds t o the wave vector along the equator of the nanotubes. Thus LO (n = l ) , TO (n = l ) , and TO ( n = 2) correspond to the Al,, El, and Ez, Raman modes, which will be explained in the theoretical analysis in Sect. 10.4. Figure 10.2 shows a clear relationship between 1 / and ~ q on the zonefolded phonon energy dispersion curves. It is important to note that the Raman intensity for graphite in the 13001600 cm' region is sensitive t o sample quality. Generally the intensity of the Ezg modes of graphitic materials is sharp and strong when the sample is highly crystalline and defect free, while disordered graphites and carbons show a broad feature around 1350 cm' [9,201,203,204]. The 1347 cm' signal seen in Fig. 10.1 may come from a symmetrylowering effect, due to defects or nanotube caps, bending of the nanotube, and the presence of carbon nanoparticles and amorphous carbon. At 186 cml, a strong Al, breathing mode is found in Fig. lO.l(a) [see Fig. 9.5(a) on the right]. Because of the strong dependence of the frequency of the A l , breathing mode on nanotube diameter (see Sect. 10.3), the frequency of the A1, breathing mode can be used as a marker for assigning the approximate diameter of the carbon nanotube. The radial breathing A1, mode can also be clearly seen in fullerenes.* In the low frequency region, the calcvlations predict nanotubespecific El, and E2, modes around 116 cm' and 377 cml, respectively, for (10,lO) nanotubes, but their intensities are expected t o be lower than that for the Al, mode. However, these El, and Ez, modes are important since they also show a diameter dependence of their mode frequencies, as shown in the lower panels of Fig. 10.1. In the very low frequency region below 30 cm', a strong low frequency Ramanactive Ezg mode is expected. However, it is difficult t o observe Raman lines in the very low frequency region, where the background Rayleigh scattering is very strong. Even for a given sample, the Raman spectra may change if we change the frequency of the excitation laser. When the excitation energy is close to an energy 'For example, the A1, of
(360
has a frequency of 497.5 cml [198].
10.2. R A M A N EXPERIMENTS O N SINGLE WALL NANOTUBES
191
Fig. 10.3: Room temperature Raman spectra for purified singlewall carbon nanotubes excited at five different laser frequencies, showing the resonant enhancement of the Raman intensity associated with the vanHove singularities in the nanotube density of states [83]. Each trace is labeled by the wavelength and power level of the laser light. of high “optical” absorption, the Raman intensity is enhanced, and this effect is known as the resonant Raman effect. Under resonant conditions, more light can be absorbed, thereby enhancing the Raman signal through the electronphonon coupling process. In Fig. 10.3 are shown Raman spectra obtained with different laser excitation frequencies. When the laser frequency increases, the Raman modes that are preferentially enhanced shift to higher frequencies, since the resonance effect is most pronounced when the joint density of states of the carbon 1~ band is large, and the laser frequency matches a peak in the optical absorption. As discussed in the 5 4.2, the density of states of the 1~ band becomes singular by folding the twodimensional energy bands of the graphene layer into the onedimensional bands of the carbon nanotube, and these singularities are known as vanHove singularities. For every onedimensional band edge, as in a carbon nanotube, a I/@ singularity is expected for the energy dependence of the onedimensional density of states (see Fig. 4.7). The 1/fi singularities for the 1D density of states results in a much stronger resonant Raman effect than would be
192
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
observed for a 2D graphene sheet or for 3D crystalline graphite. Clearly the energy separation of these singularities in the 1D density of states increases as the number of energy bands decreases. When we consider only armchair nanotubes ( n ,n ) , the energy separation between the vanHove singularities becomes large with decreasing n. The Raman resonance condition thus selects the particular carbon nanotube ( n ,m) which has a singularity in its electronic density of states at the laser frequency. The observed phonon frequency of the low frequency A1, mode provides the value of the nanotube diameter that is in resonance electronically, since the phonon frequencies for the low frequency normal modes increases with decreasing n. Thus the resonance effect is a quantum effect that can be understood in terms of both the electronic and phonon dispersion relations of the nanotubes. Since nominal singlewall carbon nanotube samples consist of nanotubes with different diameters and chiralities, the resonant Raman effect may be seen in different nanotubes for different laser excitation frequencies.
10.3
Bond Polarizability Theory of Raman Intensity for Carbon Nanotubes
In this section we discuss the nonresonant bond polarization theory for calculating the Raman intensity, which is also useful for the interpretation of the Raman spectra. The Raman intensity for h/ atoms in the unit cell is calculated by the empirical bond polarizability model [205,206];
Here W L and w s are the incident and scattered light frequencies, r] and r]' are the corresponding unit vectors for the polarization of the light, respectively. w j is the ) l/(exp(hwf/hBT)frequency of the fth normal phonon mode, while ( n ( w f ) = 1) is the phonon occupation number at temperature T.The a and ,B subscripts in Eq. (10.6) denote Cartesian components of the vector or tensor, x , g , . z , and Pap,j is the derivative of the electronic polarization tensor for the fth normal mode, which is given by [205],
(10.7)
10.3 BOND P O ~ A ~ Z A ~ r ~THEORY r T Y OF AN ~ ~ T E ~ S ~193 T Y where Pap is the electronic polarization, and the derivative is performed with respect to the yth Cartesian displacement, u,(l), for the t t h atom. The term x,(tlf) is the y component of the unit vectors of the f t h normal modes of the t t h atom. Both translational and rotational acoustic modes are included in f for simplicity. However, the acoustic modes do not contribute t o the Raman in tensity. The term Pap in Eq. (10.7) is approximated by a sum over the bond polarization contributions as follows
Pap =
1 [
c l,B
{ a l p ) + W B ) } 6,@ 3
+ {9l(B)  Q ( B ) )
(
RU(eJ
B)Rp(e8
B, 
$6Qd)]
(10.8)
R(t,B)2
where B denotes a bond which is connected to the Gth atom in the unit cell, and R ( t ,Bf is the corresponding vector from the 4th atom to the neighbor atom l' specified by B . The quantities R,(L, B ) and R(4, B ) are the a component and the length of R(&,B ) , respectively, and aql(B) and a ~ ( 3 are ) the static molecular polarizabilities for the bond B in the directions parallel and perpendicular t o the bond, respectively, Here we assumed that q ( B ) and a l ( B ) are functions of only the length R(L,B ) . When we denote the bond vector without the displacements of the two atoms of the bond as Ro(4,B ) , then R(t,B ) can be defined by
R(4,B ) = &(&, B )
+
..(.el)
 a(e),
(10.9)
while the derivative on u, in Eq. (10.7) is expressed by the derivative on R(t,B ) as follows: a d d R ( t ,B ) =&(jJ? (10.10) €3 dR(t,B ) R(&, B> Here the summation is taken over the bonds connected to the 1th atom and we use the following relations: (10.11)
and
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
194
When we calculate Pap,j in Eq. (10.7), we have terms
aR("B) in 8%
After some calculation au, (el .
da
dR,(l,B)
du,
du,
,
7
and
and making use of Eqs. (10.10)'
(10.11) and (10:12), we obtain an explicit form for Pap,!,
(10.13) where all(B)and a y ( B ) are the radial derivatives of q ( B ) and a l ( B ) ,that is
) , I ( B )all(B) , and aL(B) are given empirrespectively. The values of a l ~ ( B ~ ically as a function of the bond length between two carbon atoms or between carbonhydrogen atoms, and these values are listed for carbon nanotubes in Table 10.2. In order to obtain values for the parameters for carbon nanotubes, we start by interpolating between the values for the polarizability parameters for single (1.46A) and double (1.40di) carbon bonds in c 6 0 and related materials [205,207]. Then we fit the values so as to reproduce the Raman signal for randomly oriented nanotubes. Although the calculated values are within a reasonable range for carbon materials, the values for the polarizability parameters listed in Table 10.2 do not converge well for carbon materials, because of the different results that have been reported by various groups.
Table 10.2: Bond lengths and Raman polarizability parameters for singlewall carbon nanotubes and for various carbonrelated molecules. (Y' 20'1 Q'  a ; Molecule Bond Lengths (YI~ 2 a ~ ( ~ 1 1 Q L
+
[A1
CH4") C  K (1.09) C ~ H G ~ )c c (1.50) CZH4&) C = C (1.32)

c  c (1.46)
c60b)
C = C (1.40) C  C (1.46) C = C (1.40) SWCNC) C = C (1.42) SWCNd) C = C (1.42)
Ceoa)
~
~
1~33
1.944 2.016 4.890
+

[k31
cf21
d21
1.28 1.65 1.28 0.32 It 0.09 1.28 f 0.20 0.00 f0.20 0.07 0.04
3.13 6.50 2.30 f 0.01 7.55 f 0.40 1.28 f 0.30 5.40 f 0.70 5.96
2.31 2.60 2.30 f 0.30 2.60 If: 0.36 1.35 f 0.20 4.50 f 0.50 5.47 4 .O
4.7
~
'1 S. Guha et al. [205]. D. W. Snoke and M. Cardona [207]. E. Richter et al. (unpublished data which is used in their work[83]). R. Saito et al. [208].
I t is known, however, that the polarizability parameters of carbon are similar for a variety of carbon materials. Furthermore, the relative intensities for the Raman modes are not so sensitive to small changes in the values of the bond polarization parameters except for the lowest E29 mode. The lowest Ez9 mode is found to be most sensitive to the parameter a11 a ~ Thus . the fitted values are used for calculating appro xi mat^ Raman intensities. The Raman intensity is calculated using the eigenvectors for the vibrational modes, obtained by solving the dynamical matrix, and the polarization parameters are obtained using bond polarization theory [205]. 10.4
Raman Spectra of Nanotubes with Random Orientations
The Raman intensities for the various Ramanactive modes in carbon nanotubes are Calculated at a phonon temperature of 300 K which appears in the formula of Eq. (10.6) for the Bose distribution function for phonons. The eigenfunctions for the various vibrational modes are calcufated numerically at the I' point (k = 0). Here we consider two possible geometries for the polarization of the light: the VV
CHAPTER LO. RAMAN SPECTRA OF CARBON NANOTUBES
196
and V H configurations. In the VV configuration, the incident and the scattered po~arizationsare parallel to each other, while they are perpend~cu~ar to each other in the V H direction. Generally the cross section for Raman scettering is a function of the scattered angle of the light. However, the formulae for the bond polarization theory consider only Smattered waves [205], and thus the calculated results cannot distin~uishbetween forward and backward scattering of the light. In Fig. 10.4, we show the calculated Raman intensities for the (10,lO) armchair, (17,O) zigzag and (11,s) chiral nanotubes, whose radii are, respectively, 6,7S& 6.66A, and 6.47A and are close to one another. The Raman intensity is averaged over the sample orientation of the nanotube axis relative to the Poynting vector of the light, in which the average is calculated by summing over many ( w 50) directions, weighted by the solid angle for that direction. Thus Fig. 10.4 is the calculated result for r~domIyorientednanotubes. We divide the discussion into the following three frequency regions: the lower (w _< 500 cm'), higher (w 2 1500 cml), and middle (500 cmI 5 w 5 1500 cml) frequency ranges. Then we discuss the phonon density of states for the Ramanactive modes which depend strongly on the chirality. Since we consider randomlyoriented nanotubes in this section, we do not need t o mention the direction of the polarization vector for the V V and V W configurations. On the other hand, we need the directions of V and H for calculating the Raman intensity of a nanotube. We present the sample orientation dependence of the Raman spectra of a (10,lO) nanotube in the next section, in which we rotate the nanotube axis by fixing the polarization vectors. rU.4.1
Lower ~ r ~ ~ R ~ e~ Spectra n c~ ~ ~
n
Here we discuss the Raman intensity for the lower frequency modes below The Raman intensity is normalized for each nanotube to a maximum intensity ( A l , in the V V configuration) of unity. When we compare the VV with the V H polariz~tions(see Fig. 10.4), the Raman intensity shows anisotropy. Most importantly, the A l , mode at 165 em' is suppressed in the VH configuration, while the lower frequency El, and E2, modes are not suppressed as much. This anisotropy is due to the low dimensionality of carbon nanotubes. The degenerate vibrations of the E modes, whose eigenfunctions 500 cml.
10.4. RAMAN SPECTRA WITH RANDOM ORIENTATIONS
vv
VH
.
,
€4,
4
197
A* 1687

11 388
o
400
% 1581 BOO 1200 woo
0
400
BOO 1200 1600
1581
400 800 1200 1600
1580 1571
400
600 1200 1600
I 
1%
E, 1591
400
600 1200 1600
Raman Shift [ cm’1 Fig. 10.4: The polarization dependence of the Raman scattering intensityfor (a) (10,lO) armchair, (b) (17,O) zigzag, and (c) (11,8) ehiral nanotubes and the tube radius are given on the right. The left column is for the V V scattering configuration and the right column is for the VH configuration. are orthogonal to each other, are relevant to V N signals. From the figure we see that the relative intensities for the same mode between the V V and VII polarizations are different but are on the same order for all the E modes. When we compare the lower frequencies of these Raman modes for nan
198
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
otubes, the frequency shifts systematically with increasing diameter. In Fig. 10.5 we give the calculated mode frequencies for the lower frequency Ramanactive modes on a loglog plot as a function of the carbon nanotube radius r for ( n ,m) in the range (8 5 n 5 10, 0 5 m 5 n). Figure 10.5 clearly shows straight line dependences for all four Raman modes, thus indicating a power dependence of u ( r ) on r. No chirality dependence is found for the mode frequencies for these modes, which is consistent with the fact that the energy gap of a semiconducting nanotube and the strain energy depend only on the nanotube radius and not on the chiral angle B [81,209]. From the slopes of ~ ( rfor ) this range of r , we conclude that, except for the lowest E2, mode, the frequencies are inversely proportional to r making only a small deviation from the predictions of Fig. 10.5. This dependence is closely related to the circumferential length of the nanotube. As for the lowest E2, mode, the frequency w z S ( r ) has a dependence of r1~95f0~03, which is approximately quadratic and may reflect the effect of curvature on the nanotube. The fitted power law for the A l , mode that is valid in the region 3hi 5 r 5 7A
4.) = q l 0 , S o )
y(lo,
[+
1.0017f0.0007 1
( 10.15)
should be useful to experimentalists in interpreting their spectra. Here w(10,10) and ~ ( 1 0 , 1 0 ) are, respectively, the frequency and radius of the (10,lO) armchair l~) respectively. nanotube, with vaiues of w ( 10,10)= 165 cm and r ~ 1 0 ,=6.?85& It is the noted that the El, and A1, modes exist in a similar frequency region. However, since the intensity of the El, modes is not as strong as that for the Al, mode, the experimental Raman spectra between 100 to 300 cml are dominated by the A l , mode as shown in Figs. 10.1 and 10.3. As for the higher frequency Raman modes, we do not see a strong dependence on P , since the frequencies of the higher frequency optical modes are more sensitively determined by the local movements of the atoms. 10.4.2 Higher Frequency Raman Modes
It is interesting that the higher frequency A1, mode a t 1587 cm' does not show a suppression between the V V and V H geometries, which is relevant t o the Raman active E2, mode of graphite. In the next section we will see that the A1, modes depend on the orientation of the nanotube axis. This fact shows that
1000
R
9
fj
100
U
3
0 0
 1
10
rIAl
Fig, 10.5: Loglog plot of the lower Raman mode frequencies as a function of carbon nanotube radius.
a V H signal can be expected when the vibration of the A1, mode is different from the polarization vector. In the nanotube, the lattice can be split into two sublattices consisting A and B atoms. In the higher frequency A l , mode, the A and B atom moves in opposite directions (outofphase) in the unit cell, while in the lower frequency A l , mode the A and B atoms move in the same way (inphase). In Fig. 10.6 we show the normal mode disp~acementsfor seven Raman modes for a (lO , lO } nanotube which have a relatively large intensity. It is clear from Fig. 10.6 (e) to ( g ) , that the modes are outofphase between nearest neighbor carbon atoms, while the modes of Fig. 10.6 (a) to (d) show inphase motion. The outofphase motions observed in Fig. 10.6 (e) to (g) are similar to the motion of the Ramanactive E2, mode of graphite at 1582 C M  ~ ,which corresponds t o C=C bond stretching motions for one of the three nearest neighbor bonds in the unit cell. Thus this motion is an outofphase motion. It is reasonable that the outofphase motions of the higher frequency Raman modes of a nanotube have a large Raman intensity, because of the relation of these modes to the Eag mode of graphite. The motions shown in Fig. 10.6 are independent of the chirality. When we see the motion of the higher or the lower Ramanactive modes of a nan
200
G
~
A 10.~ ~~A~ T ~ SPECTRA ~ OF CARBON N A ~ O ~ U B ~ S
A],
165cm'
AI,
Ezs 368cmI
1.587~111'
El, 1585cm'
E2, 1591cm'
Fig. 10.6: The calculated Raman mode atomic displacements, frequencies, and symmetries for those (l0,lO) nanotube modes which show strong Raman intensity. The symmetry and the frequencies for these modes are almost independent of the chirality of the nanotube. We show the displacements for only one of the two modes in the doubly degenerate El, and Ez, modes.
otube, we can consider an envelope function for the amplitude of the vibration, multiplying it by the abovementioned outofphase or inphase motions, respectively. We can say that the envelope function should satisfy the symmetry for the Ramanactive modes among the many phonon modes. For example, the envelope functions for the Al,, El9 and E2, modes are functions with zero, two, and four nodes around the tube zaxis, respectively [see Fig. 10.6 (f), ( e ) , and
10.4. RAMAN SPECTRA WITH RANDOM ORIENTATIONS
20 1
fg) for outofphase motion, and (c), (b), and (a) for inphase motion]. Thus the envelope functions with a given symmetry are similar to one another for nanot~ubeswith any (n, rn) values. This is the reason why we get similar Raman spectra for different chirality nanotubes. We can say within the discussion of the envelope function that we see a homogeneous elastic cylinder. When we investigate the vibration of the higher frequency A l , mode at 1587 cml, the vibration corresponds to the folded vibration of one of the higher Ez9 modes of graphite. Thus, in the cyli~dricalgeometry, we may get a result that is not so polarization sensitive. On the other hand, in C60t since all 60 atoms are equivalent, no carbon atom can move in an outofphase direction around the Cs axes for either of the two A l , modes, so that both modes show similar polarization behavior to each other [198]. However, the directions of the outofphase motions of the A1, modes are different for armchair and zigzag nanotubes. In fact the C=C bondstretching motions can be seen in the horizontally and the vertically vibrating C=C bonds for armchair and zigzag nanotube, respectively. Thus the curvature of the nanotube affects the frequency of these mode. When we focus our attention on armchair nanotubes, the higher Raman frequencies depend on the radius of the nanotube l / r via the wave vector q around the equatorial direction 12021, which is understood by the zonefolding method and is discussed in Sect. 10.2. Although these higher frequency modes are difficult to distinguished from one another because of their similar frequencies, it will be possible to identify the different modes experimentally, once purified aligned samples become available, as shown in discussing the angular dependence of the Raman int~nsities,which is reviewed in Sect. 10.5. lo.4.9
Medium Frequency Raman Modes
It could be very interesting to discuss the Raman frequency in the intermediate frequency region where the frequency may be the most chirality dependent [210], The calculated results, however, show almost no intensity for the ~ n t e r m e d ~ a t ~ Raman modes around 12001~00em'. The Raman experiments on singlewall nanotubes show weak features which have been assigned to armchair modes {83]. From the calculation we cannot explain why these low intensity peaks appears. The peaks might come from a lowering of the symmetry of the nanotube. In
202
C ~ A P 10. T ~ AN ~ SPECTRA OF CARBON ~
A
~
O
fact, broad Raman peaks around the 1347 cm'l are observed experimentally [83,135]. These peaks are known to be associated with symmetrylowering effects in disordered graphite [211] and carbon fibers [212] for which a broad peak is observed around 1350 cml, The relative intensity of the broad peak around 1350 cml to the strong EQ mode at 1582 cml is sensitive to the lowering of the crystal symmetry of graphite [211,213], the amount of disorder in carbon fibers [212] and in graphite nanoclusters [214]. The amount of disorder in these systems can be controlled by the heat treatment temperature THTor by ion implantation 12151. The nonzonecenter phonon mode a t 1365 cm' has a flat energy dispersion around the M point in the Brillouin zone of graphite, which implies a high phonon density of states * f216]. Moreover, in small aromatic molecules, the frequency and the normal mode displacements are modified by the finite size effect, so that these M point phonon modes becomes Raman active [217] and have a large intensity [214,218]. Thus some symmetrylowering effects such as the effect of the end caps, bending of the nanotube and the other possible defects are likely to turn on the Raman intensity for this Mpoint mode. Note that if the nanotube is deformed to a 2 x 2 structure for any reason, the M point phonon can be folded to the I' point and the folded modes becomes Ramanactive A , modes. However, since a Peierls instability is unlikely, as is discussed in Sect. 11.3, this situation may occur only in the case of intercalated nanotubes [135]. When we caIcuIate the Raman intensity for a nanotube with open ends, the intermediate frequency Raman modes have a small intensity relative to the strong peaks in the higher and the lower frequency regions. The observed Raman signal in Fig. 10.1 in the intermediate frequency region can be relevant to the finite length of a nanotube. As shown in Fig. 10.4, the chirality dependence of the Raman spectra is not clearly observed except for the frequency. However when we consider the absoIute Raman intensity, it is i m p o r t ~ n to t consider also the effect of the phonon density of states. The three nanotubes in Fig. 10.4 have almost the same diameters. However the number of carbon atoms per 1D unit cell is very different. For example, the (10,lO) and (17,O) nanotubes have 40 and 68 carbon atoms in their 1D unit cells, respectively. However, the (11,8) nanotube has 364 carbon atoms in its unit cell. Because of the large number of states for the (11,s) nanotube, it *See
Fig. 9.4 for 2D graphite. In this case we can see a flat band appearing below 1300 c m 1
T
U
should be difficult to observe the singularities in the electronic density of states in a (11,8) nanotube within the reso~utionof the STM because the singu~arities occur so close to one another. Thus the resonant Raman effect for chiral nanotubes should also be re~ative~y d i ~ c u t~o tobserve compared with the case of achiral nanotubes. It would be interesting to be able to assign the chirality of a nanotube from the Raman spectra by using many laser excitation frequencies. 10.5
Sample Orientation Dependence
In Sect. 10.4.2, we see that the high frequency Raman modes originate from the o u t  o f ~ p h ~Ezs e mode of graphite. As a result, the frequencies of the Raman modes in the high frequency region are close to one another, However since the symmetry of these modes are d i ~ e ~ e nthese t , mode can be separated from one another by exploiting special experimental geometry conditions. In Fig. 10.7, we show the intensities of the various Ramanactive modes for the (10,lO) armchair nanotube as a function of sample orientation. Here we fix the polarization vectors to lie along the z and x axes, respectively for the V and H polarizations. Then we consider the effect of rotating the nanotube axis from the z axis. In this geometry, three rotations of the nanotube axis are possible for the VV and the V H ~onfiguratjons,and these three rotations are denoted by Bi, ( i = 1 , 2 , 3 ) as shown in Fig. 10.7, Here 81, and 82 are the angles of the nanotube axis from the z axis to the x and y axes, respectively, while 83 is the angle of the nanotube axis around the z axis from the x to the y axis. Since we put the horizontal polarization vector along the x axis, 81 and 42 are different from each other for the V H configuration. Even for the VV configuration, the rotations by 81 and 42 are not equivalent to each other in the case of the (10,lO) armchair nanotube, since the (10,lO) armchair nanotube has a tenfold symmetry axis ( C ~which O ) is not compatible with the Cartesian axes. Here we define the x,y, z axes so that we put a carbon atom along the 2 axis when 83 = 0'. In Fig. 10.7, we show the relative Raman intensities for the (10,lO) armchair nanotube for the VV and V H configurations for the various Raman modes of a (10,lO) carbon nanotube as a function of &,(i = 1 , 2 , 3 ) . In Fig. 10.7 we see that the Raman intensity for the Al, mode a t 1587 cml as a function of 81 has a m a x i ~ u mat 81 = 0, which corresponds to 82 = 83 = 0, for the V V configuration, while the El, mode at 1.585 cml has a maximum
204
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES vv
VH
EJ591
0
30
60
E$68 80
Fig. 10.7: The polarization dependence of the Raman intensities as a function of the orientation of the nanotube axis for a (10,lO) armchair nanotube. 61, and 62 are angles of the nanotube axis from the z axis toward the z and y axes, respectively. 93 is the corresponding angle around the z axis from the z t o the y axes. The left and right hand figures correspond t o the VV and V H polarizations, where V and H correspond to the light polarization in the direction of the z and z axes, respectively.
el = 45'. When 81 increases t o 45O, the relationship between the intensities of the A1, mode at 1587 cm' and of the E2, mode at 1591 cml becomes reversed for the VV configuration relative to the V H configuration. Thus, we can distinguish these two closelying modes from each other experimentally if we have an axially aligned sample. There is also an E2g mode at 1591 cm' at
10.5. SAMPLE ORIENTATION DEPENDENCE
205
which can be distinguished from the Al, and El, modes, since the E2, mode intensity at 81 = 90'. As for the other Ramanactive modes, we has a m ~ i m u m can also distinguish them by their frequencies. In Fig. 10.7, the two Ez, modes at 368 and 1591 cm'l have almost the same intensity in the VV configuration. Thus we can see only a single line in the VV configuration of the figure. However in the 8 2 dependence of the V H configuration, we can see the difference between these EzS modes. Even the modes belonging to the same irreducible representation do not always have the same angular dependence with regard to the polarization of the light. For example, the intensity of the Al, mode at 165 cml has a different angular dependence from that of the A l , mode a t 1587 cm', as shown in Fig. 10.7. Further, it is clear from the figure that the angular dependence with respect t o 81 and 6 2 is different for the V H geometry since the horizontal polarization is taken in the x direction, The symmetry analysis may be difficult even if we can get an aligned nanotube sample for which the direction of the carbon atoms is ordered, since the 10fold symmetry of the (10,lO) nanotube does not satisfy the symmetry of the trian~u l a rnanotube lattice. Thus an averaged angular dependence for 01 and 02 in the V V geometry is expected for a general aligned sample. Even in this case, since the Al, mode a t 1587 cm' is independent of 03, the signal for this mode will be clearly seen. The (9,9) armchair nanotube is of special interest, since it is one of a few examples where the nfold symmetry of the nanotube matches the t r i a n g u ~ alattice; ~ therefore, for (9,9) n an o tu b ~ sin a trjanguiar lattice, detailed angledependent selection rules can be expected. In summary, the Raman intensity of armchair, zigzag, and chiral nanotubes is discussed in Sects. 10.4 and 10.5 as a function of their polarization geometry and sample orientation. N o significant dependence on chiral angle is found for the Raman spectra. The Raman intensity is explained by the envelope function of the amplitude of the vibration, and this envelope function is sensitive only to the homogeneous elastic cylinder. However, we expect to see a large c h i d dependence of the phonon density of states which is reflected in the absolute intensity. The sample orientation dependence of the Raman intensity shows that not only the symmetry but also the direction of the displacements give rise to their own angular dependence, and this angular dependence can be used for distinguishing between the symmetry assignments for the higher frequency Raman
206
CHAPTER 10. RAMAN SPECTRA OF CARBON NANOTUBES
modes. Such a symmetry analysis will also be useful for identifying the chirality of carbon nanotubes.
CHAPTER 11.
Elastic Properties of Carbon Nanotubes
Since the C=C bond in graphite is the strongest bond in nature, a carbon nanotube is widely regarded as the ultimate fiber with regard to its strength in the direction of the nanotube axis. Furthermore, single wall nanotubes are rather flexible in the direction normal t o the nanotube surface. The static elastic properties of carbon nanotubes are discussed in Sect. 11.2. The unusual aspects of the Peieris instabilit~} associated with the distortion which makes an energy gap a t the Fermi energy, in carbon nanotubes are discussed in Sect. 11.3. Multiwall carbon nanotubes have unique properties that do not appear in single wall nanotubes, and these are summarized in Sect. 11.4.
11.1
Overview of Elastic Properties of Carbon Nanotubes
In graphite and in carbon nanotubes, three kinds of forces between carbon atoms produce their characteristic elastic properties. The fundamental atomic forces consist of strong c.rbonding and nbonding forces between intralayer C=C bonds and weak interlayer interactions. Although the three forces differ from oneanother regarding their orders of magnitude, all three forces are essential for describing the elastic properties of carbon nanotubes, as shown in the following three sections, respectively. En each section we give an overview of the relationship between the properties and the force. By rolling a graphene sheet to form a single wall carbon nanotube (SWCN), the total energy of the nanotube is increased by the strain energy associated with the curvature of the nanotube. The strain energy thus increases with decreasing nanotube diameter, so that a nanotube with a small diameter may be less stable than a nanotube with a larger diameter. In graphitic materials, sp2 covalent
207
208
CHAPTER 11. ELASTIC PROPERTIES OF CARBON NANOTUBES
bonds mainly form the D skeleton of the honeycomb lattice. Thus the strength in the direction of the nanotube axis may be considered as an elastic thin film for which classic elastic theories can be applied [219], as shown in Sect. 11.2. On the other hand, we expect a rather soft surface in SWCNs for a force applied perpendicular to the surface of a carbon nanotube, and this feature of SWCNs can also be explained by consider in^ a tangential force on the abond skeleton. Single wall carbon nanotubes have no interlayer interactions, since a hollow vacuum core exists inside each nanotube. In fact, a perpendicular deformation is not always stable and the cross section of carbon nanotubes is easily flattening by applying a force normal to the nanotube axis [220] and a large bending of single wall nanotubes is observed without breaking the skeleton [221]. Using elastic continuum theory to describe the elastic properties of nanotubes, we discuss in Sect. 11.2 the rigidity of carbon nanotubes and the weak chirality effects expected for their elastic properties. Singlewall carbon nanotubes are believed to possess many of the desirable mechanical properties of carbon fibers, but, in addition, singlewall carbon nanotubes have a number of other desirable nanotube properties with regard to their flexibility, their ability to withstand crosssectional and twisting distortions, their extensibility, and their ability to withstand compression without fracture. Just as for the carbon fibers that are produced commercially for aerospace applications, carbon nanotubes show excellent strength characteristics under extension, and molecular dynamics simulations [222] indicate that an increase in length (elongation) of several percent without fracture might be possible [95,219]. In addition to these amazing predictions for their tensile properties, singlewall nanotubes show remarkable flexibility, and can be bent around small circles or about sharp bends without breaking [ l l O ] . Whereas carbon fibers fracture easily under compression, carbon nanotubes form kinklike ridges under compression, and these ridges can relax elastically when the stress is released. Computer simu~ations12221 further indicate that when the c o m p r ~ ~ i o nor a l shear stress is released, the original circular crosssection of the nanotube can, in many cases, be restored [219]. It should be possible to utilize these excellent mechanical properties for applicat~onsdirectly, or in conjunction with their use for manipu~ating other nanostructures [53]. Although the 7~ electron contribution to the elastic energy is relatively small compared with that from the c electrons, the 7~ contribution is nevertheless
21.1 OVERVIEW OF ELASTIC PROPERTIES OF NANOTUBES
209
important for obtaining the lattice distortion known as the Peierls distortion (see Sect. 11.3.2). Although one third of the possible carbon nanotubes that can be formed are onedimensional metals, and it is well known that the Peierls instability is favored in low dimensional systems 12231, the associated lattice distortion can be negligible in the case of carbon nanotubes because of the following physical situation. The Peierls instability is known to cause a metalinsulator transition, by opening an energy gap at the Fermi energy to benefit from the eIectronic energy gain which is introduced by the distortion of the lattice into a doubled unit cell. The values of the distortion are determined by minimizing the total energy as a function of the distortion, in which the energy gain associated with the electronlattice interaction of the T electrons is balanced by the energy loss of the potential energy of the Iattice. Starting from a general theory of the Peierls instability, we focus our attention on the reason why the Peierls distortion is suppressed in carbon nanotubes in Sect. 11.3. Multiwall carbon nanotubes have many interesting properties that are not observed or explained by the physics of singlewall nanotubes. In multiwall nanotubes, the relatively weak interaction between two adjacent layers determines their relative stacking structure, which denotes the positions of the atom sites on the outer layer, relative t o those on the inner layer of the nanotube. The lattice structure of the inner and the outer layers are generally incommensurate with each other, which describes the turbostratic structure of multiwall carbon nanotubes. This turbostratic structure affects shear stress between the nanotube shells. However, in some cases, the interlayer stacking can become correlated, and experimental evidence has been found for faceting in some multilayer nanotubes [224,225]. Because of the weak and incommensurate electronic interaction between the two layers, the electronic structure between two adjacent carbon layers is considered in terms of a sum of the electronic structures of the constituent nanotubes. Furthermore, in discussing multilayer nanotubes we require that in the limit of large nanotube diamet,er, all the nanotube properties should correspond to those of graphite. These topics are briefly summarized in Sect. 11.4.
210
11.2
CHAPTER 11. ELASTIC PROPERTIES OF CARBON NANOTUBES
Strain Energy of Carbon Nanotubes
When we consider a singlewall carbon nanotube as an elastic sheet, the strain energy E, is inversely proportional to the diameter of carbon nanotube, dt: [12], (11.1)
where E is the elastic modulus of the sheet, T is the length of the carbon nanotube per 1D unit cell in the direction of the nanotube axis [see Eq. (3.5)], and d f is the thickness of the thin film, which can be considered as the interplanar distance between two turbostratic graphene layers (3.446;). Since the number of carbon atoms per unit cell N = 2LT/&a2 [see Eq. (3.9)] is also proportional to dt (i.e,, L = 2sdt), the strain energy per carbon atom is inversely proportional to the square of the nanotube diameter: (11.2)
This simple argument for a dependence of E,/N on d t 2 is confirmed by a more detailed first principles calculation of the strain energies of many carbon nanotubes with different diameters and chiralities [209], as shown in Fig. 11.1. The solid curve in the figure depicts the (l/dt)' dependence of E , given in Eq. (11.1), showing that we can understand the functional dependence of the strain energy of a carbon nanotube from the simple arguments given above for an elastic thin film. The small deviations of the strain energy as a function of nanotube diameter (or radius) suggests that the dependence of E,/N on chirality, is very weak, and this weak dependence may be due to: (1) chiralitydependent directions of the three equivalent u bonds with respect to the nanotube axis, and (2) chiralitydependent contributions of the K bonds, depending on whether there is an energy gap or not in the dispersion relations. Although the total energy depends on the nanotube chirality and thus should be related to the stability of the carbon nanotube, the abundance of a given diameter carbon nanotube should not depend on the chirality. This is because the abundance of nanotubes is determined by the initial formation of the end cap of the carbon nanotube. In fact, experimental results for the diameter distribution of single wall carbon nanotubes do not show the same diameter distribution for different catalysts [57]. Since the diameter and chirality cannot
11.2. STRAIN ENERGY OF CARBON ~ A ~ O T ~ 3 E S
211
Fig. 11.1: Strain energy per carbon atom E, as a function of nanotube radius ri = d t / 2 [Sl]. The solid curve depicts the ( l / d t ) 2 dependence of E, given in Eq. (11.1). be changed in a singlewall nanotube unless a defect exists, this result might show that the diameter and chirality that are obtained in the growth process depend mainly on the shape of the caps generated by the catalytic particle. The lower limit of the diameter of a single wall carbon nanotube seems to be the diameter of CG0. In fact there is no report of observation of a nanotube with a diameter smaller than that of (360. When a force acts pe~pendicularto the nanotube axis, the nanotube bends, as described by the Young's modulus Y [220]. When we consider a cantilever beam of length 4, the deflection d of the beam with a force f at its free end is given by [219] d =  ff3 (11.3) 3Y I where I is the areal moment of inertia of the crosssection of the nanotube r i ) / 4 , in which r, and r; are the outer and inner about its axis, I = Z(Y: radii of an elastic cylinder, respectively [220]. As a first approximation* we use Y= where the elastic modulus Cl1 for a carbon fiber for Y , C11= 1060 GPa [9,219,226]. Overney et al. calculated the beam rigidity of a carbon nanotube in the same geometry, using the Keating potential whose parameters are given by the local density functional calculation [227]. Their calculated result shows that the beam rigidity is 200 times greater than a Pr bar of the same size. The

'The Young's modulus Y is given by (S);' I where Si, denotes the compliance tensor. Since C ~= Z 220 GPa is not negligible in a carbon fiber, we expect Y for a carbon fiber (N 800 GPa) to be somewhat smaller than 4 1 for graphite. However, since we expect Clz in a nanotube to be reduced relative to graphite, we may use the Cli values for graphite to obtain a value for Y for carbon nanotubes.
212
CHAPTER 11. ELASTIC PROPERTIES O F CARBON NANOTUBES
calculated Young’s modulus for a carbon nanotube is about 1500 GPa. There are many calculations for the Young’s modulus whose value varies from 500 to 1500 GPa, depending on the potential model and on the estimation for the cross section. When we consider a single wall nanotube, we may use Eq. (11.3) and we can consider the wall thickness to be 3.44A, which is the interlayer separation between turbostratically stacked graphene layers [9]. When the diameter of single wall nanotube increases, the nanotube is unstable in the direction perpendicular to the surface. The TEM observations show evidence for nanotubes collapsing into a flattened or bent nanotube without breaking the nanotube structure. TEM photos of a collapsed nanotube look similar to the bending of a rubber nanotube [228]. On a nanometer (nm) scale, the nanotube seems to be rather soft in the direction perpendicular to the nanotube axis. The experimental observation of the Young’s modulus of a single nanotube is difficult because of its small diameter. A novel method for measuring the Young’s modulus of individual nanotubes has been developed, whereby the amplitude of a thermal vibration of the nanotube is observed as a function of temperature [229]. At a high temperature T where a classical Boltzmann distribution of probabilities, P c( exp(E/kBT), can be used, the average of the vibrational energy, (W,), for a vibrational mode, n , becomes k B T , or (W,)=kBT, where ]cg is Boltzmann’s constant. Since the averaged value of W, is proportional to the square of the amplitude ti:, we can write (11.4) where c, is a spring constant. The spring constant is estimated by directly observing the amplitude of the thermal vibration as a function of temperature within the standard deviation u2 = k
BTCn
1
(11.5)
cn
given by statistical physics. The relationship between c, and the Young’s modulus Y is given by use of elasticity theory for continuum media (11.6)
11.3. THE PEIERLS INSTABILITY OF NANOTUBES
213
+
where the values 3/, are solutions to the equation, cosp, coshp, 1 = 0. In their experiments the authors used a clamped hollow cylindrical cantilever of length L 12293. The leading numerical values for Bra,( n = 0,1,2,3,. . .) are 1.8751, 4.6941, 7.8548 and 10.9955 and for larger Pn values, fin can be found by the approximation fin (a 1 1 2 ) ~ .By fitting a, b, and L to Eq. (11.6) for various nanotubes, the estimated results for Y are found to be in the range of 1000 G P a , comparable to CIl for graphite.

11.3 11.3.1
+
The Peierls Instability of Nanotubes Bond Alternation
Next we discuss the effect o f t electrons on the elastic properties. When electrons occupy about half of the valence energy band of # n e  d i ~ e n s i ~materials, n the energy bands are unstable to a distortion of the lattice into a doubled unit cell. For the doubled unit cell in real space, the corresponding unit cell in reciprocal space is reduced by a factor of 2. Therefore, the energy dispersion relations are folded in half and an energy gap is opened at the Fermi energy a t the zone boundary of the foided Brillouin zone. This effect is known as the Peierls instability. For partially filled bands, such a distortion leads to a lowering of the energy of the system a,s the lower energy bands become occupied and the higherlying energy bands remain empty. An example of the Peierls instability is the bond alternation or the Kekul6 structure of neutral carbon nanotubes [230], which has been discussed 12302331 in terms of the SuSchriefferHeeger (SSH) model, developed initially for polyacetylene (CH), /234], and subsequently for CSOand its ions [2312331. In the SSH model, a tightbinding Hamiltonian describing bondalternat~on is solved in a large unit cell in which the transfer integral between the nth and mth atoms, ,f is defined by
and t,, becomes a function of the distortions of atoms from their originai positions, x, and 2,. In Eq. (11.7>, t:, is the transfer integral without bond alternation (2.5 3.2 eV) and a denotes the electronphonon coupling constant ( w 5.0 eVfA). When the two atoms are close to each other, the absolute value

214
CHAPTER 11. ELASTIC PROPERTIES OF CARBON NANOTUBES
of the transfer integral' becomes large. In the case of polyacetylene (CH),, the bond alternation problem can be solved by using a doubled unit cell with a distortion zn = (  l ) n z ~leading to two transfer integrals tl and t2, (tl = to  2 a q and tz = t o 2az0, with It11 < 1t21). When we neglect the overlap integral, s = 0 in Eq. (2.20) for simplicity, N A B of Eq. (2.17) becomes
+
N A B = t l e ikal2 + t2eika/2
(11.8)
and the secular equation is given by f2p  E tleika/2 + tZe+ika/2
=
(fgp
 E)2 (tf t t;
= 0.
+
tleika/2 + taeika/2 f2p  E 2tlt2 cos ka)
1
(11.9)
The solution of Eq. (11.9) yields the dispersion relations
Ef(z)= czP f Jtt + t i
+ 2tlt2 coska, (a
'IT
'IT
< k < ), a
( 11.10)
which are plotted in Fig. 11.2 for the values of tl = 1.1 and t2 = 0.9. Comparing Figs. 11.2 and 2.2, wesee that an energy gap of 2)tltzI = 8azo = 0.4 is opened at k = f a / a because of the bond alternation. The electronic energy of those electrons which are in the occupied valence energy band (E+ band in Fig. 11.2), decreases by opening the energy gap. On the other hand, the elastic energy increases by ESP= 4Kzi (1 1.11) where I< is a spring constant, and thus the optimized value of 20 is given by minimizing the total energy. Putting tl = to  2azo and t2 = to 2az0 into Eq. (ll.lO),the energy difference of the electronic energy is given by
+
.12) Thus the total energy EM = Eel
+ ESPhas a minimum, dEtot/dzo = 0 when
8Kzo = a /"'a d k d dA 'IT n/a 8x0 *It is noted that tOnm
< 0 and a > 0 in Eq. (11.7).
+ B cos La,
(11.13)
215
rr;l
Fig. 11.2: The energy dispersion relation I3k.i) for bondalternating polyacetylene given by Eq. (11.10) using values for the parameters ~2~ = 0, t l = 1.1 and t 2 = 0.9. The energy gap at k = f a / a arising from the bond alternation has a value of 2 ] t l  t 2 l = 8 ~ ~ x=00.4 in these units.
0.0 
1.0
0.5
0.5
0.0
1.0
kdz
where A and B denote A = 2t$ f 8a2x$ and B = 2t$  8a2x:, respectively. The integration of Eq. (11.13) is given analytically by
( 11.14) where K ( z ) , and & ( z ) are, respective1yJ the complete elliptical integrals of the first and the second kind defined by, K(2)
=
LTf2
HB
vczzT
and & ( a ) =
Jld
*P
d
B
u
.
(11.15)
In Eq. (11.14) z is a function of xo which is given by 2
z 2 =   2B
AfB
14(?)
(11.16)
*
To solve Eq. (11.14), we use the mathematical formula cos 28 = 1 2sin2 6,and obtain a solution for 20 over a reasonable range of a > 0. t When 1.1
< 1 w e can expand K ( z ) and E ( z ) around le = 0 to obtain: K(.) =
2
{+ 1
($2
+
(E)’.t+ ...}
and
qz,=2{l(;)22+(2.4) 1.3 2 respectively.
:+..*},
224
,
216
C H A P T E R 1 1 . ELASTIC PROPERTIES OF CARBON NANOTUBES
‘I
/
I/x
/
1
1
Fig. 11.3: The normalized energy gap of polyacetylene, which is the solution of Eq. (11.14), Egap 3 8azo/ltol, is plotted as a function of the normalized electronphonon interaction z 4 a 2 / ( ~ l t o l K ) The . inset shows a linear dependence of  log( Egap)  . as a function of 1/x.
I
X
In Fig. 11.3 we plot the normalized energy gap, Egap3 8azo/ltol, as a function of the normalized electronphonon interaction z z 4a2/(rltoIK). In the inset of Fig. 11.3 we plot  log(EgaP)as a function of l / z , clearly showing a linear dependence of  ln(Egap) on l / z which is numerically fitted by (11.17)
The functional form of the energy gap is similar to that for the superconducting energy gap according to BCS theory. Because of this lowering of the total energy, bond alternation is always found in a onedimensional metal. The corresponding lattice deformation is called the Peierls distortion. In a molecule which has degenerate and partiallyoccupied levels associated with the high symmetry of the molecular geometry, the degenerate states become unstable under a lattice distortion, which lowers the symmetry and splits the degenerate levels so as to open an energy gap between the filled and unoccupied states. This effect which is similar to the Peierls instability is called the JahnTeller effect in quantum chemistry. The Peierls instability is thus a kind of JahnTeller effect which occurs in the solid state.$ In higher dimensions, this instability does not always occur, simply because the energy gain in a small region around the Fermi energy is not always larger than the energy loss associated with the elastic energy.§ In a carbon nanotube, $The Peierls instability is sometimes called a band JahnTeller effect. §There are no pure one or two dimensional solids in three dimensional space. The Peierls instability occurs when the shape of the Fermi surface is close to that of a onedimensional
11.3. T H E PEIERLS INSTABILITY O F NANOTUBES
217
Fig. 11.4: Possible bond alternation for a honeycomb lattice. (a) a Kekul6 type inplane bond alternation,(b) a quinoid type in
plane bond alternation, and (c) an outofplane bond alternation. In the case of inplane bond alternations, thick and thin lines, respectively, denote shrunk and elongated bonds, while solid and open circles in the outofplane bond alternation denote deformations in the +z and z directions, respectively.
although the geometry is onedimensional, the electronic structure becomes close to that of graphite as the diameter increases. Thus a dimensional crossover associated with bond alternation occurs at 0 K, as described in Sect. 11.3.2. $1.3.2 PeierEs Distortion of graphite and carbon nunotubes
In chapter 2 we show that twodimensional graphite has no energy gap between the bonding and antibonding T bands because there are two equivalent carbon atoms in the unit cell which give rise to a symmetryimposed degeneracy at the Brillouin zone corner. If the two atoms were not equivalent to each other, an energy gap would appear, thereby lowering the electronic energy. Whether this symmetrylowering distortion does occur or not depends on the strength of the electronphonon coupling constant, which we will discuss in this section. In the honeycomb lattice we can consider three kinds of lattice deformations as shown in Fig. 11.4; (a) a Kekul6 type of inplane bond a~ternation,(b) a quinoid type inplane bond alternation, and (c) an outofplane bond a~ternation. In Fig. 11.4(a) and (b), thick and thin lines, respectively, denote shrunk and surface, ur when two Fermi surfaces are parallel to each other over large areas in the Brillouin zone (the nesting condition).
218
CHAPTER 11. ELASTIC PROPERTIES OF CARBON NANOTUBES
elongated bonds. In the case of an outofplane deformation, the A and B sites in the unit cell deform in the +t and 2 directions, respectively. After deformation] the unit cell becomes twice as large as the original unit cell in the case of inplane deformations, while the unit cell for outofplane deformations does not change. Thus for simplicity we consider the case of an outofplane deformation. Even if we deform the lattice by an outofplane deformation, all CC bonds are still equivalent to each other, and thus there is no relative difference in the transfer energy between the A and B sites. When the site energies have different values for the A and B sites, the two sites are not equivalent. For example the A and B sites are inequivalent in threedimensional graphite, in which the A sites have carbon atoms above and below the atom but the B sites do not.* In a single layer of graphite, there is no relative difference in the site energy between the A and B sites. However, in the case of a single layer carbon nanotube, there is a difference between the inner and outer directions. If we assume that the site energy for the A and B carbon atoms is shifted by &aro/2 in which a is the electronphonon coupling constant per distortion t o , the energy dispersion of the distorted T bands of graphite is given by solving the perturbation Hamiltonian , 31=( a t 0
tf(k)*
tf(k))
,
(11.18)
at0
where t and f(k) are defined by Eq. (2.24) and Eq. (2.25), respectively. Here we neglect the effect of the overlap matrix S and we put czP = 0 in Eq. (2.26) for simplicity. When the distortion is included, the calculated energy dispersion E ( k ) becomes
This relation implies an energy gap of 2azo at the K point. The value of t o is obtained by minimizing the total energy which is given by the sum of the ~
*In the SSH Hamiltonian they consider only the change of the transfer energy by the lattice deformation. Here we consider only the change of the site energy by the lattice deformation. Generally, the electronlattice interaction affects both the transfer integral and site energies. See, for example, R. Saito and H. Kamimura, J. Phys. SOC.Japan 52, (1983) 407.
electronic energy and potential energy of the lattice. No distortion from the honeycomb lattice is observed in crystalline graphite because the density of states at the Fermi level is zero in the case of twodimensional graphite. This situation is explained below as the limit of a carbon nanotube. Let us consider the Peierls instability of a carbon nanotube, Here we consider only outofplane distortions for the case of a zigzag carbon nanotube, (n,0), for ~ i m p ~ ~ iSince t y . the size of the unit cell does not change in the case of an outofplane ~ i s ~ o r t i othe n , electronic structure of a distorted (n, 0)zigzag nanotube is obtained by zo~efoldingas discussed in Eq. (4.7). The 4% energy dispersion relations of the distorted (n,O) zigzag nanotube, E&(k), are expressed as
Taking account of the potential energy of the lattice as K $ f 2 per unit cell of graphite, in which IC is a spring constant, we obtain the following gap equation for the (n,0) zigzag nanotube
in which X(z) is the complete lipt tical integral of the first kind defined in B4 are given by
Eq. (11.14), and A, and
(y) 2
A,=
+ 1 + 4 c o s 2 ( ~ ) and 8 , = / 4 c o s ( ~ ) / ,
(11.22)
respectively, and Eq. (11.21) is obtained by use of the mathematical formula,
(11.23) which directly follows from the definition of K in the footnote of the previous subsection.
220
CHAPTER 1 1 . ELASTIC PROPERTIES OF CARBON NANOTUBES Fig. 11.5: The normalized energy gap Egap a2zo/ltol for metallic zigzag nanotubes, ( n ,0), is plotted as a function of the normalized electronphonon interaction 2 E a2/(Iilltl)(t < 0 ) for special valuesof n = 3, 6, 12, and 999(w m, which is essentially 2D graphite) denoted by solid, dotted, dashed, and bold solid lines, respectively.
=
0.8 0.6

0.0
I.o
0.5 X
1.5
In Fig. 11.5, we plot the energy gap Egap 2 a z 0 / ( t 0 I ,which is normalized by x which is the electronphonon interaction a2 normalized by IiltoI so that 2 a Z / ( I i l t ~(lt)o < 0). The plot in Fig. 11.5 is made for special values of n that are multiples of 3, namely n = 3, 6, 12, and 999 ( 00, corresponding to 2D graphite) denoted by solid, dotted, dashed, and bold solid lines, respectively. From the figure, we see that the dependence of the energy gap of the nanotube on the electronphonon coupling constants is very close to that for the 2D case, and that an energy gap appears due to the finite values of the interaction, Actually in the case of zigzag nanotubes, the energy gap has nonzero values for small values of 2, although these values can be exponentially small, its seen in Eq. (11.17). The difference between the application of Eq. (11.17) to polyacetylene and carbon nanotubes is that the factor appearing in the exponent of Eq. (11.17) depends on n for (la, 0) zigzag nanotubes as 0: exp(nA/z) (A is constant) [711. Thus for large R a larger interaction x is necessary for opening an energy gap. The reason why we get the present results is that the electron energy gain comes only from two of the 4n energy bands which cross the Fermi energy, while the elastic energy loss comes from all of the 27a carbon atoms in the unit cell [71]. + 00, we obtain the twodimensional case in which a In the limit of nonzero value of zo appears only when cx2/Kjtoi > 1.01. Since there is no experimental distortion in 2D graphite, the normalized interaction of a 2 / I C J t ~ l satisfies a2/K1tOl < 1.01. As for the other types of d~stort~ons of carbon n ~ o t u b e shown s in Fig. 11.4, Harigaya et a1.(233] and Viet et a1.[235] independently calculated the energy gap l t o l , for metallic zigzag nanotubes (la, O ) , as a function of
=
11.4. PROPERTIE§ OF ~ ~ ~ T I NAMOTUBES W A ~ ~
221
as a function of the chiral vector or the intensity of the electronphonon interaction, using the SSH model for twodimensional graphite. The calculated result shows a similar functional dependence of the energy gap on the electronphonon interaction. A magneticinduced distortion can however occur in a nanotube since the density of states at the Fermi energy is enhanced by the presence of a magnetic field by forming the l = 0 Landau level, as discussed in detail by Ajiki and Ando [lSO]. The electronelectron repulsion interaction, which is considered to be large in conjugate polymers, is also expected to be important in carbon nanotubes, since they are aIso P owdimens~ona~ materials. Onsite ~ ~and offsite ~ electron~ interactions (Uijlai,nj,,) are taken into account in the SSH Hamiltonian, in which the twobody effect is calculated mostly within the HartreeFock approximation, while keeping selfconsistency between the charge and the lattice distortion [233]. Within the reasonable range of U N Itol, the lattice distortion is determined by the electronphonon interaction (a).For larger U , a spinPeierls interaction may occur in which the interaction between the two spins is now a function of the deformation of the lattice: ( J ]itI2/V = JO a3(zn zn+l)).t In conclusion, though metallic 1D energy bands are generally unstable under a Peierls distortion^ the Peierls energy gap obtained for metallic nanotubes is found to be greatly suppressed by increasing the nanotube diameter. Thus the Peierls gap quickly approaches the zeroenergy gap of 2D graphite [69,71]. Thus if we. consider finite temperatures or fluctuation effects, it is believed that eV) cannot be observed experimentally. The such a small Peierls gap (< coexistence of metallic and semiconducting carbon nanotubes, depending on the chirality of the carbon nanotube, is independent of the lattice deformation. N
11.4
+

Properties of ~ u l t i  ~ Nanotubes a~l
In this section, we list several interesting features that can be seen only in multiwa.11 nanotubes. Although multilayer nanotubes have not been characterized in detail for their physical properties, because of the difficulty of making measurements on the individual shells of the nanotube and of sample preparation of tThere is an kinetic exchange interaction J N it12/U which favors the ~ t i f e r r ~ m a g n e t i c interaction. Since the transfer energy t in the SSH Hamiltonian is a function of (sn 3 c n + l ) , [see Eq. {11.7)], J depends on the deformation, This effect is known as the spinPaerls distortion.

~
222
CHAPTER 1 1 . ELASTIC PROPERTIES OF CARBON NANOTUBES
a welldefined and structurally characterized multiwall nanotube, the coaxial nanotubes provide an interesting geometry, as shown below. When we consider two coaxial n ~ n o tu b eswhich share the same n ~ o t u b e axis, the chiral vectors of the inner and outer nanotubes can be determined separately, which give the radii of the constituent nanotubes and the interlayer spacing between them, However, the structures of the two nanotubes will not be commensurate to each other in almost all concentric nanotubes, since their ratio of lengths in the circumferential direction is scaled by the ratio of the two diameters, but is not scaled in the direction of the nanotube axis. Further for (n, m) nanotubes, the length of the chiral vector ch = L is proportional t o an irrational number L = adnz m2 nm. The only commensurate cases are the cases of the achiral coaxial nanotubes, since the translation vectors, T , are the same for two armchair nanotubes (721, n l ) and (n2, n2) (where T = a ) or for two zigeag nanotubes (nl,O),(n2,O) (where T = d u ) . Thus the lattice constant along the z axis has a 1 to 1 commensurate ratio. As for the circumferential direction, cyclic boundary conditions always imply a commensurate relation. In achiral nanotubes, the commensurate ratio is expressed by n1/n2. It is clear that an armchair nanotube and a zigzag nanotube cannot be commensurate in the direction of the z axis, since the ratio of T is l/&. In the case where the two are general chiral nanotubes, since the length of T = f i L / d ~is an irrational number in units of a [see Eq. (3.8)], the ratio of the T vectors for the two nanotubes will be an irrational number. In the case of ~ncommensuratecoaxial nanotubes, no periodicity appears along the z axis. This means that when we put carbon atoms on the x axis, both for the inner and outer nanotubes, we will not see any two atoms in a line parallel to the 2 axis. When we slide the inner nanotube along the z axis relative to the outer nanotube, the elastic potential is, however, a periodic function, with a period that is the larger value of the T vectors for the constituent nanotubes. When the number of carbon atoms in the unit cell of the constituent nanotubes becomes large, the potential becomes flat, since the average of the interatomic potentials a t different distances does not depend much on +. In this sense, the shear modes between two graphite layers, which is observed at 42 cm' in graphite, should be much reduced in the multiwall nanotube. One nanotube may move smoothly with respect to the other in the attractive force between the two walk. Since we have two degenerate shear modes in the x and y directions in
+
+
11.4, PROPERTIES OF MULTI WALL NANOTUBES
223
the graphitic plane, we can expect another shear mode in the nanotube which corresponds to the rotation around the z axis. Since there are two chiral vectors in a horizontal plane perpendicular to the nanotube axis, the rotation around the z axis has a periodicity of Znld,, where d, is the common divisor of the four integers, n l , m l , 712, and m2 for the ( n l , rnl) and (n2,rnz) nanotubes. Thus, we expect the motion to be smoother, the smaller is the value of d,. The normal mode for the shear displacement of the two constituents of a twowalled nanotube is a mixture of a translation and a rotation around the P axis. The direction of the normal mode d i s p ~ a ~ e m ewill ~ t sbe d ~ t e r ~ i n by e d the two chiral vectors. In all cases, we expect a downward shift for the shear stress between the adjacent walls of a multiwail nanotube, relative to the shear mode in graphite. Chandrabhas et ai. [236], however, have reported an upshift of the two shear modes to 49 cml and 58 em" from the Ezs, graphite shear mode at 42 cml. The authors attributed the upshift to defects in the nanotube axis. Except for a few nanotubes with open ends, most nanotubes have end caps which prevent mode can be expected to result the sliding motion. In that case a v~brat~onal from the sliding motion. If we could have an ideal coaxial multiwall nanotube with open ends, it would be interesting to study the nanoforces associated with sliding the inner nanotube with respect to the outer nanotube, like the micro~copicmotion of a muscle. The electronic structure of a multiwall nanotube has been calculated for a commensurate doublewall carbon nanotube by a tight binding calculation 1761. In this calculation, the value used for the largest interlayer iiiteraction in graphite associated with the overlap of the wave functions of the two ?r electrons was y1 = 0.35 eV for the two A carbon atoms with a separation (O,O,c). In the tightbinding calculation, the interlayer interaction between two carbon atoms on two different nanotube shells with a separation r is assumed to be 71 expfAT), where A = l / a is an empirical damping factor. The calculated results for the commensurate (5,5)(10,lO) and (9,0)(18,0) nanotubes show an anticrossing* of two energy dispersion curves with the same symmetry of wave functions belonging to the two different nanotubes. As for the wave functions with different symmetries, the energy dispersion relations can cross each other, since the wave functions remain orthogonal to each other even in the presence 'Anticrossing means that two energy dispersion curves repei each other at the crossing point. Anticrossingoccurs as a result of the interaction between the two energy bands.
224
CHAPTER 11. ELASTIC PROPERTIES OF CARBON NANUTUBES
of the interlayer interaction. Although we take account of the interlayer interaction, the calculated result [76] shows that the electronic properties of a twoshell coaxial nanotube look like the sum of the electronic structure of the two independent nanotubes except for the anticrossing phenomenon. Even when this anticrossing appears near the Fermi energy, we do not see the onset of an energy gap at the Fermi energy for metaimetal and meta~semicon~uctor coaxial nanotubes. Thus the calculated results show that the constituent nanotubes of a coaxial nanotube remain either metallic or semiconducting, depending on the chirality of the constituent nanotube. From this result, we can expect that it will be possible to fabricate coaxial conducting wires or capacitors shielded by semiconducting nanotubes which are suggested in the literature [141,237].Since the energy gap of a BN nanotube is the same as that for the bulk BN semiconductor, a large energy gap of about 5 eV is expected for BN nanotubes. Thus when we cover a carbon nanotube by a BN nanotube, the nanotube complex will be more interesting than carboncarbon coaxial nanotubes for device applications, since high insulation by the EN nanotube can be expected. The arc method of synthesis using a carbon rod with the materials for the BN nanotube included in the central portion of the carbon anode yields a coaxial multiwall nanotube in which a severalwall BN nanotube is surrounded by a severalwall carbon nanotube on both the outside and the inside [137]. This observation suggests further possibilities for a variety of other nanotube complexes. If the electronic structure of a mu~tiwallnanotube can be understood in terms of the electronic structure of the constituent singlewall nanotubes, it becomes easy to understand the topological STM and the transport STS experiments in which only the outermost nanotube contributes to the STM image and STS conductance measurements, respectively. In the STM experiment on single crystal graphite, a triangular lattice is observed because of the ABAB stacking of the graphite layers. In graphite, the electrons and holes near the Fermi energy mainly corresponds to B atom wavefunctions, which do not have a neighboring atom directly above or below them on the adjacent graphite layers. Thus when a small voltage is applied, the STM can only see the electrons and the holes at the B sites which form a triangular lattice. i n a multiwall nanotube and even in a singlewall carbon nanotube, a triangular pattern is observed in the STM image, which clearly shows that the A and B atoms are not equivalent to each other [54]in the nanotube plane, although the reason for this is still not clear.
Z 1.4. PROPERTIES OF
MULTI WALL NANOTUBES
225
A more sophisticated calculation was done for ~ u l t i  l a y n~ ~r o t u b e w s ith~n the local density approximation t o establish the optimum interlayer distance between an inner (5,5)armchair nanotube and an outer armchair (10,lO) nanotube. The result of this c a h l a t i o n yielded a 3.39 A interlayer separation [196,238], with an energy stabi~i~ation of 48 mev~carbonatom. The fact that the interlayer separation is somewhat less than the 3.44 A separation expected for turbostratic graphite may be explained by the interlayer correlation between the carbon atom sites both along the nanotube axis and the circumferential directions. A similar calculation for dou~lelayeredhyperfull~reneshas also been carried out, yielding an interlayer spacing of 3.524 A between the two shells of C60@C240,with an energy stabilization of 14 meV/atom [147]. In addition, for two coaxial armchair nanotubes, estimates €or the translationa~and rotationa~ energy barriers of 0.23 meV/atom and 0.52 meV/atom, respectively, were obtained, suggesting significant translational and rotational interlayer mobility for individual shells of ideal nanotubes at room temperature. Detailed band calculations for various interpfanar geometries for a t~o ayer red coaxial armchair nanotube 1196,2381 confirm the tightbinding results [76] mentioned above. In the limit of large diameter, we can expect multiwall carbon nanotubes to have the properties of graphite. In the multilayer structure, the cross section of the hollow core becomes relatively small with increasing numbers of carbon layers, and thus the multiwall structure would be advantageous for obtaining high strength per unit area in the nanotube axis direction. However, when the diameter increases to more than 1020 nm, the multiwa~~ nanotube starts t o exhibit a hexagonal pillar shape, similar to the occurrence of faceting in carbon fibers 191. In the faceting, the curvature of the nanotubes becomes concentrated a t the corners of the pillars as the interlayer correlation becomes established over a large area with a structure that is close to that of graphite. The faceting may occur in order to gain the cohesive energy of graphite through the ABAB stacking. By faceting the layers, the greatest part of the individual layers more quickly approach that of graphite than through the cylindrical growth of multiwall nanotubes. It is important to note that the faceting is not generafly found in pyrolytically generated, multilayer carbon nanotubes [59], which is related t o the growth of multiwall nanotubes in the radial direction by an accretion method.
Appendix: Programs for a (n,m) carbon nanotube
In this Appendix, we show first a simple program for generating parameters of an (n, m) carbon nanotube, which is discussed in Chapter 3. The atomic coordinates for an ( n ,m) carbon nanotube are generated in the unit cell of the nanotube by the second program. The third program gives more coordinates for several unit celIs. The source codes are written in Fortran 77. Any reader can use these codes by citing the book. A1 Parameters for an (n,m) carbon nanotube The first program A1 generates the characteristic vectors such as Ch,T,R and other related parameters. See details of the definitions given in Tables 3.2 and 3.3. We show below an example of the inputoutput on a workstation. When you input n, m values for an ( n ,m) carbon nanotube using a standard input method, which generally means a keyboard, we obtain output for the parameters in a standard output format. Example: Input and output of the program A1
tube% a l . o u t Enter n,m f o r Ch 10,lO Ch = ( 10, 10) d = 10 d,R = 30 L/a = square r o o t
Chiral vector (n,m) ==> d i s gcd(n,m) ==> d,R i s gcd(Zn~m,2m~n) of 300 ==> Length o f Ch 227
228 d,t
T T/a N R M
APPENDIX: PROGRAMS FOR A (n,m) CARBON NANOTUBE = 13.56955AA = ( 1, 1) ==> = I ==> = 20 ==> = ( 1, 0) ==> = 10 ==>
rt = 6.78478AA ==> diameter and radius Translation vector (t_I,t,2) Length of T Number of hexagon in the unit cell Symmetry vector number of T in N R
Here the diameter and the radius are in A unit. The lengths of Ch and T are shown in units of a . Since these values are a square root of an integer in units of a , the output is shown above for convenience.
A2 Coordinates for a (n,m) carbon nanotube
.
The program A2 generates (xi,yi, zi) (i = 1,. . , 2N) coordinates in the unit cell for an ( n ,m ) carbon nanotube. When n , m values are input in the same way as in the example for the A1 program, the program generates two files: Output files for A2: (No Input file) tube.xyz : 2N and coordinates (xi,yi,zi) ( i = 1 , . . . , 2N) en.xyz2 : work file which will be used in the program A3. The file tube.xyz includes the atomic coordinates of carbon atoms in the unit cell for the ( n ,m) nanotube. The other file en.xyz2 is a work file which will be used in the program A3. The file tube.xyz has a format for the xmol program* which can display the structure in its xyz format and can convert the results to many formats consistent with other software. The first line of tube.xyz is the number of carbon atoms in the unit cell. After a blank line in the second line, the atomic symbol C and ( q , y i , z i ) coordinate in A units are listed from the third line for the number of carbon atoms. The file inputoutput is specified by the OPEN statement of Fortran codes. The z axis is taken to be along the nanotube axis. The CC bond distance is taken as 1.42A. If you want to change *xmol is a graphic software package with a Copyright by Research Equipment Inc. and dba Minnesota Supercomputer Center Inc.
A3 COORDINATES FOR SEVERAL UNIT CELLS
229
this value, the parameter in the program shouid be changed.
A3 Coordinates for several unit cells The program A3 reads the en.xyz2 which is generated by the A2 program. When you enter the number of unit cells Nu from the keyboard, the program A3 outputs a fiIe tubel.xya. Thus, before we run the A3 program, we need to run the A2 program. The file tubel.xyz has the same format as tube.xyz but the number of carbon atoms becomes Nu x 2N. Input and Output files for A3: en.xyz2 : (Input) the work file made by the program A2, tubel.xyz : (Output) the coordinates (ti,~ 6 zi) , ( i = 1,.. . , 2 N x
Nu)
If you want a large numbers of carbon atoms (more than 5000), the parameters in the program should be changed.
A4 Source Codes Here we list the source cords. Anybody that uses these source codes or their m o ~ i ~ eversions d is required to cite the book.
A€ Parameters for a (n,m) nanotube C C C C C C C C C
Parameters for a (n,m) nanotube Rade by 10/16/96
R. Saito
Reference: “Physical Pxoperties of Carbon NanotubesSJ Imperial College Press, by R. Saito, G . Dresselhaus, and M.S. Dresselhaus
+eps) if ((nt2nt**2) eq.0) then if(ite9t.e 1) write(*,40) nt format(’ T7; = >, i3) else if(itest.e 1) write(*,41) nt2 format( ’ T7; = square root of), i6) endif
.
40
41
c N 50
c R
nn=2*12/ndr if(itest.eq.il write(*,tiO) nn format(’ N = ’, i4) ichk=O if (nr.eq.0) then n60=1 else n60llr
endif C
itest2=0
231
A4 SOURCE CODES C
67
61 60
do 60 np=abs(n60) ,abs(nbO) do 61 nqabs(ns) ,abs(ns) 52 7 nr*nq  ns*np if(32.eq.1) then jl = m *np  n*nq if(itest2.eq. 1) arite(*,67) n,m,nr,ns,n,nq,jl,j2 format( ’n,m,nr,118,np,nq,jl, ’ ,6i4,2i6P if( jl.gt.0 .and. j1.lt.nn j2ihen ichk=ichk+l nnp(ichk)=np nnq(ichk)=nq endif endif continue continue
C
if(ichk.eq.0) then write(*,*) ’n,m,nr,ns=’,n,m,nr,ns stop ’ not found p,q strange!!’ endif C
itest3=l C
if (ichk.ge .2) then if (itest3.eq.1) then write(*,*) ’n,m,y,?s=’,n:m,nrps write(*,*) ’ichkm ,ichk, ndr= , ndr write(*,66) (nnp(i) ,nnq(i), (m*nnp(i)n*nnq(i)) stop ’ more than 1 pair of p,q strange!!’ endif if(nr.ne.0
,nn,i=l,ichk)
.and. ns.ne.0) then
C
77 C
if(itestl.eq.1) then do 77 i=l,ichk if((m*nnp(i)n*nnq(i)).lt.nn) continue endif
goto 777
write (* ,*> ’n,m,nr,ns=’ ,n:m ,nr,ns write(*,*) ’ichk=’,ichk, ndr=’, ndr write(*,66) i f (ir eq. 0) then igcm=j return else
.
10
.
1‘ 4 J =lr endif got0 10 end
A2 Atomic Coordinates for a ( n ,rn) nanotube in the unit cell C
c Atomic Coordinates i n t h e u n i t c e l l of a (n,m) nanotube C
c Made by 10/31/95
by T. Takeya and R . Saito
C
c Reference: “Physical Properties of Carbon Nanotubes” Imperial College Press, C by R. S a i t o , G. Dresselhaus, and M.S. Dresselhaus C C
c Input: n,m (from keyboard) c Output: tube.xyz (coordinates. See d e t a i l i n t h e above book.) C en.xyz2 ( a work f i l e f o r the program A3) C
implicit real*8 (ah,oz) C
c
acc: CC bond distance.
C
parameter (acc = 1.42d0) parameter (nk=1300) dimension x(nk) ,y(nk) ,z(nk) C
write(*,*)’ Enter n.m f o r Ch=(n,m)’ read(*,*) n,m C
C C
c a l l genll(n,m,np,nq,ndr) write(*,*)’ R = (’, np,
’,’,
nq
, ’1’
233
A4 SOURCE CODES C
c
a: t h e length of t h e u n i t vector sq3 = 1.732....
p i = 3.141592.
..
C
sq3=sqrt(3.OdO) pi=4,OdO*atan ( 1. OdO) a z s q r t (3.OdO) *acc C
c
r;IRI
, c;lC,hl , t ; l T I
C
r=a*sqrt (df l o a t (np*np+nq*nq+np*nq)) c=a*sqrt(dfloat(n*n+m*m+n*m)~ t = s q r t (3 .OdO) *c/dfloat (ndr) w r i t e (* ,*) t=I ,t , df l o a t (n*n+m*m+n*~) write (*, 190)~/2.OdO/pi C c I 9 0 format(' r a d i u s =',f10.4) C C C
nn: t h e number of hexagon i n t h e u n i t c e l l M nnt2*(n**2*m**2+m*n)/ndr
C
c
write(*,*)
'
N =',nn*2
C
C
rs: r a d i u s of t h e tube
C
if(2*nn.gt.nk)
s t o p 'parameter nk is too small'
C
rs=c/(2.OdO*pi) C C
C C C
q l : t h e c h i r a l angle f o r Ch 42: t h e ' c h i r a l ' angle f o r R 93: t h e angle between Ch and R ql=atan( (sq3*df l o a t (m) /df l o a t (2*n+m) ) q2=atan( (sq3*df loat (nq) /df l o a t (2*np+nq)1 q3=qlq2
C C C C
94: a period of an angle f 5 r t h e A atom q5: t h e d i f f e r e n c e of t h e angle between the A and B atoms q4=2.OdO*pi/dfloat (nn) q6~acc*cos((pi/6.OdO)ql)/c*2~OdO*pi
C C C C
hi : h2: Delta z between t h e A and B atoms hlsabs ( t ) /abs (sin(q3) ) hZ=acc*sin( (pi/6.OdO)ql)
C C C C C C C C C C
write(*,*) write (* ,*) write(*, *) write (* ,*)
'ql: =',ql*l80.0dO/pi 'q2 : =' ,q2*180.OdO/pi 'q4: =' ,q4*i80.OdO/pi 'q5 : 3' ,q5*180.OdO/pi
Calculate 2*nn atoms i n t h e u n i t c e l l . The A atom
APPENDIX: PROGRAMS FOR A (n,m) CARBON NANOTUBE
234 ii=O
do 100 i=O,nn1
xi0 yl=O zl=O k=int(df loat ( i) *abs(r) /hl xl=rs*cos(dfloat (i)*q4) yl=rs*sin(dfloat (i)*q4) zl=dfloat ((df loat(i)*abs ( r )dfloat (k)*hl)) *sin(q3) kk2=abs(int (zl/t))+l C
c Check the A atom is in the unit cell 0 < zl < t C
if(z1.gt.t0.02)then zl=zlt*dfloat(kk2) endif if(zl.lt.0.02) then zl=zl+t*dfloat (kk2) endif ii=ii+i x (ii) =xi y(ii)=yl z(ii)=zl C C C
The B atoms
zd=(dfloat (i)*abs(r)dfloat ii=ii+l C
c Check the
(k)*hl)*sin(q3)h2
B atom is in the unit cell 0 < 23 < t
C
if((z3.ge.O.02).and.(z3.le.tO.O2))then
c yes x2 =rs*cos (dfloat (i) *q4+q5)
y2 =rs*sin(dfloat(i)*q4+ 5) 22 =dfloat (dfloat (i)*abs?r) dfloat(k)*hl )*sin(q3)h2 x(ii)=x2 y(ii)=y2 z (ii)=22 else c no
100 C
x2 =rs*cos (dfloat(i) *q4+q5) y2 =rs*sin(dfloat(i)*q4+ 5) 22 =dfloat (dfloat (i)*abs?r)dfloat(k+l)*hl)*sin(q3)h2 kk=abs(int(z2/t))+l if(z2.gt.t0.0l)then z2=z2t*dfloat (kk) endif if(z2.lt.0.01) then z2=z2+t*dfloat(kk) endif x(ii)=x2 y(ii)=y2 z(ii)=z2 endif continue
A4 SOURCE CODES c Out put to the file tube.xyz C
117
open(60, f ile= ’tube.xyz ’1 write (60,*) 2*nn write (60,*) ’ ’ do i=l,nn*2 write(60, ii7)x(i) ,y(i) ,z(i> end do format ( ’C’ ,3f10.5) close(6O)
C
c Out put to the file en.xyz2 C
I18
116
open(60,file=’en,xyz2’) write(60,*)2*~ write(60,ii8)t,acc format (2f25.6) do i=i,nn*2 write(60,116)i,x(i) ,y(i) ,z(i) end do fornat (ii5,3f25.20)
close(60) stop end C
c This subroutine calculates np,nq and ndr from n,m C
subroutine genll(n,m,np,nq,ndr) dimension nnp(iO0) ,nnq(iOO) C
nd=igcm(n,m) if (mod((nm) ,3*nd) .eq.O) then ndr=3*nd else ndr=nd endif C L
12=n*n+m*m+n*m if (12.le.O) stop ’12.le.0’ l=int (sqrt (dfloat (12) )+eps) dt=a*sqrt (dfloat (12)) /3.1415926525 c T
nr (2*m+n)/ndr ns= (2*n+m) /ndr nt2=3*12/ndr/ndr nt=int (sqrt (dfloat (nt2))+eps) c N nn=2*12/ndr c R ichk=O if (nr.eq.0) then n60=i else n60m endif C
itest21
235
236 C
61 60
APPENDIX: PROGRAMS FOR A (n,m) CARBON NANOTUBE do 60 np=abs (n6O) ,abs(1160) do 61 nq=abs(ns) ,abs(ns) j2 = nr*nq  ns*np if(j2.eq.l) then J l = m *np  n*nq if( jl.gt.0 .and. j1.lt.nn ) then ichk=ichk+l nnp(ichk)slp nnq(ichk)slq endif endif continue continue
C
if (ichk.eq.0) then stop ’ not found p,q strange!!’ endif C
itest31 C
if(ichk.ge.2) then if (itest3.eq.1) then stop ’ more than 1 pair of p,q strange!!’ endif if(nr.ne.0 .and. ns.ne.O) then C
77
if (itestl.eq.1) then do 77 i=l,ichk if ((m*nnp(i)n*nnq(i)) continue endif
.lt.nn) goto 777
C
endif endif 777 continue C
2
1
if (itest .eq.1) then np=nnp ( 1) nq=nnq( 1) endif continue return continue stop end
C
c calculate the highest common divisor C
integer function igcm(ii, jj) i=abs(ii) j=abs(jj) if(j.gt.i) then lu=j J 1 i=iw
A4 SOURCE CODES
237
endif i f ( j eq. 0) then igcm=i return endif continue ir=mod(i, j ) i f (ir.eq.0) then igcm=j return else :=J J‘lr endif got0 10 end
.
10
A3 Atomic Coordinates for several unit cells of a (n,rn) nanotube c Atomic Coordinates f o r several unit c e l l s of a (n,m) nanotube C
c Made by 10/31/95
by T. Takeya and R . Saito
C
c Reference: “Physical Properties of Carbon Nanotubes” Imperial College Press, C by R. S a i t o , G. Dresselhaus, and M.S. Dresselhaus
C
C
c Input : n (from keyboard, t h e number of the u n i t c e l l . ) C : en.xyz2 (a work f i l e made by t h e program A2) c Output: tubel.xyz (atomic coordinates) C
i m p l i c i t real*8(ah, 02) parameter (nk=5000, aa=1.42) dimension x(nk), (nk) ,z(nk) dimension iic(nkT.ic(nk.3) ,iZ(nk,3) C
10 C
write(*,*) ’enter the number of the unit c e l l Nu =’ read(*,*)n open(Gl,FILE=’en.~yz2’) read(dl,*)nn read(6l,*)t do 10 i = l , n n read(61,*)j , x ( i ) , y ( i ) , z ( i ) continue c l o s e ( 6 l . statusi’keep ’1 write(*,*) ’Number of t o t a l atoms = ’, n*nn if(n*nn.gt.nk) stop ’change parameter nk t o a l a r g e r value’
C
ii=nn do 20 i = l , n n do 21 jj=O,n1 iii=ii+i+j ’*ii z ( i i i ) = z (ij+df l o a t ( jj + l ) *t
238
21 20
APPENDIX: PROGRAMS FOR A (n,m) CARBON NANOTUBE x (iii)=x (i) y (iii)=y (i) continue cont inue
C
100 700
open(GO,FILE=’tubel .xyz’) arite(60,*)n*nn write (60,*) ’ ’ do 100 i=l,n*nn nrite(60,7OO)x(i) ,y (i) ,z (i) continue format (’Cl, 3f 10.5) close(60)
C
stop end
References
1. T. A. Edison, US Patent 470,925 (1892). (issued March 15, 1892). 2. P. Schutzenberger and L. Schutzenberger, Compt. Rend 111, 774 (1890). 3. C. H. Pelabon, Compt. Rend. 137,706 (1905). 4. R. Bacon, J . Appl. Phys. 31,283290 (1960). 5. C. Herring and J . K. Galt, Phys. Rev. 85,1060 (1952). 6. A. P. Levitt, in Whisker Technology, (WileyInterscience, New York, 1970). 7. A. W. Moore, A. R. Ubbelohde, and D. A. Young, Brit. J . Appl. Phys. 13, 393 (1962). 8. L. C. F. Blackman and A. R. Ubbelohde, Proc. Roy. SOC. A266, 20 (1962). 9. M. S. Dresselhaus, G. Dresselhaus, K. Sugihara, I. L. Spain, and H . A. Goldberg, Graphile Fibers and Filaments (SpringerVerlag, Berlin, 1988), Vol. 5 of Springer Series in Materials Science. 10. T. Koyama, Carbon 10, 757 (1972). 11. M. Endo, T. Koyama, and Y. Hishiyama, Jap. J. Appl. Phys. 15, 20732076 (1976). 12. G . G. Tibbetts, Appl. Phys. Lett. 42, 666 (1983). 13. G. G. Tibbetts, J. Crystal Growth 66,632 (1984). 14. M. Endo. Mecanisme de croissance en phase vapeur de fibres d e carbone (The growth mechanism of vaporgrown carbon fibers). PhD thesis, University of Orleans, Orleans, France, 1975. (in French). 15. M. Endo. PhD thesis, Nagoya University, Japan, 1978. (in Japanese). 16. A. Oberlin, M. Endo, and T.Koyama, Carbon 14,133 (1976). 17. A. Oberlin, M. Endo, and T. Koyama, J . Cryst. Growth 32, 335349 (1976). 18. R. Kubo, 1977. (private communication to M. Endo). 239
240
REFERENCES 19. S. Iijima, Nature (London) 354,56 (1991). 20. H. W. Kroto, J. R. Heath, S. C. O'Brien, R. F. Curl, and R. E. Smalley, Nature (London) 318,162163 (1985). 21. R. E, Smalley, DoD Workshop in W ~ h ~ n g t oDC n , (December 1990). 22. D. R. Huffman, DoD Workshop in Washington, DC (December 1990). 23. M. S. Dresselhaus, DoD Workshop in Washington, DC (December 1990). 24. M, S. Dresselhaus, G . ~resseIhaus,and P. C . ~ k l u n d ,University of Pennsylvania Workshop (August 1991). 25. J . H. Weaver, J. L. Martins, T. Komeda, Y. Chen, T. R. Ohno, G. H. KrolI, N. Troullier, R. E. Haufler, and R, E. Smalley, Phys. Rev. Lett. 66,17411744 (1991). 26. F. P. Bundy. In Solid State Physics under Pressure: Recent Advance with Anvil Devices, edited by S. Minomura, page 1,D. Reidei, Dordrecht, 1985. 27. F. P. Bundy, J. Geophys. Res. 85,6930 (1980). 28. F. P. Bundy, W. A. Bassett, M. S. Weathers, R. J . Hemley, H . K. Mao, and A. F. Goncharov, Carbon 34,141153 (1996). 29. R. J . Lagow, J . J. Kampa, H. C. Wei, S. L. Battle, J . W. Genge, D. A. Laude, C. J. Harper, R. Bau, R. C. Stevens, J. F. Haw, and E. Munson, Science 267,362367 (1995). 30. V. I. Kasatochkin, A. M. Sladkov, Y. P. Kudryavtsev, N . M. Popov, and V. V. Korshak, Dokl. Chem. 177,1031 (1967). 31. V, I. Kasatochkin, V. V. Korshak, Y. P. Kudryavtsev, A. M. Sladkov, and I. E. Sterenberg, Carbon 11, 70 (1973). 32. A. G. Whittaker and P. L. Kintner, Carbon 23,255 (1985). 33. A. G. Whittaker and P. L. Kintner, Science 165,589 (1969). 34. A. G. Whittaker, Science 200,763 (1978). 35, A. G. Whittaker, E. J . Watts, R. S. Lewis, and E. Anders, Science 209, 1512 (1980). 36. A, El Gorsey and G . Donnary, Science 363 (1968). 37. V. I. Kasatochkin, M. E. Kasakov, V. A. Savransky, A. P. Nabatnikov, and N. P. Radimov, Dokl. Akad. Nauk, USSR 201,1104 (1971). 38, R. B. Heimann, J. Kleirnan, and N. M.Slansky, Nature (London) 306, 164 (1983). 39. A. G. Whittaker and G. M. Wolten, Science 178,54 (1972).
REFERENCES
241
40, A. G. Whittaker, G . Donnay, and K. Lonsdale, Carnegie Institution Year Book 69,311 (1971). 41. J . S. Speck, M. Endo, and M. S. Dresselhaus, J . Crystal Growth 94,834 (1989). 42. J . S. Speck, M. S. Dresselhaus, and M. Endo. In Extended Abstracts of the Symposium on Graphite Intercalation Compounds at the Materials Research Society Meeting, Boston, edited by M. Endo, M. S. Dresselhaus, and G. Dresselhaus, page 169, Materials Research Society Press, Pittsburgh, PA, 1988. 43. J . S. Speck, J. Appl. Phys. 67, 495 (1990). 44. M. Endo, CHEMTECH 18,568 (1988). September issue. 45. C. Kittel, in Introduction to Solid State Physics, 6th ed., (John Wiley and Sons, New York, NY, 1986). 46. N. W. Ashcroft and N. D. Mermin, in Solid State Physics, (Holt, Rinehart and Winston, New York, NY, 1976). 47. R. S. Mulliken, in Life of a Scientist, (SpringerVerlag, New York, Berlin, 1989). 48. G. S. Painter and D. E. Ellis, Phys. Rev. B 1,4747 (1970). 49. R. A. Jishi, L. Venkataraman, M. S. Dresselhaus, and G. Dresselhaus, Phys. Rev. B 51,11176 (1995). 50. M . S. Dresselhaus, G. Dresselhaus, and R. Saito, Carbon 33, 883891 (1995). 51. S. J . Tans, M. H. Devoret, H. Dai, A. Thess, R. E. Smalley, L. J. Geerligs, and C. Dekker, Nature (London) 386,474 (1997). 52. C. Journet, W. K. Maser, P. Bernier, A. Loiseau, M. Lamy de la Chapelle, S. Lefrant, P. Deniard, R. Lee, and J . E. Fischer, Nature (London) 388,756 (1997). 53. M. R. Falvo, G. J . Clary, R. M. Taylor 11, V. Chi, F. P. Brooks J r , S Washburn, and R. Superfine, Nature (London) 385 (1997). 54. C. Dekker, S. J . Tans, M . H. Devoret, L. J . Geerlings, R. J . A. Groeneveld, L. C. Venema, J . W. G. Wildoer, A. R. M. Verschueren, A. Bezryadin, A. Thess, H. Dai, and R. A. Smalley. In Proc. of the Int. Winter School on Electronic Properties of Novel Materials: Molecular Nanostructures, edited by H. Kuzmany, J. Fink, M. Mehring, and S. Roth, SpringerVerlag, New York, 1997. Kirchberg, Austria.
242
REFERENCES 55. A. Thess, R. Lee, P. Nikolaev, H. Dai, P. Petit, J . Robert, C. Xu, Y . H. Lee, S. G. Kim, A. G. Rinzler, D. T. Colbert, G. E. Scuseria, D. Tomrinek, J . E. Fischer, and R. E. Smalley, Science 273, 483487 (1996). 56. J . M. Cowley, P. Nikolaev, A. Thess, and R. E. Smalley, Chem. Phys. Lett. 265, 379384 (1997). 57. C. H. Kiang, W. A. Goddard 111, R. Beyers, and D. S. Bethune, Carbon 33, 903 (1995). 58. S. Iijima and T. Ichihashi, Nature (London) 363,603 (1993). 59. M. Endo, K . Takeuchi, K. Kobori, K. Takahashi, H. Kroto, and A. Sarkar, Carbon 33,873 (1995). 60. P. M. Ajayan. In Carbon Nanotubes: Preparation and Properties, edited by T. Ebbesen, page 111, CRC Press, Inc., Boca Raton, Florida, USA, 1997. Chapter 111. 61. P. M. Ajayan. In Fullerenes and Nanotubes, edited by Pierre Delhaks and P. M. Ajayan, page this volume, Gordon and Breach, Paris, France, 1998. Series: World of Carbon, volume 2. 62. S. Iijima. In Fullerenes and Nanotubes, edited by Pierre Delhaks and P. M. Ajayan, Gordon and Breach, Paris, France, 1998. Series: World of Carbon, volume 2. 63. Ph. Lambin and A . A. Lucas, Phys. Rev. B 56,3571 (1997). 64. W. Cochran, F. H. C. Crick, and V. Vand, Acta Cryst. 5, 581 (1952). 65. C. H. Olk and J . P. Heremans, J . Mater. Res. 9, 259262 (1994). 66. K.Sattler, Carbon 33,915 (1995). 67. J . C. Charlier, X. Gonze, and J . P. Michenaud, Europhys. Lett. 28, 403408 (1994). 68. J . C. Charlier. In Fullerenes and Nanotubes, edited by Pierre Delhaks and P. M. Ajayan, Gordon and Breach, Paris, France, 1998. Series: World of Carbon, volume 2. 69. Riichiro Saito, Mitsutaka Fujita, G. Dresselhaus, and M. S. Dresselhaus, Phys. Rev. B 46,18041811 (1992). 70. M. S. Dresselhaus, G. Dresselhaus, R. Saito, and P. C. Eklund, in C ~ O Related Balls and Fibers, chapter 18, pages 387417, edited by J. L. Birman, C. S&benne,and R. F. Wallis (Elsevier Science Publishers, B.V. 1992, New York, 1992). Balkanski Festschrift.
REFERENCES
243
71. J. W. Mintmire, B. I. Dunlap, and C. T. White, Phys. Rev. Lett, 68, 631634 (1992). 72. J . W . Mintmire, D. H. Robertson, and C. T. White, J . Phys. Chem. Solids 54, 1835 (1993). 73. T. Hamada, M. Furuyama, T. Tomioka, and M. Endo, J. Mater. Res. 7,11781188 (1992). ibid., 26122620. 74. R. Saito, M. Fujita, G. Dresselhaus, and M. S. Dresselhaus. In Electrical, Optical and Magnetic Properties of Organic Solid State Materials, MRS Symposia Proceedings, Boston, edited by L. Y. Chiang, A. F. Garito, and D. J . Sandman, page 333, Materials Research Society Press, Pittsburgh, PA, 1992. 75. R. Saito, M. Fujita, G. Dresselhaus, and M. S. Dresselhaus, Appl. Phys. Lett. 60,22042206 (1992). 76. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, J. Appl. Phys. 73, 494 (1993). 77. M. S. Dresselhaus, R. A. Jishi, G. Dresselhaus, D. Inomata, K. Nakao, and Riichiro Saito, Molecular Materials 4,2740 (1994). 78. R. A. Jishi, D. Inomata, K. Nakao, M. S. Dresselhaus, and G. Dresselhaus, J . Phys. SOC.Jpn. 63,22522260 (1994). 79. G . Dresselhaus and M. S. Dresselhaus, Phys. Rev. 140A,401 (1965). 80. G . Dresselhaus, M. S. Dresselhaus, and J . G. Mavroides, Carbon 4, 433 (1966). 81. J. W. Mintmire and C . T. White, Carbon 33, 893 (1995). 82. J. W. G . Wildoer, L. C. Venema, A. G. Rinzler, R. E. Smalley, and C. Dekker, Nature (London) 391,5962 (1998). 83. A. M. Rao, E. Richter, S. Bandow, B. Chase, P. C. Eklund, K. W. Williams, M. Menon, K. R. Subbaswamy, A. Thess, R. E. Smalley, G. Dresselhaus, and M. S. Dresselhaus, Science 275, 187191 (1997). 84. H. Ajiki and T . Ando, J . Phys. SOC. Jpn. 62, 24702480 (1993). Erratum: ibid page 4267. 85. M. L. Elert, C. T . White, and J . W. Mintmire, Mol. Cryst. Liq. Cryst. Sci. Technol., Sect. A 125,329 (1985). 86. C. T. White, D. H. Roberston, and J . W. Mintmire, (1995). unpublished. 87. X. Blase, L. X. Benedict, E. L. Shirley, and S. G. Louie, Phys. Rev.
REFERENCES
244
Lett. 72,1878 (1994). 88. J . C. Charlier, X. Gonze, and J . P. Michenaud, Europhys. Lett. 29, 4348 (1995). 89. J. C. Charlier, X. Gonze, and J. P. Michenaud, Carbon 32, 289299 (1994). 90. S. G. Louie. In Progress in Fullerene Research: International Winter School on Electronic Properiies of Novel Materials, edited by H . Kuzmany, J. Fink, M. Mehring, and S. Roth, page 303, 1994. Kirchberg Winter School, World Scientific Publishing Co., Ltd., Singapore. 91. X. Blase, A. Rubio, S. G . Louie, and M. L. Cohen, Phys. Rev. B 51, 6868 (1995). 92. N. G. Chopra, J . Luyken, K. Cherry, V. H. Crespi, M. L. Coheri, S. G. Louie, and A. Zettl, Science 269,966 (1995). 93. Z. WengSieh, K. Cherrey, N. G. Chopra, X . Blase, Y. Miyamoto, A. Ru
94. 95. 96. 97. 98. 99. 100. 101.
102.
bio, M. L. Cohen, S. G. Louie, A. Zettl, and R. Gronsky, Phys. Rev. B 51,11229 (1995). D. S. Bethune, C. H. Kiang, M. S. de Vries, G . Gorman, R. Savoy, J. Vazquez, and R. Beyers, Nature (London) 363,605 (1993). B. I. Yakobson and R. E. Smalley, American Scientist 85,324 (1997). M. Yudasaka, T. Komatsu, T. Ichihashi, and S. Iijima, Chem. Phys. Lett. 278,102 (1997). P. C. Eklund et al., unpublished (1997). UK Workshop. J . M. Cowley and F. A. Sundell, Ultramicroscopy 68,1 (1997). H. Kataura, A. Kimura, Y. Maniwa, S . Suzuki, H. Shiromaru, T. Wakabayashi, S. Iijima, and Y. Achiba, unpublished (1997). in press. T. W. Ebbesen and P. M. Ajayan, Nature (London) 358,220 (1992). T. W. Ebbesen, H. Hiura, J . Fujita, Y. Ochiai, S. Matsui, and K. Tanigaki, Chem. Phys. Lett. 209,8390 (1993). S. Seraphin, D. Zhou, J . Jiao, J . C. Withers, and R. Loufty, Carbon 31, 685689 (1993).
103. 104. 105. 106.
Y. Saito and M. Inagaki, Jpn. J . Appl. Phys. 32,L954 (1993). T. W. Ebbesen, Annu. Rev. Mater. Sci. 24,235264 (1994). P. M. Ajayan and S. Iijima, Nature (London) 358,23 (1992). V . P. Dravid, X. Lin, Y. Wang, X. K. Wang, A. Yee, J . B. Ketterson, and R. P. H.Chang, Science 259,1601 (1993).
245 107. S . Iijima, Mater. Sci. Eng. B19,172 (1993). 108. R. E. Smalley, Accounts Chem. Res. 25, 98 (1992). 109. Y. Saito, T. Yoshikawa, M. Inagaki, M, Tomita, and T. Hayashi, Chem. Phys. Lett. 204, 277 (1993). 110. M. Endo, K. Takeuchi, S. Igarashi, K. Kobori, M. Shiraishi, and H. W. Kroto, J. Phys. Chem. Solids 54, 18411848 (1993). 111. J . J . Cuomo and J . M. E. Harper, IBM Tech. Disclosure Bulletin 20, 775 (1977). 112. J . A. Floro, S. M. Rossnagel, and R. S. Robinson, J . Vac. Sci. Technol. A l , 1398 (1983). 113. Z. Ya. Kosakovskaya, L. A. Chernozatonskii, and E. A. Fedorov, J E T P Lett. (Pis’ma Zh. Eksp. Teor.) 56, 26 (1992). 114. A. Loiseau, (1998). private communication. 115. D. Laplaee, P. Bernier, W. K. Maser, G. Flamant, T. Guillard, and A. Loiseau, Carbon page xx (1997). 116. T. W. Ebbesen. In Carbon Nanotubes: Preparation and Properiaes, edited by T. Ebbesen, page 139, CRC Press, Inc., Boca Raton, Florida, USA, 1997. Chapter IV. 117. S. C. Tsang, P. J. F, Harris, and M. L. H, Green, Nature (London) 362, 520 (1993). 118. P. M. Ajayan, T. W, Ebbesen, T. Ichihashi, S. Iijima, K. Tanigaki, and H. Hiura, Nature (London) 362,522 (1993). 119. H. Hiura, T. W. Ebbesen, and K. Tanigaki, Adv. Mater. 7,275 (1995). 120. F. Ikazaki, S. Oshima, K. Uchida, Y. Kuriki, H. Hayakawa, M. Yumura, K. Takahashi, and K. Tojima, Carbon 32, 1539 (1994). 121. S. Bandow, (1997). private communjcation. 122. The mass spectra of the CS2 extract show evidence for Coo and CToin the normal ratio C ~ O : C ~1~and N~ much : higher concentrations of unknown molecular species or carbon clusters with masses in the range 107 < M € 361 arnu. 123. For characterization by electron microscopy, the various samples were dispersed ultrasonically in ethanol and a drop of this solution was placed
onto the carbon microgrid. High resolution scanning electron microscopy (HRSEM) and transmission electron microscopy (TEM) measurements were carried out at 5 kV (Nitachi S900) and 120 kV (Philips
246
124. 125. 126.
127. 128. 129. 130. 131. 132. 133. 134. 135. 136. 137. 138. 139. 140. 141. 142.
REFERENCES EM400), respectively. The low acceleration voltage was selected for HRSEM because it enhances the image contrast. E. Dujardin, T. W. Ebbesen, TI. Hiura, and K. Tanigaki, Science 265, 1850 (1994). P. M. Ajayan and S. Iijima, Nature (London) 361,333 (1993). T. W. Ebbesen. In Carbon Nanotubes: Preparation and Properties, edited by T. Ebbesen, page 225, CRC Press, Inc., Boca Raton, Florida, USA, 1997. Chapter VII. C. GuerretPiCcourt, Y. Le Bouar, A. Loiseau, and H . Pascard, Nature (London) 372,159 (1994). A. Loiseau and H. Pascard, Chem. Phys. Lett. 256,246 (1996). S. C. Tsang, Y. K. Chen, P. J. F. Harris, and M. L. H. Green, Nature (London) 372, 159 (1994). J. Y. Yi and J. B ~ r n ~ oJ.~ cChem. , Phys. 96, 8634 (1992). 0. Zhou, R. M . Fleming, D. W. Murphy, C. H . Chen, R. C. Haddon, A. P. Ramirez, and S. H. Glarurn, Science 263, 1744 (1994). H. Hiura and T. W. Ebbesen, (1997). Unpublished. E. G. Gal’pern, I. V . Stankevich, A. L. Chistykov, and L. A. Chernozatonskii, Chem. Phys. Lett. 214, 345 (1993). M . S. Dresselhaus and G . Dresselhaus, Advances in Phys. 30, 139326 (1 981). A. M . Rao, P. C. Eklund, S. Bandow, A. Thess, and R. E. Smatley, Nature (London) 388, 257 (1997). R. S. Lee, H . J . Kim, J. E. Fischer, A. Thess, and R. E, Smalley, Nature (London) 388, 255 (1997). K . Suenaga, C. Colliex, N. Demoncy, A. Loiseau, H. Pascard, and F . Willaime, Science 278,653 (1997). J. Goma and A. Oberlin, Thin Solid Films 65, 221 (1980). M. Guigon, A. Oberlin, and G. Desarmot, Fibre Sci. and Technol. 20, 55 (1984). M. Guigon, A. Oberlin, and G. Desarmot, Fibre Sci. and Technol. 20, 177 (1984). Riichiro Saito, ~ i t s u t a k aFujita, G. ~ r e s s e ~ ~ aand u s ,M.S . D r e s s ~ I ~ a u s , Materials Science and ~ngineeringB19,185191 (1993). M. Endo and H. W. Kroto, J. Phys. Chem. 96,6941 (1992).
REFERENCES
247
143. S. Iijima, T. Ichihashi, and Y. Ando, Nature (London) 358, 776 (1992). 144. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, Chem. Phys. Lett. 195, 537 (1992). 145. R. E. Smalley, Mater. Sci. Eng. B19, 17 (1993). 146. S. Iijima. private communication. 147. Y. Yosida, Fullerene Sci. Tech. 1,55 (1993). 148. M. S. Dresselhaus, G. Dresselhaus, and R. Saito, Phys. Rev. B 45, 6234 (1992). 149. K. Tanaka, M. Okada, K. Okahara, and T. Yarnabe, Chem. Phys. Lett. 191, 469 (1992). 150, L. Langer, L. Stockman, J . P. Heremans, V. Bayot, C . H. Olk, C. Van Haesendonck, Y. Bruynseraede, and J . P. Issi, J . Mat. Res. 9, 927 (1994). 151. J. Heremans, C. H. Olk, and D. T. Morelli, Phys. Rev. B 49, 15122 (1994). 152, X. K. Wang, R. P. H. Chang, A. Patashinski, and J. B. Ketterson, J . Mater. Res. 9, 1578 (1994). 153. J. M. Luttinger, Phys. Rev. 84, 814817 (1951). 154. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, Phys. Rev. B 50, 14698 (1994). 155. D. R. Hofstadter, Phys. Rev. B 14, 22392249 (1976). 156. F. A. Butler and E. Brown, Phys. Rev. 166, 630 (1968). 157. J . W. McClure, Phys. Rev. 104, 666 (1956). r o~ ed., ,~ (John Wihy 158. H. S. M. Coxeter, in ~ ~ ~ r o to~ G ~e oc ~ ~e ~z2nd and Sons, New York, NY, 1969). 259. M. Yoshida and E. Osawa, Bulfetin Chem. SOC.Jpn. 68, 2073 (1995). ibid. p. 2083. 160. H. Ajiki and T. Ando, J . Phys. Soc. Jpn. 65, 505 (1996). 161. B. I. Dunlap, Phys. Rev. B 49, 5643 (1994). 162. B. I. Dunlap, Phys. Rev. B 50, 8143 (1994). 163. M. Tsukada and N. Shima, J. Phys. SOC.Jpn, 56, 2875 (1987). 164. P. A. Lee, A. D. Stone, and H. Fukuyama, Phys. Rev. B 35, 1039 (1987). 165. L. Langer, V. Bayot, J . P. Issi, L. Stockman, C. Van Haesendonck, Y. Bruynseraede, 3. P. Heremans, and C. H. Oik, Extended Abstracts
REFERENCES
248
166. 167. 168. 169. 170,
171. 172.
of the Carbon Conference page 348 (1995). R.Landauer, IBM Journal of Research and Development 1,223 (1957). R. Landauer, Phil. Mag, 21, 863 (1970). T. Nakanishi and T. Ando, J . Phys. SOC.Japan 66 (1997). in press. R. Tamura and M. Tsukada, Phys. Rev. B 55,4991 (1997). scaling law of nanotube conductance. T. Ando, Phys. Rev. B 44, 8017 (1991). S. Ihara and S. Itoh, Carbon 33, 931 (1995). S. Motojima, M. Kawaguchi, I(. Nozaki, and H . Iwanaga, Carton 29, 379 (1991).
173. V. Ivanov, J . B. Nagy, Ph. Lambin, A. A. Lucas, X. B. Zhang, X. F. Zhang, D. Bernaerts, G. Van Tendeloo, S. Amelinckx, and 5 . Van Lunduyt, Chem. Phys. Lett. 223, 329 (1994). 174. J. Liu, H. Dai, J . H. Hefner, D. 2'. Colbert, R, E. Smalley, S. J. Tans, and C. Dekker, Nature (London) 385,780 (1997). 175. Needed et al., (1992). 176. K. Akagi, R. Tamura, M. Tsukada, S. Itoh, and S . Ihara, Phys. Rev. Lett. 74, 2307 (1995). 177. S. Datta, Transport in mesoscopic systems (Cambridge University Press, Cambridge, UK, 1995). 178. B. J. Wees et al., Phys. Rev. Lett. 60, 848 (1988). 179. L. Chico, V. H. Crespi, L. X. Benedict, S. G. Louie, and M. L. Cohen, Phys. Rev. Lett. 76,971974 (1996). 180. D. Thouless, Phys. Rev. Lett. 39, 1167 (1977). 181. N.Kamimura and H. Aoki, in The Physics of Interacting Electrons in e ~ ~ , Press, Oxford, 1989). ~ ~ s o r Sd ~~ s~ ~d (CIarendon 182. M. S. Dresselhaus, M. Endo, and J . P. Issi. In FluorineCarbon
and FiuorideCarbon Materials: Chemistry, Physics and Applications, edited by T. Nakajima, pages 95186, Marcel Dekker, Inc, New York, 1994. Chapter IV. 183. P. A, Lee and T, V. Ramakrishnan, Rev, Mod. Phys. 5 7 , 287 (1985). 184. L. Langer, V. Bayot, E. Grivei, 3. P. Issi, J. P. Heremans, C . H, Olk, L. Stockman, C. Van Haesendonck, and Y. Bruynseraede, Phys. Rev. Lett. 76, 479482 (1996). 1 % . T. W, Ebbesen, H. Hiura, M. E. Bisher, M. M. J. Treacy, J. L. Shreeve
186. 187. 188. 189. 190. 191. 192. 193. 194. 195. 196. 197. 198.
199.
200. 201.
202.
Keyer, and R. C , Haushalter, Advanced Materials 8, 155 (1996). T. W. Odom, J , L. Huang, P. Kim, and C. M . Lieber, Nature (London) 391, 6264 (1998). M, Bockrath, D. H. Cobden, P. L. McEuen, N. G. Chopra, A. Zettl, A. Thess, and R. E. Smalley, Science 275, 19221924 (1997). C. L, Kane and E. J . Mele, Phys. Rev. Lett. 78, 1932 (1997). C. A. Klein. In C h e ~ %and s ~Physics ~ of Carbon, edited by P. L. Walker, Jr., page 217. Marcel Dekker, Inc., New York, 1966. Vol. 2. C. A. Klein, J . Appl. Phys. 33, 3388 (1962). A. A . Bright and L. S. Singer, Carbon 17, 59 (1979). V. Bayot, L. Piraux, J. P. Michenaud, and J . P. Issi, Phys. Rev. B 40, 3514 (1989). R. A. Jishi, L. Venkataraman, M. S. Dresselhaus, and G. Dresselhaus, Chem. Phys. Lett. 209, 7782 (1993). T. Aizawa, R. Souda, S. Otani, Y. Ishizawa, and C. Oshima, Phys. Rev. B 42, 11469 (1990). C. Oshirna, T, Aizawa, R. Souda, Y. Ishizawa, and Y. Sumiyoshi, Solid State Cornmun. 65, 1601 (1988). J. C. Charlier. Carbon Nanolfibes and Fullerenes. PhD thesis, Catholic University of Louvain, Belgium, 1994. Department of Physics. M. Tinkham, Group Theory and Quantum Mechanics (McGrawHill, New York, N, Y., 1964). M. S. Dresselhaus, G. Dresselhaus, and P. C. Eklund, Science of Fullerenes and Carbon Nanotubes (Academic Press, New York, NY, 1996). J . M . Holden, Ping Zhou, XiangXin Bi, P. C. Eklund, Shunji Bandow, R. A. Jishi, K. Das Chowdhury~G. ~ r ~ s s e l h a uand s , M. S. Dresselhaus, Chem. Phys. Lett. 220, 186 (1994). T. Guo, C.M. Jin, and R. E. Smalley, Chem. Phys. Lett. 243, 4954 (1995). M, S. Dresselhaus and G. Dresselhaus, Light Scattering in Solids I11 51, 3 (1982). edited by M. Cardona and G. Guntherodt, SpringerVerlag Berlin, Topics in Applied Physics. A. Kasuya, Y. Sasaki, Y. Saito, K. Tohji, and Y. Nishina, Phys. Rev. Lett. 78, 4434 (1997). Raman experiment in carbon nanotubes.
250
REFERENCES
203. M. S. Dresselhaus, G. Dresselhaus, and P. C. Eklund, J . Raman Spect. 27, 351371 (1995). 204. D. S. Knight and W. B. White, J . Mater. Res. 4, 385 (1989). 205. S. Guha, J . MenCndez, J . B. Page, and G. B. Adams, Phys. Rev. B 53, 13106 (1996). 206. G. W. Chantry, in The Raman Eflect, vol. 1 ed., (Dekker, New York, NY, 1971). 207. D. W. Snoke, M. Cardona, S. Sanguinetti, and G. Benedek, Phys. Rev. B 53, 12641 (1996). 208. R. Saito, T. Takeya, T . Kimura, G. Dresselhaus, and M. S. Dresselhaus, Phys. Rev. B (1998). 209. D. H. Robertson, D. W. Brenner, and J . W. Mintmire, Phys. Rev. B 45, 12592 (1992). 210. P. C. Eklund, J . M. Holden, and R. A. Jishi, Carbon 33, 959 (1995). 211. F. Tuinstra and J . L. Koenig, J . Chem. Phys. 53, 1126 (1970). 212. T. C. Chieu, M. S. Dresselhaus, and M. Endo, Phys. Rev. B 26,5867 (1982). 213. P. Lespade, R. AlJishi, and M. S. Dresselhaus, Carbon 20,427 (1982). 214. M. J . Matthews, X. X. Bi, M. S. Dresselhaus, M. Endo, and T. Takahashi, Appl. Phys. Lett. 6 8 , 10781080 (1996). 215. M. S. Dresselhaus and R. Kalish, Ion Implantation in Diamond, Graphite and Related Materials (SpringerVerlag; Springer Series in Materials Science, Berlin, 1992). Volume 22. 216. R. AlJishi and G. Dresselhaus, Phys. Rev. B 26, 4514 (1982). 217. K. Yoshizawa, K. Okahara, T. Sato, K. Tanaka, and T . Yamabie, Carbon 32,1517 (1994). 218. S. Krichene, J . P. Buisson, and S. Lefrant, Synth. Metals 17, 589594 (1986). 219. B. I. Yakobson, C. J . Brabec, and J . Bernholc, Phys. Rev. Lett. 76, 2511 (1996). 220. R. S. Ruoff and D. C. Lorents, Carbon 33, 925 (1995). 221. M. S. Dresselhaus, G. Dresselhaus, P. C. Eklund, and R. Saito, Physics World lO(12) (December 1997). 222. J. Bernholc. Quantum molecular dynamics simulations of microtube bending (unpublished).
REFERENCES
251
223. R. E. Peierls, in ~ ~ f f Theory n t ~of ~Solzds, (Oxford Univeristy Press, London, 1955). 224. X. F. Zhang, X. B. Zhang, G. Van Tendeloo, S. Amelinckx, M. Op de Beeck, and J. Van Landuyt, J. Cryst. Growth 130, 368382 (1993). 225, M. Liu and J. M. Cowley, Ultramicroscopy 53,333 (1994). 226. B. T. Kelly, in Physics of Graphite, (Applied Science (London), 1981). 227. G . Overney, W. Zhong, and D. TomAnek, Z. Phys. D 27,93 (1993). 228. J. Bernholc, J . Y, Yi, Q . M. Zhang, C. J . Brabec, E. B. Anderson, B. N. Davidson, and S. A Kajihara, Zeitschrift fur Physik D: Atoms, Molecules and Clusters 26, 74 (1993). 229. M. M. J . Treacy, T. W. Ebbesen, and J. M. Gibson, Nature (London) 381,678 (1996). 230. K. Harigaya and M. F’ujita, Phys. Rev. B 47, 16563 (1993). 231. B. Friedman, Phys. Rev. B 45, 1454 (1992). 232. K . Harigaya, Phys. Rev. B 45, 13676 (1992). 233. K. Harigaya, Synthetic Metals 56, 32023207 (1993). 234. W, P. Su, J . R. Schrieffer, and A. J. Heeger, Phys. Rev. Lett. 42, 1698 (1979). see also Phys. Rev. B 22,2099 (1980). 235. N. A. Viet, H. Ajiki, and T. Ando, J . Phys. SOC.Jpn. 63,3036 (1994). 236, N. Chandrabhas, A. K. Sood, D. Sundararaman, S. Raju, V. S. Raghunathan, G. V . N. Rao, V. S, Satry, T. S . Rad~akrishnan,Y. Hariharan, A. Bharathi, and C. S, Sundar, PRAMANAJournal of Phys. 42, 375385 (1994). 237. M. S. Dresselhaus, G. Dresselhaus, and Riichiro Saito, Materials Science and Engineering B19,122128 (1993). 238. J. C. Charlier and J . P. Michenaud, Phys. Rev. Lett. 70, 18581861 (1993).
Index
1s Core Orbitals ....................
........................... ............................. al a2 ............................. Sij
9 25 caxis crystallite sizes L , ...........89 CN group ........................ 184 D, group ......................... 184 D, point group .................... 48 d R ................................. 39 dt ................................. 38 E2, optic mode ...................188 K point ........................... 60 k . p perturbation theory ..........106 k2 dependence .................... 170 L .................................. 38 Mpoint mode .................... 202 N ................................. 40 Smatrix ......................... 145 sp hybridization .................... 5 sp2 hybridization ...................7 sp3 hybridization ...................8 sp" hybridization ................... 5 THT............................... 89 VH configurations ................196 VV configuration ................. 196 rvib .............................. 185 T bands of 2D graphite H j j i .......................... 26 Sjjr ........................... 27 energy dispersion relations .... 27 T bands ........................... 26 T bond ............................. 7 11, .................................. 41 u bands of 2D graphite ............ 29 H.j ........................... 29 acc
..............................
u bond
bl b2 ..............................
K I Kz ............................
R .................................
T ................................. Ch ................................
29 7 38 47 47 41 39 37
2D graphite acoustic modes .............. 170 Brillouin zone ................. 25 force constant parameters ....169 graphite ...................... 25 Landau level ................. 106 optical modes 170 phonon dispersion relations . . 166 reciprocal lattice unit vectors . 25 unit cell ...................... 25 unit vectors ...................25
................
A AB effect ......................... 110 ABAB stacking., .................. 87 abundance of nanotubes .......... 210 acetylene ........................... 7 additive property ................. 148 AharonovBohm effect ............108 amorphous carbon ................. 12 amorphous graphite ................12 Anderson localization ............. 147 angle of rotation around the nanotube axis 11, ......... 41
253
254 antibonding r* bands ..............24 arc method ........................ 77 areal moment of inertia. ..........211 armchair nanotube .................36 atomic s i t e s . . .................... 185 axis of cone ....................... 121
ballistic transport ................ 139 bamboo structure ..................81 band JahnTeller effect ........... 216 121 bending angle .................... 81 bending ........................... 80 benzene gas ....................... bias window ...................... 157 156 bistability ........................ Bloch's theorem ...................17 224 BN nanotube ..................... bond alternation ..................213 bond polarization theory ..........192 167 bondbending ..................... bondstretching ...................167 bonding x bands ...................24 breathing A1, mode .......... 172,190 Bright model ..................... 160 broad Raman peaks around the 1347 cm' .......... 202 bulk modulus ...................... 15
C Cz absorption process ..............89 cantilever beam ...................211 81 capping ............................ 79 carbide ............................ carbon arc synthesis ............... 73 carbon fiber with high THT....... 147 carbon fibers ....................14,15 carbon nanotube
beam rigidity ................211 Brillouin Zone ................45 circumferential length .........38 curvature., ...................70 density of states .............. 66 38 diameter ...................... dynamical matrix ............ 173 electronic structure in a magnetic field ...........108 electronic structure ........... 59 energy gap .................... 66 growth rate ...................78 oxidation., ...................84 parameters ...................46 Peierls instability ............219 phonon dispersion relations .. 171 quantum transport .......... 152 reciprocal lattice vectors ...... 45 157 resistivity .................... solid state properties .......... 66 strain energy ................210 35 structure ..................... the number of hexagons N .... 40 45 unit cell ...................... carbon whisker ...................2,82 carbonization temperature .........87 carbyne ............................ 13 catalytic chemical vapor deposition . .2 CGS units ......................... 95 CH, ............................... 22 channels .......................... 142 chemical potentials ...............142 39 chiral angle B ...................... 36 chiral nanotube .................... chiral vector C h ...................37 35 chirality ........................... classic elastic theories .............208 classical conductance ............. 139 classical transport ................ 144 classification ....................... 35
INDEX coaxial nanotubes ................222 132 cobalt catalyst .................... 138 coherence ......................... coiled carbon nanotubes ..........130 electronic structure ..........134 222 commensurate .................... commensurate doublewall carbon nanotube ........223 complete elliptical integrals .......215 conductance G[O].................137 conductance regimes . . . . . . . . . . . . . .141 conductance ...................... 127 137 conductivity ...................... 5 core electrons ....................... core orbitals ........................ 9 Coulomb charging effect .......... 155 crystallite size along the caxis L, .................89 current operator ..................127 CVD ............................... 2 cyclotron frequency wc .............95 cyclotron radius T , ................95
de Broglie wavelength XB .........138 desorption temperature hydrogen ..................... 88 88 oxygen ........................ diamagnetism for graphite ........ 106 11 diamond ........................... diffusion constant D ..............151 diffusive motion ..................139 121 dihedral angle .................... dimensionless inverse magnetic length L/2irC ...........112 disorder in carbon fibers ..........202 distorted columnar structures ......89 dynamical matrix D ( k ) ........... 165
255
eccentricity ....................... edge states .......................
123 126 EELS ............................. 11 effective mass ..................... 110 Einstein relation ..................151 elastic modulus Cxl ...............210 elastic scattering ..................138 elastic thin film. ..................210 electron energy loss spectra ........ 11 electronelectron interaction ...... 221 electronelectron scattering ....... 138 electronphonon coupling constant ................ 213 electronic polarization tensor ..... 192 electronic properties of a twoshell coaxial nanotube ........224 encapsulated metal cluster ......... 79 energy dispersion armchair and zigzag nanotubes ............... 61 energy stabilization ...............225 enhanced backward scattering .... 152 ensemble average ................. 150 envelope function .................200 equation of motion ............... 163 Euler theorem., ..................132
F faceting .......................... 225 138 Fermi sphere ..................... Fermi wavelength XF ............. 138 finite size effect ...................202 flux quantum ..................... 100 focusedion beaminduced deposition .............. 154 force constant model .............. 163 correction of force constant . . 178
256 force constant tensor ......... .163.167 Fourier transform .................164 free electron in a magnetic field .... 95
G Gaussian broadening ..............124 132 genus ............................. 186 gerade ............................ graphitization temperature .........87 growth mechanism .................89
irreducible representation ......... 184 J.
K
JahnTeller effect .................216 joint density of states .............191 115,123 junction ...................... shape of a junction ..........120 Keating potential .................211 Kekule structure ..................213
L H heat treatment temperature THT. .202 helical pitch ...................... 133 helically coiled nanotube ..........131 helixshaped structure ............132 heptagonal defect ..............81. 116 high strength per unit area ....... 225 highly oriented pyrolytic graphite ... 2 hollow cylindrical cantilever .......213 HOPG .............................. 2 hybridization ....................... 5
...
Iijima ............................... 4 in zero magnetic field ............. 111 inphase motion .................. 199 inplane bond alternation .........217 inplane crystallite sizes La ........ 89 incommensurate coaxial nanotubes ..............222 infraredactive modes. ............183 interband coupling ................107 intercalated graphite with fluorine ............147 interlayer interaction .............207 inversion center ................... 186
Landau energy bands twodimensional graphite .... 104 carbon nanotube .............111 Landau gauge ..................... 95 97 Landau radius ..................... Landau degeneracy ................ 97 Landauer formula .................144 laser vaporization method ..........74 layerbylayer removal ..............84 length of cone axis ................123 linear k dispersion ................107 local density approximation ........71 localization length L , ............. 147 localization phenomenon ..........147 longitudinal acoustic mode ........177 Lorentz force ...................... 95
magneticinduced distortion .......221 McClure .......................... 106 mean free path L , ............... 138 mesophase pitch fibers ............. 15 mesoscopic systems ...........127,138 metalmetal coaxial nanotubes ....224 metalmetal junction ............. 124
INDEX
257
metalsemiconductor coaxial nanotubes .............. 224 metalsemiconductor junction . . . . .124 8 methane ............................ MKS (SI) units ................... 9 5 molecular polarizabilities . . . . . . . . .193 momentum relaxation length L , . .138 momentum relaxation time t , .... 139 Mott localization .................147 multiwall nanotubes .........209. 221
N nanotube junctions ............... 116 negative curvature ................116 negative magnetoresistance . . . . . . .151 Landau level formation . . 160.151 . Ni/Co catalyst . . . . . . . . . . . . . . . . . . 187 nonsymmorphic translational group .................... 52 nonzonecenter phonon mode .....202 192 normal mode ..................... normalized electronphonon interaction ..............216
0 open ends ......................... 89 outofphase motion ..............199 outofplane deformation dotfill 218 overlap integral matrix ...... . . . .19 oxidation ................... .... 84
PAN (polyacrylonitrile) ..... ... .... 15 PAN fibers ................. . .14.2 parameters of 2D graphite tight binding method . . . . . . 32
Pauli exclusion principle .......... 138 Peierls distortion ..............216. 70 Peierls instability .................213 pentagon ......................... 187 PES ............................... 10 phasecoherent motion ............151 phase diagram of carbon ........12. 13 phase relaxation time t , ..........139 phaserelaxation length L , ........138 phonon density of states ...... 171.202 phonon mode ..................... 163 phonon occupation number ....... 192 photoelectron spectroscopy .........10 a bond ......................... 7,207 pitch fiber ......................... 14 polarizability parameters ......... 194 192 polarization ..................... polyacetylene (CH), (see alse transpolyacetylene) 7.22.2 13 normalized energy gap .......215 2 polyacrylonitrile .................... power law for the A1, mode ...... 198 projection operator ............... 184
Q quantized conductance Go ........ 143 quantized current .................143 quantized resistance Ro ...........143 quantum confinement ..............95
R radial ............................ 167 Raman experiment ...............187 Raman mode of carbon nanotube atomic displacements ........200 higher frequency modes ...... 198 lower frequency modes ....... 196 medium frequency modes .... 201
Raman polarizability parameters . . 195 Raman spectra angular dependence ..........205 polarization dependence ..... 197 Ramanactive modes ..............183 random phase .................... 150 rareearth metals ..................79 Rayleigh scattering ...............190 regular triangle ...................120 137 resistance., ....................... resistance of a mesoscopic wire R, 144 137 resistivity., ...................... 127 resolvent ......................... resonance tunneling ...............156 resonant Raman effect ............191 Rh/Pd catalyst ...................187 rope .............................. 187 rotation angle II, ...................43 rotation around the z axis .... 203,223
STM image ....................... 224 strain energy per carbon atom .... 210 strongly localized regime ..........147 STS experiments .................224 SuSchriefferHeeger (SSH) model 213 199 sublattices ........................ 133 superlattice ....................... symmetry assignment .............205 symmetry vector R ................41 symmetrylowering effects .........202
T (10. 10) armchair nanotube ........187 thermal diffusion length L T . , .....151 thermal vibration .................212 Thomas A . Edison .................. 1 tight binding approximation in a static magnetic field ...... 98 tight binding method .............. 17 .......................... 19 Sjj!.......................... 19 tilt and twist boundaries ...........89 timereversed processes A: .......151 toroidal carbon nanotube .........133 130 torus c 3 6 0 ........................ 15 tows ............................... transpolyacetylene irbands ...................... 22 ' F I J J I ......................... 23 S J J I.......................... 24 Bloch orbitals ................. 22 Brillouin zone .................22 energy dispersion relations .... 24 reciprocal lattice vector. ...... 22 unit vector .................... 22 transfer integral matrix ............ 19 139 transit time t t .................... transition metals ...................79 translation r ....................... 43
njjl
sample length L ..................139 sample orientation dependence . . . .203 scaled force constant ..............181 secondrank tensor ................168 secular equation ...............165,20 186 selection rules .................... 134 semimetal ....................... semitoroidal structure. ...........130 shear modes between two graphite layers ..........222 207 abonding ........................ sliding motion., .................. 223 sound velocity .................... 178 sp2 hybridization ...................7 sp3 hybridization ...................8 space group symmetry operation R = ( $ 1 ~ ) ................43 spinPeierls interaction ...........221
INDEX
259
translation in the direction of T r . 41 translational vector T .............37 transmission probability .......... 144 transport experiments ............ 159 transverse acoust>icmode . . . . . . . . .177 tube opening ...................... 85 tubule axis length ................123 tunneling conductance ............123 turbostratic graphite., .............89 twisted helical carbon nanotube ...132 twisting motion .............. .169,178 twoband semimetal model ........160 twodimensional cosine band in a magnetic field .........100 twodimensional graphite (see 2Dgrphite) twodimensional van Hove singularities .............125 twopoint resistance ..............155
ungerade ......................... 186 unitary matrix .................... 168 universal conductance fluctuations (UCF)127.148.161 valence electrons .................... 5 vanHove singularities ............ 191 vapor grown carbon fiber . . . . . .2,14.79 vapor growth method . . . . . . . . . . . . . .80 vaporization temperature ....... 77. 88 vector potential ................... 9 5 voltage drop. .................127. 144
w wavy ribbons ...................... 89 weakly localized regime ........... 147 wire frame model .................123 wrinkled layers .................... 89
X.Y.z XPS ................................ 9 Young’s modulus Y ...............211 zerogap semiconductor ............64 zigzag nanotube ...................36 zone folding phonon mode ............163, 172 zonecenter vibrations ............ 183 zonefolding Energy dispersion .............59